Hindawi Publishing Corporation
Advances in Condensed Matter Physics
Volume 2010,Article ID681070,40 pages
doi:10.1155/2010/681070
Review Article
Competition of Superconductivity and Charge Density Waves in
Cuprates:Recent Evidence and Interpretation
A.M.Gabovich,
1
A.I.Voitenko,
1
T.Ekino,
2
Mai Suan Li,
3
H.Szymczak,
3
and M.Pe¸kała
4
1
Institute of Physics,National Academy of Sciences of Ukraine,46 Nauka Avenue,Kyiv 03680,Ukraine
2
Graduate School of Integrated Arts and Sciences,Hiroshima University,HigashiHiroshima 7398521,Japan
3
Institute of Physics,Al.Lotnik
´
ow 32/46,02668 Warsaw,Poland
4
Department of Chemistry,University of Warsaw,Al.
˙
Zwirki i Wigury 101,02089 Warsaw,Poland
Correspondence should be addressed to A.M.Gabovich,alexander.gabovich@gmail.com
Received 2 June 2009;Accepted 1 September 2009
Academic Editor:Sasha Alexandrov
Copyright © 2010 A.M.Gabovich et al.This is an open access article distributed under the Creative Commons Attribution
License,which permits unrestricted use,distribution,and reproduction in any medium,provided the original work is properly
cited.
Explicit and implicit experimental evidence for charge density wave (CDW) presence in highT
c
superconducting oxides is
analyzed.The theory of CDWsuperconductors is presented.It is shown that the observed pseudogaps and diphump structures
in tunnel and photoemission spectra are manifestations of the same CDW gapping of the quasiparticle density of states.
Huge pseudogaps are transformed into modest diphump structures at low temperatures,T,when the electron spectrum
superconducting gapping dominates.Heat capacity jumps at the superconducting critical temperature and the paramagnetic
limit are calculated for CDW superconductors.For a certain range of parameters,the CDW state in a dwave superconductor
becomes reentrant with T,the main control quantity being a portion of dielectrcally gapped Fermi surface.It is shown that in
the weakcoupling approximation,the ratio between the superconducting gap at zero temperature Δ(T
=
0) and T
c
has the
BardeenCooperSchrieﬀer value for swave Cooper pairing and exceeds the corresponding value for dwave pairing of CDW
superconductors.Thus,large experimentally found values 2Δ(T
=
0)/T
c
≈
5
÷
8 are easily reproduced with reasonable input
parameter values of the model.The conclusion is made that CDWs play a signiﬁcant role in cuprate superconductivity.
1.Introduction
Ever since the earliest manifestations of highT
c
supercon
ductivity were found in 1986 [1],the whole theoretical power
[2–22] has been applied to explain and describe various
normal and superconducting properties of various oxide
families with critical temperatures,T
c
,ranging up to 138 Kto
date [23–27].Unfortunately,even conceptual understanding
of the mechanisms and character of superconductivity in
cuprates is still lacking.Strictly speaking,there is a number
of competing paradigms,every of them pretending to be
“the theory of superconductivity” (see,e.g.,[2]) but not
recognized as such by other respected experts in the ﬁeld.
After the discovery of highT
c
oxides,experimentalists
found several other superconducting families with T
c
higher
than 23.2 K reached by the precuprate recordholder,Nb
3
Ge
[28,29].For instance,one may refer to fullerides [30,31],
doped bismuthates [32–34],hafnium nitrides [35,36],and
magnesium diborides [37–40].One should also mention
more controversial cases of superconducting oxides H
x
WO
3
with T
c
≈
120K [41] and Sr
0.9
La
0.1
PbO
3
−
δ
with T
c
≈
65K [42].Finally,an unexpected and counterintuitive
discovery of the ironbased oxypnictide [43,44] or oxygen
free pnictide [45] layered superconductors with T
c
over 50K
has been made recently (see also reviews [46–49]).
Presumably,the latter materials with FeAs layers have
been overlooked as possible candidates for highT
c
super
conductors,since Fe ions in solids usually possess magnetic
moments,which promote magnetic ordering,the latter
being detrimental to superconductivity,especially the spin
singlet one [50–55].Strictly speaking,such an omission
is of no surprise because superconductivity in oxides is
rather gentle,sensible to impurities,including the excess or
deﬁciency of oxygen [56] in these nonstoichiometric [57,58]
2 Advances in Condensed Matter Physics
compounds.Recent discovery [59] of previously unnoticed
highT
c
superconductivity in parent compounds T
R
2
CuO
4
(R
=
Pr,Nd,Sm,Eu,Gd) is very symptomatic in this
regard,since an accurate removal of apical oxygen from
thin ﬁlms raised T
c
from exact zero (those compositions
were earlier considered by theoreticians as typical correlated
MottHubbard insulators) to 32.5Kfor Nd
2
CuO
4
.As for the
ferroarsenide family,one of its members,EuFe
2
(As
0.7
P
0.3
)
2
,
reveals a true superconducting transition at 26K,followed
by the ferromagnetic ordering of Eu
2+
magnetic moments
below 20K,coexisting with superconductivity [60],which
is quite unusual in view of the antagonism indicated above
between two kinds of cooperative phenomena.
What is more,none of the mentioned superconductors
except Ba
1
−
x
K
x
BiO
3
[33] were discovered due to theoretical
predictions.Hence,one may consider the theoretical discov
ery of Ba
1
−
x
K
x
BiO
3
as an accidental case,since,according to
the wellknown chemist Cava:“one of the joys of solid state
chemistry is its unpredictability” [61].The same opinion
was expressed by the other successive chemist Hosono:
“understanding the mechanism with respect to predicting
the critical temperature of a material is far from complete
at the present stage even for brilliant physicists.Such a
situation provides a large opportunity including a good luck
for material scientists who continue the exploration for a
new material,not limited to superconductors,and a new
functionality based on their own view points” [48].That
is why Pickett recently made a sad remark that “the next
breakthrough in superconductivity will not be the result of
surveying the history of past breakthroughs” [62].It means
that microscopic theories of superconductivity are incapable
of describing speciﬁc materials precisely,although together
they give an adequate overall picture.In this connection,
the failure of the most sophisticated approaches to make
any prediction of true or,at least “bare” T
c
,(provided
that the corresponding T
c
value is not known a priori)
despite hundreds of existing superconductors with varying
fascinating properties,forced Phillips [63] to reject all appar
ently ﬁrstprinciple continuum theories in favor of his own
percolative ﬁlamentary theory of superconductivity [64–67]
(see also the random attractive Hubbard model studies of
superconductivity [68,69] and the analysis of competition
between superconductivity and charge density waves studied
in the framework of similar scenarios [70–72]).We totally
agree with such considerations in the sense of the important
role of disorder in superconductors with high T
c
on the
verge of crystal lattice instability [73–83].Nevertheless,it
is questionable whether a simple oneparameter “master
function” of [63,67] would be able to make quantitative and
practically precise predictions of T
c
.As for the qualitative
correctness of the dependence T
c
versus weighted number
R
of Pauling resonating valence bonds [63,67,84],it
can be considered at least as a useful guideline in the
superconductivity ocean.The phenomenological character
of the master function (chemical trend diagram) T
c
(
R
) is
an advantage rather than a shortcoming of this approach,as
often happens in the physics of superconductors (see,e.g.,
more or less successful criteria of superconductivity with
diﬀerent extent of phenomenology [85–98]).
On the other hand,attempts to build sophisticated
microscopic theories of the bosonmediated Bardeen
CooperSchrieﬀer (BCS) attraction,treating the Coulomb
repulsion as a single Coulomb pseudopotential constant μ
∗
,
are incapable of predicting actual critical superconducting
properties [63,91,99–101].The same can be said [67]
about HubbardHamiltonian models with extremely strong
repulsive Coulomb energy parameter U,which is formally
based on the opposite ideology (see,e.g.,[102,103]).As an
example of the theories described above,one can indicate
work [104],where the strongcoupling Eliashberg equations
for the electronphonon mechanism of superconductivity
[105,106] were solved numerically taking into account
even vertex corrections and treating the dispersive Coulomb
interaction not on equal footing,but as a simple constant μ
∗
.
In this connection,it seems that the prediction of [104] that
the maximal T
c
for new ironbased superconductors is close
to 90K is unjustiﬁed.Of course,the same is true for other
studies of such a kind.
It is remarkable that,for hole and electrondoped
cuprates,there is still no clarity concerning the speciﬁc
mechanisms of superconductivity [17,107–115] and the
order parameter symmetry [109,116–130],contrary to the
“oﬃcial” viewpoint [131–133]) and even the very character
of the phenomenon (in particular,there have been furious
debates concerning the Cooper pairing versus boson conden
sation dilemma in cuprates [8,134,135]).The same seems
to be true for other old and new “exotic” superconductors
[46,107,108,136–153],their exoticism being in essence a
degree of our ignorance.
It would be of beneﬁt to consider all indicated problems
in detail for all classes of superconductors and show possible
solutions.Unfortunately,it cannot be done even in the scope
of huge treatises (see,e.g.,[154–157]).The objective of this
review is much more modest.Speciﬁcally,it deals mostly
with highT
c
cuprate materials,other superconductors being
mentioned only for comparison.Moreover,in the present
state of aﬀairs,it would be too presumptuous to pretend to
cover all aspects of the oxide superconductivity.Hence,we
will restrict ourselves to the analysis of lattice instabilities
and concomitant charge density waves (CDWs) in high
T
c
oxides.Their interplay with superconductivity is one of
the fascinating and fundamentally important phenomena
observed in cuprates and discussed by us earlier [158–160].
Nevertheless,in this rapidly developing branch of the solid
state physics,many new theories and experimental data on
various CDW superconductors appeared during last years.
They are waiting for both unbiased and thorough analysis.
This article discusses this new information,referring the
reader to our previous reviews for more general and
established issues,as well as some cumbersome technical
details.
The outline of this review is as follows.In Section 2,
for the sake of completeness,we brieﬂy consider possible
mechanisms of superconductivity in cuprates,the prob
lem of the relationship between BCS pairing and Bose
Einstein condensation (BEC),and the multigapness of
the superconducting order parameter.Section 3 is devoted
to the experimental evidence for CDWs,the socalled
Advances in Condensed Matter Physics 3
pseudogaps,diphump structures,and manifestations of
intrinsic inhomogeneity in cuprate materials.The original
theory of CDW superconductors and the interpretation of
CDWrelated phenomena in highT
c
oxides are presented
in Section 4.At the end of Section 4,some recent data
on coexistence between superconductivity and spin density
waves (SDWs)—a close analogue of CDWs—are covered.
This topic became hot once more after the discovery of
ferropnictides [43–48,161].Short conclusions are made in
Section 5.
2.Considerations on Peculiarities and
Mechanisms of Superconductivity in Oxides
When BaPb
1
−
x
Bi
x
O
3
−
δ
(BPB) was shown [162] to be a
superconductor with a huge (at that time!) T
c
≈
13K
for x
≈
0.25,a rather low concomitant concentration of
current carriers n
≈
1.5
÷
4.5
×
10
21
cm
−
3
,and poor electric
conductivity [56] (the phase diagram of BPB is extremely
complex,with a number of partial metalinsulator structural
transitions [56,163–167]),it looked like an exception.
Now,it is fully recognized that oxides with highest T
c
are
bad metals fromthe viewpoint of normal state conductivity
[168].In particular,the mean free path of current carriers
is of the order of the crystal lattice constant,so that the
IoﬀeRegel criterion of the metalinsulator transition [169]
is violated.Moreover,there exists an oxide superconductor
SrTiO
3
−
δ
with a tiny maximal T
c
≈
0.5K,attained by
doping,but an extremely small n < 10
20
cm
−
3
[170].
Note that the undoped semiconducting SrTiO
3
−
δ
is so close
to the metalinsulator border that it may be transformed
into a metal by the electrostaticﬁeld eﬀect [171] (this tech
nique has been successfully applied to other oxides [172]).
Moreover,a twodimensional metallic layer has been dis
covered [173] at the interface between two insulating oxides
LaAlO
3
−
δ
and SrTiO
3
−
δ
,which was later found to be
superconducting with T
c
≈
0.2K[174,175].The appearance
of superconductivity at nonmetallic charge carrier densi
ties in oxides of diﬀerent classes comprises a hint that
it is not wise to treat various oxide families separately
(see,e.g.,[176]),all of them having similar perovskite
like ion structures [23,25,26,177–181] and similar
normal and superconducting properties [27],whatever
the values of their critical parameters are.As for the
apparent dispersion of the latter among superconducting
oxides,it mostly reﬂects their conventional exponential
dependences on atomic and itinerantelectron characteristics
[9,10].
The junior member of the superconducting oxide family,
SrTiO
3
−
δ
,demonstrates (although not in a spectacular
manner) several important peculiarities,which are often
considered as properties intrinsic primarily to highT
c
cuprates.Indeed,in addition to the low n,this polar,almost
ferroelectric [182,183],material was shownto reveal polaron
conductivity [184] and is suspected to possess bipolaron
superconductivity [185–187],ﬁrst suggested by Vinetskii
almost 50 years ago [188].It means that SrTiO
3
−
δ
might
be not a BardeenCooperSchrieﬀer (BCS) superconductor
[189] with a large coherence length ξ
0
a
0
,where a
0
is the crystal lattice constant,but most likely an example
of a material with ξ
0
a
0
,so that a Bosecondensation
of local electron pairs would occur at T
c
,according to the
SchafrothButlerBlatt scenario [190] or its later extensions
[8,134,135,191–199].
The concept of bipolarons (local charge carrier pairs) has
been later applied to BPB [200–203],Ba
1
−
x
K
x
BiO
3
−
δ
(BKB,
T
c
≤
30K[204,205]) [203,206,207] and cuprates [195,199,
208–211].It was explicitly shown for BPB and BKB by X
ray absorption spectroscopy [203] that bipolaronic states and
CDWs coexist and compete,which might lead,in particular,
to the observed nonmonotonic dependence T
c
(x) [212].At
the same time,Hall measurements demonstrate that the
more appropriate characteristics T
c
(n) is monotonic [56,
213,214],so that the expected suppression of T
c
at high n
as a consequence of screening of the electronphonon matrix
elements [99,215,216] is not achieved here as opposed to
the curve T
c
(n) [170] in reduced samples of SrTiO
3
−
δ
.As
for cuprates,the bipolaron superconductivity mechanism,
as well as any other BEC scheme,in its pure state would
require an existence of the preformed electron (hole) pairs
(bipolarons),which might be the case [177,217],and a prior
destruction of the Fermi surface (FS),the condition con
tradicting observations (see,e.g.,[218]).Therefore,boson
fermion models for charge carriers in superconductors was
introduced [134,219–225] and,later on,severely criticized
[226,227].In any case,the available objections concern
the bipolaronic mechanism of superconductivity itself,the
occurrence of polaronic eﬀect in oxides with high dielectric
permittivities raising no doubt [115,177,199,228–232].
It is remarkable that the bosonfermion approach men
tioned above is not a unique tool for describing super
conductivity in complex systems.A necessary “degree of
freedom” connected to another group of charge carriers
has been introduced,for example,as the socalled (
−
U)
centers [233–235],earlier suggested by Anderson [236]
as a phenomenological reincarnation of bipolarons in
amorphous materials [188].Independently,narrowband
nondegenerate charge carriers submerged into the sea of
itinerant electrons were proposed for cuprates as another,
not fully hybridized kind of the “second heavy component”
[237,238].For completeness,we should also mention a
quite diﬀerent model involving a second heavy charge carrier
subsystem (delectrons in transition metals [239] or heavy
holes in degenerate semiconductors [240]),necessary to
convert highfrequency Langmuir plasmons intrinsic to the
itinerant electron component into the ionacoustic collective
excitation branch,in order that a highT
c
superconductivity
would appear.Those hopes,however,lack support fromany
evidence in natural or artiﬁcial systems (see the analysis
of plasmon mechanisms [206,241–247],the optimism of
some authors seems to us and others [248] a little bit
exaggerated).As can be readily seen from the References
given above,all nonconventional approaches,rejecting or
generalizing the BCS scheme and going back to the expla
nations of a relatively weak superconductivity in degener
ate semiconductors [138,191,215,249–252],have been
applied to every family of superconducting oxides,including
cuprates.
4 Advances in Condensed Matter Physics
Strontium titanate became a testing ground [253] of
one further attractive idea (based on the same concept
of several interacting charge carrier components) of two
gap or multigap superconductivity,with the interband
interplay being crucial to the substantial increase of T
c
and other critical parameters.The corresponding models
came into being in connection with the transition sd
metals [254,255].They were subsequently applied to analyze
superconductivity in multivalley semiconductors [256,257],
highT
c
oxides [231,258–266],MgB
2
[40,267–269],ZrB
12
[270],V
3
Si [271],Mg
10
Ir
19
B
16
[272],YNi
2
B
2
C [273],NbSe
2
[274,275],R
2
Fe
3
Si
5
(R
=
Lu,Sc) [276],Sc
5
Ir
4
Si
10
[277],
Na
0.35
CoO
2
·
1.3H
2
O[278] as well as pnictides LaFeAsO
1
−
x
F
x
[279],LaFeAsO
0.9
F
0.1
[280],SmFeAsO
0.9
F
0.1
[281],and
Ba
0.55
K
0.45
Fe
2
As
2
[282],Ba
1
−
x
K
x
Fe
2
As
2
with T
c
32K
[283].We did not explicitly include into the list such
modiﬁcations of magnesium diboride as Mg
1
−
x
Al
x
B
2
or
Mg(B
1
−
x
C
x
)
2
,and so forth.
Since,instead of one,two or more wellseparated super
conducting energy gaps,a continuous,sometimes wide,gap
distribution is often observed (see results for Nb
3
Sn in [284]
and MgB
2
in [285–289]),the original picture of the gap
multiplicity in the momentum,k,space loses its beauty,
whereas the competing scenario [76,290] of the spatial
(rspace) extrinsic or intrinsic gap spread becomes more
adequate and predictive [77–79].For the case of cuprates,
it has been recently shown experimentally that the spread is
really spatial,but corresponds to the pseudogap (CDWgap)
rather than its superconducting counterpart,the latter most
probably being a single one [291] (see also the discussion in
[83] and below).
In accordance with what was already mentioned,the
application of very diﬀerent,sometimes conﬂicting,models
to oxide families,including cuprates,means an absence of
a deep insight into the nature of their superconducting and
normal state properties.We are not going to analyze here the
successes and failures of the microscopic approaches to high
T
c
superconductivity in detail;instead we want to emphasize
that even the bosonmediators (we accept the applicability
of the Cooperpairing concept to oxides on the basis of
crucial ﬂuxquantization experiments [292,293]) are not
known for sure.Indeed,at the early stages of the highT
c
studies,magnons were considered as glue,coupling electrons
or holes.The very temperaturecomposition (doping) phase
diagrams supported this idea,since undoped and slightly
doped oxides were found antiferromagnetic [26,103,294–
304].However,a plethora of theories suggesting virtual
spin ﬂuctuations as the origin of superconductivity in
highT
c
oxides and leading to the d
x
2
−
y
2
symmetry of the
superconducting order parameter have been developed [6,
11,15,103,302,305–310].
Fortunately for the scholars,it became clear that reality
is richer for oxides than was expected,so that (i) the order
parameter may include a substantial swave admixture [109,
116–129];and (ii) phonons still exist in perovskite crystal
lattices,inevitably aﬀecting or,may be,even determining
the pairing process [4,10,112,115,311],not to talk
about polaron and bipolaron eﬀects discussed above.It
should be noted that there are reasonable scenarios of
dwave order parameter symmetry in the framework of the
electronphonon interaction alone [208,312–316] (a similar
conclusion was made for the case of plasmon mechanism
[317]).
At the same time,if one adopts a substantial (crucial?)
role of spinﬂuctuation mechanismin superconductivity,the
ubiquitous phonons can (i) be neutral to the dominant d
wave pairing;(ii) act synergetically with spin ﬂuctuations;
(iii) or reduce T
c
,as it would have been for switchedoﬀ
phonons.The existing theories support all three variants,
although some authors cautiously avoid any direct conclu
sions [103].For instance,Kuli
´
c demonstrated the destructive
interference between both mechanisms of superconductivity
[4].Phononic reduction of the magnetically induced T
c
was
claimed in [308,318],whereas anisotropic phonons seemto
enhance T
c
,thus obtained [319].Finally,according to [228,
320,321],spins and phonons act constructively in cuprates.
Once again,the microscopic approach was incapable of
unambiguously predicting a result for the extremely complex
system.
One should bear in mind that the problemis much wider
than the interplay between spin excitations and phonons.
Namely,it is more correct to consider the interplay between
Coulomb interelectron and electronlattice interactions
[232,322].Of course,the latter is also Coulombic in nature,
phonons being simply an ion sound,that is,ion Langmuir
plasma oscillations [323] screened in this case by degenerate
light electrons [324] (thus,acoustic phonons constitute a
similar phenomenon as the acoustic plasmons in the electron
system [239,240] with an accuracy to frequencies).One of
the main diﬃculties is howto separate the metal constituents
in order that some contributions would not be counted
twice [322,325–333].Since it is possible to do rigorously
only in primitive plasmalike models [91,92,99,251,322],
the problem has not been solved.Therefore,empirical
considerations remain the main source of future success for
experimentalists,as it happened,for example,in the case of
MgB
2
[37].
3.CDWs and CDWRelated Phenomena
in Cuprates
The reasoning presented in Section 2 demonstrates that for
the objects concerned,it is insuﬃcient to rely only on
microscopic theories,so that phenomenological approaches
should deserve respect and attention.In actual truth,they
might not be less helpful in understanding the normal and
superconducting properties of cuprates,being generaliza
tions of a great body of experimental evidence collected
during last decades.In this section,we are going to show
that two very important features are common to all highT
c
families.Speciﬁcally,these are the intrinsic inhomogeneity
of nonstoichiometric superconducting ceramic and single
crystalline samples [334–343] and the persistence of CDWs
[340,344,345] and other phenomena,which we also
consider as CDWmanifestations (diphump structures,DHS
[339,346–348],and pseudogaps below and above T
c
[349–
358] in tunneling spectra and angleresolved photoemission
spectra,ARPES).
Advances in Condensed Matter Physics 5
(π/a
0
,π/a
0
)
(π/a
0
,0)
q
CDW
Figure 1:(Color online) Fermi surface nesting;and tightbinding
calculated Fermi surface (solid black curve) of optimally doped
Bi
2
Sr
2
CuO
6+δ
based on ARPES data [373].The nesting wave vector
(black arrow) in the antinodal ﬂat band region has length 2π/6.2a
0
.
Underdoped Bi
2
Sr
2
CuO
6+δ
Fermi surfaces (shown schematically as
red dashed lines) show a reduced volume and longer nesting wave
vector,consistent with a CDW origin of the dopingdependent
checkerboard pattern reported here (Taken from[344]).
CDWs were seen directly as periodic incommensurate
structures in superconducting Bi
2
Sr
2
CaCu
2
O
8+δ
(BSCCO)
using various experimental methods [12,334,359–370].
Photoemission studies reveal the 4a
0
×
4a
0
chargeordered
“checkerboard” state in Ca
2
−
x
Na
x
CuO
2
Cl
2
[371],and tunnel
measurements visualized the same kind of ordering in
BSCCO [370].Scanning tunnel microscopy (STM) mea
surements found CDWs in Bi
2
Sr
1.4
La
0.6
CuO
6+δ
(T
max
c
≈
29K) with an incommensurate period and CDW wave
vectors Q depending on oxygen doping degree [340].The
same method revealed nondispersive (energyindependent)
checkerboard CDWs in Bi
2
−
y
Pb
y
Sr
2
−
z
La
z
CuO
6+x
(T
c
≈
35K
for the optimally doped composition) [344].In this case,Q
substantially depends on doping,rising fromπa
−
1
0
/6.2 in an
optimally doped sample to πa
−
1
0
/4.5 for an underdoped sam
ple with T
c
≈
25K.It is easily explained by the authors taking
into account the shrinkage of the hole FS with decreasing
hole number,so that the vector Q that links the ﬂat nested
FS sections grows,whereas the CDW period decreases (see
Figure 1).One should note that,in the presence of impurities
(e.g.,an inevitably nonhomogeneous distribution of oxygen
atoms),the attribution of the observed charge order (if any)
to unidirectional or checkerboard type might be ambiguous
[372].
A similar coexistence of CDWs and superconductivity
was observed in a good many diﬀerent kinds of materials
with a reduced dimensionality of their electron system,
so that the corresponding FS includes nested (congruent)
sections [158–160].For completeness,we will add some new
cases discovered after our previous reviews were published.
First of all,the analogy between CDWs in cuprates and
layered dichalcogenides was proved by ARPES [352,374–
376].It should be noted that CDW competition with
superconductivity in cuprates was supposed as early as
in 1987 on the basis of heat capacity and optical studies
[377],whereas the similarity between highT
c
oxides and
dichalcogenides was ﬁrst noticed by Klemm [378,379].
Additionally,a new dichalcogenide system Cu
x
TiSe
2
was
found with coexisting superconductivity and CDWs (at
0.04 < x < 0.06) [380,381].The coexistence between two
phenomena was observed in the organic material α(BEDT
TTF)
2
KHg(SCN)
4
,but superconductivity was attributed to
boundaries between CDWdomains,where the CDWorder
parameter is suppressed [382].Highpressure studies of
another organic conductor (Per)
2
[Au(mnt)
2
] revealed an
appearance of superconductivity after the CDWsuppression
[383].Still,it remained unclear,whether some remnants of
CDWs survived in the superconducting region of the phase
diagram.Application of high pressure also suppressed CDWs
in the compound TbTe
3
at about P
=
2.3 GPa,inducing
superconductivity with T
c
≈
1.2K,enhanced to 4K at P
=
12.4 GPa [384],the behavior demonstrating the competition
of Cooper and electronhole pairings for the FS [385,
386].The same experiments in this quasitwodimensional
material revealed two kinds of CDW anomalies merging at
P
=
2.3 GPa,as well as antiferromagnetism,which makes
this object especially promising.Finally,CDWs were found
in another superconducting oxide Na
0.3
CoO
2
·
1.3 H
2
O by
speciﬁc heat investigations [387–389],showing twoenergy
gap superconductivity for asprepared samples and non
superconducting CDWdielectrized state after ageing of the
order of days.The sample ageing is a situation widely met
for superconductors [390,391],whereas the dielectrization
of assynthesized superconducting ceramic samples accom
panied by a transformation of bulk superconductivity into a
percolating one with the CDWbackground was observed for
BPBlong ago [56,392].Nevertheless,such a scenario was not
proved directly at that time,while the bulk heat capacity peak
in Na
0.3
CoO
2
·
1.3 H
2
O [387–389] unequivocally shows the
emergence of CDWs instead of superconductivity.
We emphasize that CDWs compete with superconduc
tivity,whenever they meet on the same FS.This is the
experimental fact,which agrees qualitatively with a number
of theories [385,386,393–397].
Returning to cuprates,we want to emphasize that the
existence of pseudogaps above and below T
c
is one of
their most important features.Pseudogap manifestations are
diverse,but their common origin consists in the (actually,
observed) depletion of the electron densities of states (DOS).
It is natural that tunnel and ARPES experiments,which are
very sensitive to DOS variations,made the largest contri
bution to the cuprate pseudogap data base (see references
in our works [81–83,158–160]).Recent results show that
the concept of two gaps (the superconducting gap and
the pseudogap,the latter considered here as a CDW gap)
[82,352,353,357,377,398–404] begins to dominate in
the literature over the onegap concept [211,355,405–416],
according to which the pseudogap phenomenon is most
frequently treated as a precursor of superconductivity (for
instance,a gas of bipolarons that Bosecondenses below
T
c
[413] or a dwave superconductinglike state without
a longrange phase rigidity [416]).The main arguments,
6 Advances in Condensed Matter Physics
which make the onegap viewpoint less probable,is the
coexistence of both gaps below T
c
[349,417],their diﬀerent
position in the momentum space of the twodimensional
Brillouin zone [351,353,356,418,419],and their diﬀerent
behaviors in the external magnetic ﬁelds H[420],for various
dopings [417],and under the eﬀects of disordering [419].
Nevertheless,some puzzles still remain unresolved in the
pseudogap physics.For instance,Kordyuk et al.[352] found
that the pseudogap in Bi(Pb)
2
Sr
2
Ca(Tb)Cu
2
O
8+δ
revealed
by ARPES is nonmonotonic in T.Such a behavior,as they
indicated,might be related to the existence of commensurate
and incommensurate CDW gaps,in a close analogy with
the case of dicahlcogenides [421].Another photoemission
study of La
1.875
Ba
0.125
CuO
4
has shown [354] that there seems
to be two diﬀerent pseudogaps:a dwavelike pseudogap—
a precursor to superconductivity—near the node of the
truly superconducting gap and a pseudogap in the antinodal
momentum region—it became more or less familiar to the
community during last years [350,351,353,356,403,418,
419] and is identiﬁed by us as the CDWgap.
Despite existing ambiguities,the most probable scenario
of the competition between CDW gaps (pseudogaps) and
superconducting gaps in highT
c
oxides,in particular,in
BSCCO,includes the former emerging at antinodal (nested)
sections of the FS and the latter dominating over the nodal
sections (see Figure 2,reproduced from[403],where BSCCO
was investigated,and results for (Bi,Pb)
2
(Sr,La)
2
CuO
6+δ
presented in [356]).Since CDW gaps are much larger
than their superconducting counterparts,the simultaneous
existence of the superconducting gaps in the antinodal region
might be overlooked in the experiments.This picture means
that the theoretical model of the partial dielectric gapping
(of CDWorigin or caused by a related phenomenon—spin
density waves,SDWs) belonging to Bilbro and McMillan
[385] (see also [56,158–160,386,397,422–428]) is ade
quate for cuprates.On the other hand,the coexistence of
CDW and superconducting gaps,each of them spanning
the whole FS [429–432],can happen only for extremely
narrow parameter ranges [433].Moreover,as is clearly
seen from data presented in Figure 2 [403] and a lot of
other measurements for diﬀerent classes of superconductors,
complete dielectric gapping has not beenrealized.The reason
is obvious:nested FS sections cannot spread over the whole
FS,since the actual crystal lattice is always threedimensional
and threedimensionality eﬀects lead to the inevitable
FS warping detrimental to nesting conditions formulated
below.
It is interesting that pseudogaps were also observed in
oxypnictides LaFeAsO
1
−
x
F
x
and LaFePO
1
−
x
F
x
by ARPES
[434] and SmFeAsO
0.8
F
0.2
by femtosecond spectroscopy
[435],where SDWs might play the same role as CDWs do in
cuprates.At the same time,in iron arsenide Ba
1
−
x
K
x
Fe
2
As
2
,
photoemission studies detected a peculiar electronic order
ing with a (π/a
0
,π/a
0
) wave vector [436],a true nature of
which is still not known,but which might be related either
to the magnetic reconstruction of the electron subsystem
(SDWs) and/or to structural transitions (when CDWs
accompanied by periodic crystal lattice distortions emerge
in the itinerant electron liquid near the structural transition
Δk
(meV)
0
20
40
60
(0,π)
(π,π)
(π,0)
Γ
Δk
UD75K
0
15
30
45
60
75
90
(a)
Δk
(meV)
0
20
40
(0,π)
(π,π)
(π,0)
Γ
Δk
UD92K
0
15
30
45
60
75
90
(b)
Δk
(meV)
0
20
40
(0,π)
(π,π)
(π,0)
Γ
Δk
OD86K
0
15
30
45
60
75
90
T
T
c
T < T
c
T > T
c
(c)
Figure 2:(Color online) Schematic illustrations of the gap function
evolution for three diﬀerent doping levels of Bi
2
Sr
2
CaCu
2
O
8+δ
.(a)
Underdoped sample with T
c
=
75K.(b) Underdoped sample with
T
c
=
92K.(c) Overdoped sample with T
c
=
86K.At 10K above T
c
there exists a gapless Fermi arc region near the node;a pseudogap
has already fully developed near the antinodal region (red curves).
With increasing doping,this gapless Fermi arc elongates (thick red
curve onthe Fermi surface),as the pseudogap eﬀect weakens.At T <
T
c
a dwave like superconducting gap begins to open near the nodal
region (green curves);however,the gap proﬁle in the antinodal
region deviates fromthe simple d
x
2
−
y
2
form.At a temperature well
belowT
c
(T
T
c
),the superconducting gap with the simple d
x
2
−
y
2
formeventually extends across entire Fermi surface (blue curves) in
(b) and (c) but not in (a).(Taken from[403].)
temperature T
d
[437,438]).The interplay between structural
and magnetic instabilities is important for pnictides [161],
Advances in Condensed Matter Physics 7
since,for example,structural and SDW anomalies appear
jointly at 140 K in BaFe
2
As
2
[439].It is not inconceivable
that pnictides may be a playground for density waves as
well as highT
c
oxides,with a rich variety of attendant
manifestations.
The DHS is another visiting card of cuprates,being
a peculiarity in tunnel and photoemission spectra at low
T
T
c
and energies much higher than those of coherent
superconducting peaks [81–83,160,339,347,348,440,
441].It is remarkable that in the SIN tunnel junctions,
where S,I,and N stand for a highT
c
superconductor,an
insulator,and a normal metal,respectively,a DHS might
appear for either one bias voltage V polarity only [347] or
both [442,443],depending on the speciﬁc sample.In S
IN junctions,currentvoltagecharacteristics (CVCs) with
two symmetrically located DHSs (one per branch) are also
observed,but with amplitudes that can diﬀer drastically
[442,443].In SIS symmetric junctions,DHS structures
are observable (or not) in CVC branches of both polarities
simultaneously [347],which seems quite natural.It is very
important that although the CVC for every in the series of S
INjunctions with BSCCOas an superconducting electrodes
was nonsymmetric,especially due to the presence of the
DHS,the CVC obtained by averaging over an ensemble
of such junctions turned out almost symmetric,or at
least its nonsymmetricity turned out much lower than the
nonsymmetricity of every CVC taken into consideration
[443].
There is quite a number of interpretations concerning
this phenomenon [347,444–450].We have discussed most
of them in detail in our previous publications,whereas
our theory and necessary reference to other models will be
presented below.
STM mapping of highT
c
oxide samples revealed sub
stantial inhomogeneties of energy gap spatial distribution
[334,336,338,339,341–343,363,370,441,451–459].
The same conclusion was made from the interlayer tun
neling spectroscopy [460,461],more conventional SIN
tunnel (pointcontact) studies [440,442],optical femtosec
ond relaxation spectroscopy [337],and inelastic neutron
scattering measurements [335].It is quite natural that
some inhomogeneity should exist,since the oxygen content
is always nonstoichiometric in those compounds [304].
Indeed,correlations were found between oxygen dopant
atompositions and the nanoscale electronic disorder probed
by STM [336].The problem has been recently investigated
theoretically making allowance for electrostatic modula
tions of various system parameters by impurity atoms
[462].
Nevertheless,the gap distributions occurred to be anom
alously large,with sometimes conspicuous twopeak struc
tures in BSCCO [451,457,463],Bi
2
Sr
1.6
Gd
0.4
CuO
6+δ
[338],
(Cu,C)Ba
2
Ca
3
Cu
4
O
12+δ
[440],and TlBa
2
Ca
2
Cu
2
O
10
−
δ
[442].Nanoscale electronic nonhomogeneity on the crystal
surface was shown to substantially aﬀect the CDWlike DOS
modulation observed by STMin Bi
2
Sr
1.4
La
0.6
CuO
6+δ
[340].
Large gap scatterings obviously do not correlate with
sharp transitions into the superconducting state at any
doping of well prepared samples (implying Cooperpairing
homogeneity),which was demonstrated,for example,by
speciﬁc heat studies [464].To solve the problem,one
should bear in mind that the gaps measured by STM
technique are of two kinds (in our opinion,superconducting
gaps and pseudogaps—CDWgaps),which cannot be easily
distinguished experimentally [81–83,160,337].The guess
was proved in [291],where contributions of both gaps in
the STMspectra of (Bi
0.62
Pb
0.38
)
2
Sr
2
CuO
6+x
were separated
by an ingenious trick.Namely,the authors normalized the
measured local conductances by removing the largergap
inhomogeneous background.Then,it became clear that the
superconducting gap is more or less homogeneous over the
sample’s surface,whereas the larger gap (the pseudogap,i.e.,
the CDWgap) is essentially inhomogeneous.
The intimate origin of the pseudogap variations is cur
rently not understood.At the same time,the inhomogeneity
of electron characteristics is also inherent to the related solid
solutions BPB,which was demonstrated by spatially resolved
electron energy loss spectroscopy [465].It is reasonable to
suggest that this inhomogeneity both in BPB and highT
c
oxides is strengthened near free surfaces in agreement with
Josephson current measurements across BPBbicrystal tunnel
boundaries [466].
Still,there is an interesting phenomenon,which might
explain trends for electric properties in cuprates to be
inhomogeneous.We mean a spontaneous phase separation,
suggested long ago for antiferromagnets [467–470] and the
electron gas in paramagnets [471–474].This idea was later
transformed into stripe activity in cuprate and manganite
physics,where alternating conducting and magnetic regions
constituted separated “phases” [12,302,475–480].Recently,
a lot of evidence for local lattice distortions,JahnTeller
polaron occurrence,and other percolation and ﬁlamentary
structure formation appeared [177,217,228,481–485],sup
porting new sophisticated theoretical eﬀorts in the science
of phase separation [84,230,379,486–493],mostly but
not necessarily dealing with highT
c
oxides.The electronic
inhomogeneity in cuprates,as discussed above,belongs
to the same category of phenomena.Whatever its origin,
intrinsic inhomogeneity of cuprates and other oxides seems
to be an important feature that needs explanation in order to
understand superconductivity (much more homogeneous)
itself.Note that electronic phase separation into magnetic
and nonmagnetic domains was also found in the iron pnic
tide superconductor Ba
1
−
x
K
x
Fe
2
As
2
[494],whereas disorder
induced inhomogeneities of superconducting properties was
observed in TiNﬁlms [495].
Another highT
c
oxide,YBa
2
Cu
3
O
6+x
,containing CuO
chains in addition to CuO
2
planes,was known for a long
time as a material exhibiting onedimensional CDWs [496].
However,the authors of more recent tunnel measurements
[497] concluded that the wouldbe CDW manifestations
might have a diﬀerent nature,since the observed one
dimensional modulation wavelengths have rather a strong
dispersion.Nevertheless,it seems that in view of the
large CDW amplitude scatter in BSCCO discovered later,
this conclusion is premature,with local variations of the
FS shape being a possible origin of CDW wave vector
modiﬁcations.
8 Advances in Condensed Matter Physics
As one sees from the evidence discussed above,CDW
modulations are observed in cuprates both directly (as
patterns of localized energyindependent electron states in
the conventional rspace) and indirectly (as concomitant
gapping phenomena).The pseudogap energy E
PG
> Δ
SC
constitutes an appropriate scale for CDWgapping.Here,Δ
SC
is the superconducting gap.On the other hand,at low ener
gies E < Δ
SC
,singleparticle tunneling spectroscopy probes
mixed electronhole dwave Bogoliubov quasiparticles [498],
which are delocalized excitations.In this case,it is natural
to describe the tunnel conductance in the momentum,
kspace.The interference between Bogoliubov quasiparticles
is especially strong for certain wave vectors q
i
(i
=
1,...,16)
connecting extreme points on the constant energy contours
[499–502].The interference kspace patterns involve those
wave vectors [343,416,499,503–505],this picture being
distinct fromand complementary to the partially disordered
CDW unidirectional or checkerboard structures [344,359,
365,371,458,506–508].
It is remarkable that interference rspace patterns on
cuprate surfaces,the latter being in the superconducting
state,are not detected,contrary to the clearcut STM
observations of electron de Broglie standing waves,induced
by point defects or step edges,revealed in conductance
maps on the normal metal surfaces [509,510].The latter
waves are in eﬀect Friedel oscillations [511] formed by two
dimensional normal electron density crests and troughs with
the wave length π/k
F
,k
F
being the Fermi wave vector.
On the other hand,spatial oscillating structures of local
DOS in the dwave superconducting state are determined
by other representative vectors q
i
,so that the characteristic
oscillations can be denominated as Friedellike ones at most
[502,512].Nevertheless,the attenuation of both kinds of
spatial oscillations due to superconducting modiﬁcations
of the screening medium should be more or less similar.
Namely,in the isotropic superconducting state,the electron
gas polarization operator loses its original singularity at k
=
2k
F
for gapped FS sections [513].As a consequence,Friedel
oscillations gain an extra factor exp(
−
2r/πξ
0
) [514,515],
where ξ
0
is the BCS coherence length [498].For dwave
superconductors,the attenuation will be weaker and will
totally disappear in the orderparameter node directions.
However,those distinctions are not crucial,since the nodes
have a zero measure.The modiﬁcation of screening by
formation of Bogoliubov quasiparticles in dwave highT
c
oxides explains the absence of conspicuous spatial structures
in STM maps,which correspond to the wave vectors q
i
mentioned above.
We consider the observed CDWs in oxides as a conse
quence of electronhole (dielectric) pairing on the nested
sections of corresponding FSs [158–160,516].Such a
viewpoint is also clearly supported by the experiments in
layered dichalcogenides [374–376],the materials analogous
to cuprates in the sense of superconductivity appearance
against the dielectric (CDW) partial gapping background
[378,379].At the same time,other sources of CDW
instabilities are also possible [517,518].As for the micro
scopic mechanism causing CDWformation,it might be an
electronphonon (Peierls insulator) [519,520] or a Coulomb
one (excitonic insulator) [431,521,522],or their speciﬁc
combination.Excitonic instability may also lead to the SDW
state [522,523],also competing with superconductivity for
the FS [160,524–529].It should be noted that researchers
asserted that they found plenty of Peierls insulators or par
tially gapped Peierls metals [158–160,530–532].At the same
time,the excitonic phase,being mathematically identical in
the meanﬁeld limit [533] and physically similar [534] to the
Peierls insulator,was not identiﬁed unequivocally.One can
only mention that some materials claimed to be excitonic
insulators,namely,a layered transitionmetal dichalcogenide
1TTiSe
2
with a commensurate CDW [535,536],alloys
TmSe
0.45
Te
0.55
[537],Sm
1
−
x
La
x
S [538],and Ta
2
NiSe
5
with a
direct band gap at the Brillouin zone Γ point in the parent
highT state [539].Therefore it is reasonable that precisely
in the later case,the lowT excitonic state is not accompanied
by CDWs.
It is necessary to indicate that in many cases,the claimed
“charge stripe order” and the more unpretentious “charge
order” are an euphemism describing the old good CDWs:
“Stripes is a term that is used to describe unidirectional
densitywave states,which can involve unidirectional charge
modulations (charge stripes) or coexisting charge and spin
density order spin stripes” [12].We do not think it makes
sense to use the term “stripes” in the cases of pure CDW
or spindensitywave (SDW) ordered states.At the same
time,this term should be reserved for diﬀerent possible
more general kinds of microseparation [12,477,479,540–
542],having nothing or little to do with periodic lattice
distortions,FS nesting,or Van Hove singularities.The need
to avoid misnomers and duplications while naming concepts
is quite general in science,as was explicitly stressed by
John Archibald Wheeler,who himself coined many terms in
physics (“black hole” included) [543].
In this connection,it seems that some experimental
ists unnecessarily vaguely attribute the spatially periodical
charge structure in the lowtemperature tetragonal phase
of La
1.875
Ba
0.125
CuO
4
,revealed by Xray scattering [544],
to the hypothetical nematic structure or the checkerboard
Wigner crystal.Indeed,quite similar spatial charge structures
found in La
1.875
Ba
0.125
−
x
Sr
x
CuO
4
by neutron scattering [545]
were correctly and without reservation identiﬁed as CDW
related ones,whereas a checkerboard structure (if any)
can be considered as a superposition of two mutually
perpendicular CDWs.The same can be written about the
“stripe” terminology used in [546],where Xray scattering
revealed a periodical charge structure in the lowtemperature
tetragonal phase of another cuprate La
1.8
−
x
Eu
0.2
Sr
x
CuO
4
.
One should mention two other possible collective states
competing withCooper pairing.Namely,these are states with
microscopic orbital and spin currents that circulate in the
ground state of excitonic insulator (there can be four types of
the latter [522]).The concept of the state with current circu
lation,preserving initial crystal lattice translational symme
try,was invoked to explain cuprate properties [547].Another
order parameter,hidden from clearcut identiﬁcation by
its supposed extreme sensitivity to sample imperfection,is
the socalled ddensity waveorder parameter [548,549].
It is nothing but a CDW order parameter times the same
Advances in Condensed Matter Physics 9
formfactor f (k)
=
cos(k
x
)
−
cos(k
y
),the product being
similar to that for d
x
2
−
y
2
superconductors.Here,k
x
and
k
y
are the wavevector components in the CuO
2
plane.To
some extent,the dielectric order parameter of the Bilbro
McMillan model [159,160,385] and its generalizations—
they are presented below—contains the same physical idea
as in the ddensitywave model:nonuniformity of the CDW
gap function in the momentumspace.
Although the destructive CDWaction on superconduc
tivity of many good materials is beyond question [56,160,
380,384,545,550,551],it does not mean that maximal T
c
are
limited by this factor only.For instance,T
c
falls rapidly with
the hole concentration p in overdoping regions of T
c
−
p
phase diagrams for diﬀerent Pbsubstituted Bi
2
Sr
2
CuO
6+δ
compounds,even in the case when the critical doping value
p
cr
corresponding to T
d
→
0 lies outside the superconduct
ing dome [552].A Cudoped superconducting chalcogenide
Cu
x
TiSe
2
constitutes another example conﬁrming the same
trend [380].Namely,CDW manifestations die out for x
0.06,whereas T
c
starts to decrease for x > x
optimal
=
0.08.
As has been already mentioned,overdoping can reduce T
c
simply owing to screening of matrix elements for electron
phonon interaction [99,215,216].
4.Theory of CDWSuperconductors and
Its Application to Cuprates
The majority of our results presented below were obtained
for swave superconductors with CDWs.It is a case,
directly applicable to many materials (e.g.,dichalcogenides,
trichalcogenides,tungsten brozes,etc.).On the other hand,
as was indicated above,the exact symmetry of the supercon
ducting order parameter in cuprates is not known,although
the dwave variant is considered by most researchers in the
ﬁeld as the ultimate truth.Notwithstanding any future solu
tion of the problem,our theory of CDWrelated peculiarities
in quasiparticle tunnel CVCs can be applied to cuprates,
since we are not interested in small energies eV < Δ,where
the behavior of a reconstructed DOS substantially depends
on whether it is the s or dwave order parameter [553–
555].Here,e > 0 is the elementary charge,and Δ is the
amplitude of the superconducting order parameter.As for
the thermodynamics of CDW superconductors,we present
both s and dcases,each of them having their own speciﬁc
features.
4.1.Thermodynamics of sWave CDW Superconductors.The
DysonGorkov equations for the normal (G
i j
) and anoma
lous (F
i j
) temperature Green’s functions in the case of
coupled superconducting Δ
αγ
i j
and dielectric (CDW) Σ
αγ
i j
matrix order parameters are the starting point of calculations
and can be found elsewhere [160,386,397,426,427].Greek
superscripts correspond to electron spin projections,and
italic subscripts describe the natural split of the FS into
degenerate (nested,d) and nondegenerate (nonnested,n)
sections.For the quasiparticles on the nested sections,the
standard condition leading to the CDWgapping holds:
ξ
1
p
= −
ξ
2
p +Q
,
(1)
where p is the quasimomentum,Q is the CDW vector
(see the discussion above),Planck’s constant
=
1.This
equation binds the electron and hole bands ξ
1,2
(p) for the
excitonic insulator [431,522] and diﬀerent parts of the
onedimensional selfcongruent band in the Peierls insulator
case [516].At the same time,the rest of the FS remains
undistorted below T
d
and is described by the electron
spectrumbranch ξ
3
(p).Such an approach was suggested long
ago by Bilbro and McMillan [385].We adopt the strong
mixing approximation for states from diﬀerent FS sections.
This means an appearance of a single superconducting
order parameter for d and nd FS sections.The spinsinglet
structure (swave superconductivity and CDWs) of the
matrix normal (Σ
αγ
i j
=
Σδ
αβ
) and anomalous (Δ
αγ
i j
=
I
αβ
)
selfenergy parts (where (I
αβ
)
2
= −
δ
αβ
) in the weakcoupling
limit is suggested.Here,δ
αβ
is the Kronecker delta.The self
consistency equations for the order parameters obtained in
accordance with the fundamentals can be expressed in the
following form[386]:
1
=
V
BCS
N
(
0
)
μI
(
D
)
+
1
−
μ
I
(
Δ
)
,
1
=
V
CDW
N
(
0
)
μI
(
D
)
,
(2)
where
I
(
x
)
=
Ω
0
dξ
ξ
2
+x
2
tanh
ξ
2
+x
2
2T
.(3)
Here,the Boltzmann constant k
B
=
1,V
BCS
and V
CDW
are
contact fourfermion interactions responsible for supercon
ductivity and CDWgapping,respectively.The gap
D
(
T
)
=
Δ
2
(T) +Σ
2
(T)
1/2
(4)
is a combined gap appearing on the nested FS sections,
whereas the order parameter Δdeﬁnes the resulting observed
gap on the rest of the FS (compared with the situation in
cuprates [344,350,356,403]).The parameter μ characterizes
the degree of the FS dielectrization (hereafter,we use this
nonconventional terminstead of “gapping” in some places to
avoid confusion with the superconducting gapping),so that
N
d
(0)
=
μN(0) and N
nd
(0)
=
(1
−
μ)N(0) are the electron
DOSs per spin on the FS for the nested and nonnested
sections,respectively.The upper limit in (3) is the relevant
cutoﬀ frequency,which is assumed to be equal for both
interactions.If the cutoﬀs BCS and CDW are considered
diﬀerent,the arising correction,log(Ω
CDW
/Ω
BCS
),is loga
rithmically small [385] and does not change qualitatively
the subsequent results.Only in the case of almost complete
electron spectrum dielectric gapping (μ
→
1) does the
diﬀerence between BCS and CDW become important for
the phase coexistence problem [433].This situation is,
however,of no relevance for substances with detectable
superconductivity,since T
c
tends to zero for μ
→
1.In
this subsection,we conﬁne ourselves to the case Re Σ > 0,
ImΣ
=
0,since the phase ϕ of the complex order parameter
Σ
≡ 
Σ

e
iϕ
does not aﬀect the thermodynamic properties,
whereas tunnel currents do depend on ϕ [160,556,557],
which will be demonstrated explicitly below.
10 Advances in Condensed Matter Physics
Introducing the bare order parameters Δ
0
=
2Ωexp[
−
1/V
BCS
N(0)] and Σ
0
=
2Ωexp[
−
1/V
CDW
N
d
(0)],
we can rewrite the system of (2) in an equivalent form,
convenient for numerical calculations:
I
M
[
Δ,T,Δ
(
0
)
]
=
0,
I
M
(
D,T,Σ
0
)
=
0,
(5)
where
I
M
(
G,T,G
0
)
=
∞
0
⎛
⎝
1
ξ
2
+G
2
tanh
ξ
2
+G
2
2T
−
1
ξ
2
+G
2
0
⎞
⎠
dξ
(6)
is the standard M
¨
uhlschlegel integral [558],the root of which
G
=
sM
¨
u(G
0
,T) is the wellknown gap dependence for the
swave BCS superconductor [9],G
0
=
G (T
=
0),and [385]
Δ
(
0
)
=
Δ
0
Σ
−
μ
0
1/(1
−
μ)
.
(7)
However,(5) mean that both gaps Δ(T) and D(T) have
the BCS form G
=
sM
¨
u(G
0
,T) [386],namely:(i) Δ(T)
=
sM
¨
u[Δ(0),T],that is,the actual value of the superconducting
gap of the CDWsuperconductor at T
=
0 is Δ(0) rather than
Δ
0
,and the actual superconducting critical temperature is
T
c
=
γΔ(0)/π;(ii) at the same time,D(T)
=
sM
¨
u(Σ
0
,T),
which determines T
d
=
γΣ
0
/π.Here,γ
=
1.7810...is the
Euler constant.
From(4),we obtain that,at T
=
0,
Σ
2
0
=
Δ
2
(
0
)
+Σ
2
(
0
)
.
(8)
Replacing Δ(0) by its value (7),we arrive at the conclusion
that in the model of swave superconductor with partial
CDWgapping,two order parameters coexist only if Δ
0
< Σ
0
.
Then,according to (7),Δ(0) < Δ
0
;that is,the formation of
the CDW,if it happens,always inhibits superconductivity,in
agreement with the totality of experiments [160,375,380,
382,551].Also,vice versa,according to (4),for T < T
c
,
Σ(T) < sM
¨
u(Σ
0
,T);that is,superconductivity suppresses
dielectrization.
In Figure 3,the dependences Δ(T) and Σ(T) are shown
for various parameters of the partially dielectrized CDW
swave superconductor.It can be easily inferred from the
data shown in both panels that,in agreement with the
foregoing,Δ(T)/Δ(0) curves coincide with the M
¨
uhlschlegel
one for any values of the dimensionless parameters μ and
σ
0
≡
Σ
0
/Δ
0
.The novel feature,which has been overlooked
in other investigations,is the possibility of such a strong
suppression of Σ for low enough T that it becomes smaller
than Δ,although T
d
is larger than T
c
(see Figure 3(b)).This
intriguing situation can be realized for the parameter σ
0
close
to unity.One should note that the actual gaps Δ and D (the
former coincides with the superconducting order parameter)
are monotonic functions of T.However the dielectric order
parameter is not.
The magnitudes of T
c
and Δ(0) strongly depend on μ
and σ
0
,although the simple BCSlike scaling between them
survives,that is,for CDWswave superconductors Δ(0)/T
c
=
π/γ
≈
1.76.Although for,say,Σ
0
≥
1.5Δ
0
and reasonable
μ
=
0.5 [386],the demand of selfconsistency between Σ(T)
and Δ(T) becomes less important quantitatively.It justiﬁes
our previous approach with Tindependent Σ [427] and the
estimation of combined gap as (Δ
2
BCS
(T) +Δ
2
PG
)
1/2
with T
independent Δ
PG
made on the basis of interlayer tunneling
measurements in BSCCOmesas [559];selfconsistency leads
to new qualitative eﬀects and cannot be avoided.As for
the magnitude of the very Δ
PG
,inferred from tunneling
measurements,it was found in [559] to be substantially
smaller than that of Δ
BCS
(T
→
0),whereas the opposite case
turned out to be true both for BSCCO [349,399,560,561],
Bi
2
−
x
Pb
x
Sr
2
CaCu
2
O
8+δ
[460],and (Bi,Pb)
2
Sr
2
Ca
2
Cu
3
O
10+δ
[562].Other tunnel measurement for BSCCO[417] revealed
Δ
PG
> Δ
BCS
(T
→
0) for underdoped samples and Δ
PG
<
Δ
BCS
(T
→
0) for overdoped ones.A marked sensitivity
of Δ
PG
to doping together with strong inhomogeneity,
discoveredinBibasedceramics [334–336,338,343,359,440,
441,456–458,563,564] and Ca
2
−
x
Na
x
CuO
2
Cl
2
[565],may
be responsible for the indicated discrepancies.
Since the BCS character of the gap dependences for the
CDWswave superconductor is preserved,the Tdependence
of the heat capacity C for the doubly gapped electron liquid
(i.e.,below the actual T
c
) equals to the superposition of two
BCSlike functions:
C
(
T
)
=
2π
2
N
(
0
)
3
1
−
μ
T
c
c
BCS
T
T
c
+μT
d
c
BCS
T
T
d
,
(9)
where
c
BCS
t
=
T
T
BCS
c
=
C
BCS
(
T
)
C
BCS
T
=
T
BCS
c
+0
.(10)
It should be noted that the normalized discontinuity
ΔC/C
n
(T
c
) at the superconducting phase transition may also
serve as indirect evidence for the CDW gap on the FS,
because in this case it is not at all a trivial BCS jump:
ΔC
BCS
γ
S
T
c
=
12
7ζ
(
3
)
≈
1.43.
(11)
Here,C
n
(T)
=
γ
S
T
≡
(2π
2
N(0)/3)T is the normal
electrongas heat capacity,whereas γ
S
is the Sommerfeld
constant.CDWdriven deviations from the BCS behavior
was recognized long ago [425,566].However,only the self
consistent approach [386] allows us to give a quantitative
answer at any value of the parameters appropriate to the
partially CDWgapped superconductor.It can be seen from
Figure 4(a),where the conventionally normalized supercon
ducting phase transition anomaly is shown as a function of
μ.The discontinuity is always smaller than the BCS value
(11),in agreement with previous qualitative considerations
[425,566].At the same time,the BCS ratio is restored not
only for μ
=
0,that is,in the absence of the dielectrization,
but also for μ
→
1.In the former case,it is clear,because
we are dealing with a conventional BCS superconductor.
On the other hand,for large enough μ,CDW gapping
Advances in Condensed Matter Physics 11
Δ/Δ0
,Σ/Σ0
0
0.5
1
1.5
t
=
T/T
c
0 0.5 1 1.5 2
σ
0
=
1.5
μ
=
0 (BCS)
μ
=
0.1
μ
=
0.5
Σ
Σ
Δ
Δ
Δ
(a)
Δ/Δ0
,Σ/Σ0
0
0.5
1
t
=
T/T
c
0 0.5 1 1.5 2 2.5
σ
0
=
1.1
μ
=
0 (BCS)
μ
=
0.5
μ
=
0.9
Σ
Σ
Δ
Δ
Δ
(b)
Figure 3:Temperature dependences of the superconducting (Δ) and dielectric (Σ) order parameters for diﬀerent values of the dimensionless
parameters μ (the portion of the nested Fermi surface sections,where the chargedensitywave,CDW,gap develops) and σ
0
(see explanations
in the text).(Taken from[386].)
almost completely destroys superconductivity,so T
c
T
d
.
Therefore,in the relevant superconducting T range,the
contribution to C(T) from the d FS sections,governed by
the gap D
≈
Σ,becomes exponentially small.Another term,
determined by the n FS section,ensures the BCS limiting
value of the normalized discontinuity.
The dependences of ΔC/C
n
on σ
0
for various values of μ
are depicted in Figure 4(b).One sees that the eﬀect is large
for σ
0
close to unity,whereas the diﬀerence between 1.43 and
ΔC/C
n
goes to zero as σ
−
2
0
,verifying the asymptotical result
[425].It should be noted that the heat capacity calculation
scheme adopted for swave CDW superconductors can be
applied also to other types of order parameter symmetry.
Experimental data on heat capacity,which could conﬁrm
the expressed ideas,are scarce.For Nb
3
Sn,it was recently
shown by speciﬁc heat measurements using the thermal
relaxation technique that T
c
≈
17
÷
18K is reduced when
the critical temperature of the martensitic transition T
d
≈
42
÷
53K grows [567].Unfortunately,a large diﬀerence
between T
c
and T
d
made the eﬀects predicted by us quite
small here,which is probably the reason why they have not
been observed in these studies.
As for cuprates,reference should be made to
La
2
−
x
Ba
x
CuO
4
−
y
[568],La
2
−
x
Sr
x
CuO
4
−
y
[569],and
YBa
2
Cu
3
O
7
−
y
[570],where underdoping led to a reduction
of ΔC/C
n
.The same is true for measurements of the
heat capacity in Bi
2
Sr
2
−
x
La
x
CuO
6+δ
single crystals [571],
which demonstrated that the ratio ΔC/C
n
for a strongly
underdoped sample turned out to be about 0.25,that is,
much below BCS values 12/7ζ(3)
≈
1.43 and 8/7ζ(3)
≈
0.95
[572] for swave and dwave superconductivity,respectively.
There is also an opposite evidence for the relationship
ΔC/C
n
> 1.43,for example,in the electrondoped highT
c
oxide Pr
1.85
Ce
0.15
CuO
4
−
δ
[573].More details,as well as
information on other CDWsuperconductors,can be found
in [386].In any case,despite the wellknown challenging
controversy for BPB [392,574–576],the problem was not
studied enough for any superconducting oxide family,
probably due to experimental diﬃculties.
4.2.Enhancement of the Paramagnetic Limit in sWave CDW
Superconductors.Upper critical magnetic ﬁelds H
c2
[577–
579] (along with critical currents [132,579,580]) belong
to main characteristics of superconductors crucial for their
applications.In particular,knowing the upper limits on
upper critical ﬁelds is necessary to produce superconducting
materials for highperformance magnets,not to talk about
scientiﬁc curiosity.
One of such limiting factors is the paramagnetic destruc
tion of spinsinglet superconductivity,which was discovered
long ago theoretically by Clogston [581] and Chandrasekhar
[582].In the framework of the BCS theory,they obtained a
limit
H
BCS
p
=
Δ
BCS
(
T
=
0
)
μ
∗
B
√
2
(12)
from above on H
c2
at zero temperature,T.Here,Δ
BCS
(T)
is the energy gap in the quasiparticle spectrum of BCS s
wave superconductor,and μ
∗
B
is the eﬀective Bohr magneton,
which may not coincide with its bare value μ
B
=
e/2mc,
where is Planck’s constant,equal to unity in the whole
12 Advances in Condensed Matter Physics
ΔC/C
n(Tc
)
0
0.5
1
1.5
μ
=
N
d
(0)/N(0)
0 0.2 0.4 0.6 0.8 1
σ
0
=
1.1
σ
0
=
1.5
σ
0
=
2
(a)
ΔC/C
n(Tc
)
0
0.5
1
1.5
σ
0
=
Σ
0
/Δ
0
1 2
μ
=
0.1
μ
=
0.5
μ
=
0.8
(b)
Figure 4:Dependences of the normalized heat capacity discontinuity ΔC at T
c
on μ (a) and σ
0
(b).(Taken from[386].)
article but shown here explicitly for clarity,mis the electron
mass,and c is the velocity of light.
Limit (12) may be overcome at a high concentration of
strong spinorbit scatterers,when the spins of the electrons,
constituting the Cooper pairs,are ﬂipped [583].Then,the
actual H
c2
(T
=
0) starts to exceed [584] the classical bound.
Such an enhancement of H
c2
has been observed,for example,
in Al ﬁlms coated with Pt monolayers [585].The Pt atoms
served there as strong spinorbit scatterers due to their
large nuclear charge Z.One should indicate a possibility of
exceeding value (12),if the energy,E,dependence of the
normal state density of states is signiﬁcant,which is the case
in the neighborhood of the van Hove singularity [518].Then,
the BCS approximation of N(E)
N(0) is no longer valid,so
that the actual H
p
may become larger than limit (12) [586].
We have found another reason,why the Clogston
Chandrasekhar value can be exceeded.Namely,it is the
appearance of a partial CDWdriven dielectric gap on
the d sections of the FS [427,587–589].The expected
increase of the calculated limiting paramagnetic ﬁeld H
p
for
CDW superconductors,as compared to H
BCS
p
,is intimately
associated with paramagnetic properties of the normal CDW
state,which are very similar to those for BCS swave
superconductors [382,590–592].
It should be emphasized that the very selfconsistency
of the twogap solution [386] made the treatment of the
paramagnetic limit problem [589] transparent and less
involved than previous approximations [427,587,588].
To calculate the paramagnetic limit,we considered the
relevant free energies F per unit volume for all possible
ground state phases in an external magnetic ﬁeld H.The
parent nonreconstructed phase (actually existing only above
T
d
!),withboth superconducting and CDWpairings switched
oﬀ and in the absence of H,served as a reference point.At
T < T
d
,we deal with relatively small diﬀerences δF reckoned
from this hypothetical “doublynormal” state [498].In our
case,in the ClogstonChandrasekhar spirit [581,582],there
are two energy diﬀerences to be compared [589],speciﬁcally,
that of a paramagnetic phase in the magnetic ﬁeld [593]
(diamagnetic eﬀects are not taken into account when one is
interested in the paramagnetic limit per se)
δF
p
= −
N
(
0
)
μ
∗
B
H
2
(13)
and that of a CDWsuperconducting phase
δF
s
= −
N
n
(
0
)
Δ
2
(
0
)
2
−
N
d
(
0
)
D
2
(
0
)
2
.
(14)
Here,Δ(0) is determined by (7),whereas D(0),as stems from
(8),is equal to Σ
0
=
πT
d
/γ.A simple algebra leads to the
analytical equation for the increase of the paramagnetic limit
over the ClogstonChandrasekhar value (12):
H
p
H
BCS
p
2
=
1 +μ
Σ
0
Δ
0
2/(1
−
μ)
−
1
.
(15)
This relationship is expressed in terms of genuine (bare)
systemparameters μ,Σ
0
,and Δ
0
.However,experimentalists
are interested in the dependence of H
p
/H
BCS
p
on actual
measurable quantities.The transformation of (15) can be
easily made,and one arrives at the ﬁnal formula
H
p
H
BCS
p
2
=
1 +μ
⎡
⎣
Σ(0)
Δ(0)
2
−
1
⎤
⎦
=
1 +μ
T
d
T
c
2
−
1
.
(16)
Advances in Condensed Matter Physics 13
Δ(0)/Σ(0)
=
Tc
/T
d
0
0.2
0.4
0.6
0.8
1
μ
0 0.2 0.4 0.6 0.8 1
H
p
/H
BCS
p
1.01
1.1
1.5
2
3
5
Figure 5:Contour plot of the ratio H
p
/H
BCS
p
on the plane
(T
c
/T
d
,μ).Here H
p
is the paramagnetic limit for CDWsupercon
ductors and H
BCS
p
is that for BCS spinsinglet superconductors,T
c
and T
d
are the observed critical temperatures of the superconduct
ing and CDWtransitions,respectively.(Taken from[589].)
To calculate the expected paramagnetic limit,one needs to
know μ,which was estimated,for example,as 0.2 for NbSe
3
[594] or 0.15 for La
2
−
x
Sr
x
CuO
4
[595].
The contour curves inthe parameter space obtained from
(16) are displayed in Figure 5 One can readily see that for
typical T
c
/T
d
≈
0.05–0.2 (some A15 compounds are rare
exceptions [160]) and moderate values of μ
≈
0.3–0.5,
the augmentation of the paramagnetic limit becomes very
large.There is a number of CDW superconductors [589],
where the increase of the paramagnetic limit was detected,
in accordance with the results presented here.Unfortunately,
not so much can be said about highT
c
oxides.It seems that
extremely high values of H
c2
observed in these materials are
the reason of the unjustiﬁed neglect to the problem.
4.3.DipHump Structures and Pseudogaps in Tunnel Current
Voltage Characteristics for Junctions Involving CDW Super
conductors.In Section 3,a lot of evidence was presented
concerning diphump structures (DHSs) and pseudogaps
in highT
c
oxides [81–83,160,559].Broadly speaking,
pseudogaps and DHSs have much in common.In particular,
they can coexist with superconducting coherent peaks,
their appearance in currentvoltage characteristics (CVCs)
is to some extent random,and their shapes are sample
dependent.Therefore,a suggestion inevitably arises that
those two phenomena might be governed by the same
mechanism.Our main assumption is that both pseudogaps
and diphump structures are driven by CDW instabilities
discussed above and that their varying appearances are
coupled with the intrinsic,randomly inhomogeneous elec
tronic structure of cuprates.In the strict sense,according
to the adopted scenario,both DHSs and pseudogaps are
the manifestations of the same dielectric DOS depletion,
the former being a result of superimposed CDW and
superconductivityinduced CVCfeatures belowT
c
.To justify
our approach,it is crucial that direct spatial correlations
betweenirregular patterns of CDWthreedimensional super
modulations [365] and topographic maps of the super
conducting gap amplitudes on the BSCCO surface were
displayed by tunneling spectroscopy [458].
A detailed description of our approaches to the prob
lems of tunneling through junctions with CDW isotropic
superconductors as electrodes,and the emergence of DHSs
in the CVCs of highT
c
oxides can be found elsewhere [81–
83,160,386,596].Here,we will present only a summary of
our new results,brieﬂy touching only those issues that are
necessary for the rest of the paper to be selfcontained.
We should emphasize diﬀerent roles of the order param
eter phases in determining quasiparticle tunnel currents.
Concerning the superconducting order parameter,its phase
may be arbitrary unless we are interested in the Josephson
current across the junction.On the other hand,the CDW
phase ϕ governs quasiparticle CVCs of junctions with CDW
superconductors as electrodes [556,557].The value of ϕ
can be pinned by various mechanisms in both excitonic and
Peierls insulators,so that ϕ acquires the values either 0 or
π in the ﬁrst case [522] or is arbitrary in the unpinned
state of the Peierls insulator [516].At the same time,in
the case of an inhomogeneous CDWsuperconductor,which
will be discussed below,a situation can be realized,where ϕ
values are not correlated over the junction area.Then,the
contributions of elementary tunnel currents may compen
sate one another to some extent,and this conﬁguration can
be phenomenologically described by introducing a certain
eﬀective phase ϕ
eﬀ
of the CDWorder parameter.If the spread
of the phase ϕ is random,the most probable value for ϕ
eﬀ
is π/2,and the CVC for a nonsymmetric junction involving
CDWsuperconductor becomes symmetric.
Most often,CVCs for cuprateIN (i.e.,SIN) junctions
reveal a DHS only at V
=
V
S
−
V
N
< 0 [597–599],so that
the occupied electron states belowthe Fermi level are probed
for CDWsuperconductors.In our approach,it corresponds
to the phase ϕ close to π.This preference may be associated
with some unidentiﬁed features of the CDWbehavior near
the sample surface.
On the other hand,there are SIN junctions,where
DHS structures are similar for both V polarities [347,442,
443,600].As for those pseudogap features,which were
unequivocally observed mostly at high T,no preferable V
sign of their manifestations was found.We note that the
symmetricity of the tunnel conductance G(V)
=
dJ/dV,
where J is the tunnel current through the junction,might
be due either to the microscopic advantage of the CDWstate
with ϕ
=
π/2 or to the superposition of diﬀerent current
paths in every measurement covering a spot with a linear
size of a CDW coherence length at least.Both possibilities
should be kept in mind.The variety of G(V) patterns in
the SIN setup for the same material and with identical
doping is very remarkable,showing that the tunnel current
is rather sensitive to the CDW phase ϕ.Nevertheless,the
very appearance of the superconducting domain structure
for cuprates with local domaindependent gaps and critical
14 Advances in Condensed Matter Physics
temperatures [601] seems quite plausible for materials with
small coherence lengths.Essentially the same approach has
been proposed earlier to explain superconducting properties
of magnesiumdiboride [78].
On the basis of information presented above and using
the selfconsistent solutions for Δ(T) and Σ(T),we managed
to describe the observed rich variety of G(V) patterns by
calculating quasiparticle tunnel CVCs J(V) for two typical
experimental setups.Namely,we considered SINand SI
S junctions,where “S” here means a CDWsuperconductor.
A unique tunnel resistance in the normal state R enters into
all equations,since we assume the incoherent tunneling to
occur,in accordance with the previous analysis for BSCCO
[122,602].The used Green’s function method followed the
classical approach of Larkin and Ovchinnikov [603].We skip
all (quite interesting) technical details,since they can be
found elsewhere [81–83,160,386,596].
The obtained equations for J(V) form the basis for
calculations both J(V) and G(V) (sub,superscripts ns and
s denote SIN and SIS junctions,resp.).They must be
supplemented with a proper account of the nonhomoge
neous background,since,as was several times stressed above,
STMmaps of the cuprate crystal surfaces consist of random
nanoscale patches with diﬀerent gap depths and widths,as
well as coherent edge sharpnesses.In this connection,our
theory assumes the combination CDW+ inhomogeneity to
be responsible for the appearance of the DHSs.Our main
conclusion is that it is the dispersion of the parameter Σ
0
—
and,as a result,the Dpeak smearing (the Δpeak also
becomes smeared but to a much lesser extent)—that is the
most important to reproduce experimental pictures.The
value of the FS gapping degree μ is mainly responsible for
the amplitude of the DHSs.At the same time,neither the
scattering of the parameter μ nor that of the superconducting
order parameter Δ
0
can result in the emergence of smooth
DHSs,so that sharp CDWfeatures remain unaltered.There
fore,for our purpose,it was suﬃcient to average only over
Σ
0
rather than simultaneously over all parameters of CDW
superconductors,although the variation of any individual
parameter made the resulting theoretical CVCs more similar
to experimental ones.
Although it is a wellrecognized matter of fact that CDW
driven Dsingularities in G(V) scatter more strongly for a
nonhomogeneous medium than main coherent supercon
ducting peaks at eV
= ±
Δ (SIN junctions) or
±
2Δ (SI
S junctions),this phenomenon has not yet been explained.
It seems that the sensitivity of the Peierls [604,605]
or excitonicinsulator [431,606] order parameters to the
Coulomb potential of the impurities,for example,oxygen
ions,might be the reason of such a dispersion.On the other
hand,swave superconductivity is robust against impurity
inﬂuence (Anderson theorem[607–609]).As for anisotropic
superconductivity with dwave or other kinds of symmetry,
they are suppressed by nonmagnetic impurity scattering
[3,554,610,611] due to scatteringinduced order parameter
isotropization.Their survival in disordered cuprate samples,
especially in the context of the severe damage inﬂicted by
impurities on the pseudogap,testiﬁes that the Cooperpair
order parameter includes a substantial isotropic component.
The parameter Σ
0
was assumed to be distributed within
the interval [Σ
0
−
δΣ
0
,Σ
0
+ δΣ
0
].The normalized weight
function W(x) was considered as a bellshaped fourthorder
polynomial within this interval and equal to zero beyond it
(see the discussions in [81]).In any case,the speciﬁc formof
W(x) is not crucial for the ﬁnal results and conclusions.
Our approach is in essence the BCSlike one.It means,
in particular,that we do not take a possible quasiparticle
“dressing” by impurity scattering and the electronboson
interaction,as well as the feedback inﬂuence of the super
conducting gapping,into account [612,613].Those eﬀects,
important per se,cannot qualitatively change the random
twogap character of superconductivity in cuprates.
As was already mentioned,we have assumed so far that
both Δ and Σ are swaveorder parameters.Nevertheless,
our approach to CVC calculations is qualitatively applicable
to superconductors with the dwave symmetry,if not to
consider the intragap voltage range

eV

< Δ.
The results of calculations presented below show that
the same CDW + inhomogeneity combination can explain
DHSs at low T as well as the pseudogap phenomena at
high T,when the DHS is smoothed out.Thus,theoretical
Tdependences of tunnel CVCs mimic the details of the
DHS transformation into the pseudogap DOS depletion for
nonsymmetric and symmetric junctions,involving cuprate
electrodes.We consider the CDWdriven phenomena,DHS
included,as the tip of an iceberg,a huge underwater part of
which is hidden by strong superconducting manifestations,
less inﬂuenced by randomness than their CDWcounterpart.
To uncover this part,one should raise T,which is usually
done with no reference to the DHS,the latter being sub
stantially smeared by the Fermidistribution thermal factor.
It is this DOS depletion phenomenon that is connected to the
pseudogapping phenomena [14,18,334,348,399,441].
The results of calculations of G
ns
(V) in the case when
parameter Σ
0
is assumed to scatter are shown in Figure 6
for ϕ
=
π.The value ϕ
=
π was selected,because this case
corresponds to the availability of the DHS in the negative
voltage branch of the nonsymmetric CVC,and such an
arrangement is observed in the majority of experimental
data.In accordance with our basic equations,all the four
existing CVC peculiarities at eV
= ±
Δ and
±
D become
smeared,although to various extent:the large singularities
at eV
= ±
Δ almost preserve their shape,the large singularity
at eV
= −
D transforms into a DHS,and the small one at
eV
=
D disappears on the scale selected.The onepolarity
diphump peculiarity in experimental CVCs for BSCCO
[597] is reproduced excellently.Owing to relationship (7),
the actual parameter Δ also disperses,but,due to the
small value of μ,this ﬂuctuation becomes too small to be
observed in the plot.Thus,the calculated CVCs of Figure 6
demonstrate all principal features intrinsic to the tunnel
conductivity of SIN junctions at low T,involving CDW
superconductors,speciﬁcally,asymmetry with respect to the
V sign is associated with the phase ϕ
/
=
π/2 of the CDW
order parameter,the emerging CDW induces singularities
at eV
= ±
D,whereas the intrinsic CDW inhomogeneity
transforms the major one into a DHS,totally suppressing the
minor.
Advances in Condensed Matter Physics 15
RdJ/dV
0
0.5
1
1.5
2
eV (meV)
−
100
−
50 0 50 100
δΣ
∗
0
=
10meV
δΣ
∗
0
=
20meV
δΣ
∗
0
=
29meV
Figure 6:(Color online) Bias voltage,V,dependences of the
dimensionless diﬀerential conductance RG(V)
=
RdJ/dV for the
tunnel junction between an inhomogeneous CDWsuperconductor
and a normal metal,expressed in energy units.Here,J is the
quasiparticle tunnel current,R is the resistance of the junction
in the normal state,and e > 0 is the elementary charge.The
bare parameters of the CDW superconductor are Δ
∗
0
=
20meV,
Σ
∗
0
=
50meV,and μ
=
0.1;the temperature T
=
4.2K.Various
dispersions δΣ
∗
0
centered around the mean value Σ
∗
0
=
50meV.
(Taken from[81].)
An example of the transformation,with T,of the
DHSdecorated tunnel spectra into the typical pseudogap
like ones is shown in Figure 7 for SIN junctions with
ϕ
=
π (panel (a)) and π/2 (panel (b)).The CDW
superconductor parameters are Δ
0
=
20meV,Σ
0
=
50meV,
μ
=
0.1,and δΣ
0
=
20meV;the temperature T
=
4.2K.For this parameter set,the “actual” superconducting
critical temperatures T
c
of random domains lie within the
interval of 114–126 K,and T
d
is in the range of 197–
461 K.From Figure 7(a),the transformation of the DHS
including pattern of the CVCs calculated for T
T
c
into the pseudogaplike ones in the vicinity of T
c
or above
it becomes clear.The asymmetric curves displayed in (a)
are similar to the measured STM G
ns
(V) dependences for
overdoped and underdoped BSCCO compositions [441].
The overall asymmetric slope of the experimental curves,
which is independent of gaps and T,constitutes the main
distinction between them and our theoretical results.It
might be connected to the surface charge carrier depletion
induced by CDWs and mentioned above.Another interesting
feature of our results is a modiﬁcation and a shift of the Δ
peak.Although Δ diminishes as T grows,the Δpeak moves
toward higher bias voltages;such a behavior of the Δpeak
is to be undoubtedly associated with its closeness to the Σ
governed DHS.In experiments,a confusion of identifying
this Δdriven singularity with a pseudogap feature may arise,
since the observed transformation of Δfeatures into Dones
looks very smooth [348].
It is notable that in the case of asymmetric G
ns
(V),
the lowT asymmetry preserves well into the normal
state,although the DHS as such totally disappears.The
extent of the sample randomness substantially governs
CVC patterns.Therefore,pseudogap features might be less
or more pronounced for the same materials and doping
levels.At the same time,for the reasonable spread of the
problem parameters,the superconducting coherent peaks
always survive the averaging (below T
c
,of course),in
accordance with experiment.Our results also demonstrate
that the dependences Δ(T) taken from the tunnel data
may be somewhat distorted in comparison to the true
ones due to the unavoidable Δ versus Σ interplay.One
should stress that in our model,“hump” positions,which
are determined mainly by Σ rather than by Δ,anticorrelate
with true superconducting gap values Δ inferred from the
coherent peaks of G(V).It is exactly what was found for
nonhomogeneous BSCCOsamples [614].
Similar CDWrelated features should be observed in the
CVCs measured for symmetric SIS junctions.The G
s
(V)
dependences for this case with the same sets of parameters as
in Figure 7 are shown in Figure 8.In analogy with symmetric
junctions between BCS superconductors,one would expect
an appearance of singularities at eV
= ±
2Δ,
±
(D + Δ),and
±
2D.Such,indeed,is the case.However,the magnitudes of
the features are quite diﬀerent (the details of the analysis can
be found in [81,83]).As readily seen,the transformation
of the symmetric DHS pattern into the pseudogaplike
picture is similar to that for the nonsymmetric junction.This
simplicity is caused by a smallness of the parameter μ
=
0.1,
so that the features at eV
= ±
2D,which are proportional to
μ
2
,are inconspicuous on the chosen scale.At the same time,
the singularities at eV
= ±
(D+Δ) are of the squareroot type.
Note that for arbitrary Σ and Δmagnitudes,those energies
do not coincide with the values
±
(Σ+Δ) (in more frequently
used notation,
±
(Δ
PG
+ Δ
SG
)),which can be sometimes met
in literature [615].The later relation becomes valid only for
Σ
Δ.
The appearance of the Tdriven zerobias peaks is a
salient feature of certain CVCs displayed in Figure 8.As
is well known [603],this peak is caused by tunneling
of thermally excited quasiparticles between empty states
with an enhanced DOS located above and below equal
superconducting gaps in symmetric SIS junctions.Such a
feature was found,for example,in G
s
(V) measured for grain
boundary symmetric tunnel junctions in epitaxial ﬁlms of
the swave oxide CDWS Ba
1
−
x
K
x
BiO
3
[616].One should be
careful not to confuse this peak with the dc Josephson peak
restricted to V
=
0,which is often seen for symmetric high
T
c
junctions [399].The distinction consists in the growth of
the quasiparticle zerobias maximumwith increasing T up to
a certain temperature,followed by its drastic reduction.On
the other hand,the Josephson peak decreases monotonously
as T
→
T
c
.
The proﬁle and the behavior of the zerobias peak
at nonzero T can be explained in our case by the fact
that,in eﬀect,owing to the nonhomogeneity of electrodes,
16 Advances in Condensed Matter Physics
RdJ/dV
0
0.5
1
1.5
2
eV (meV)
−
100
−
50 0 50 100
T
=
4.2K
T
=
30K
T
=
77.8K
T
=
120K
T
=
300K
(a)
RdJ/dV
0
0.5
1
1.5
2
eV (meV)
−
100
−
50 0 50 100
T
=
4.2K
T
=
30K
T
=
77.8K
T
=
120K
T
=
300K
(b)
dI/dV(GΩ−1)
0.5
1
1.5
V
sample
(mV)
−
200
−
100 0 100 200
4.2K
46.4K
63.3K
76K
80.9K
84K
88.9K
98.4K
109K
123K
151K
166.6K
175K
182K
194.8K
202.2K
293.2K
T
c
=
83K
(c)
Figure 7:G(V) dependences for the tunnel junction between an inhomogeneous CDWS and a normal metal for various temperatures T.
The CDWorder parameter phase ϕ
=
π (a) and π/2 (b),and the spread of the CDWorder parameteramplitude δΣ
∗
0
=
20meV.All other
parameters are indicated in the text.(c) STMspectra for underdoped BSCCOIr junctions registered at various temperatures.(Reprinted
from[598],taken from[83].)
the junction is a combination of a large number of symmetric
and nonsymmetric junctions with varying gap parameters.
The former compose a mutual contribution to the current
in the vicinity of the V
=
0 point,and the width of this
contribution along the Vaxis is governed by temperature
alone.On the other hand,every junction from the latter
group gives rise to an elementary current peak in the
CVC at a voltage equal to the relevant gap diﬀerence.All
such elementary contributions formsomething like a hump
around the zerobias point,and the width of this hump along
the Vaxis is governed by the sumof actual—dependent on
the zeroT values and on the temperature itself—gap spreads
in both electrodes.It is clear that the T behavior of the
current contribution of either group is rather complicated,
to say nothing of their combination.
From our CVCs calculated for both nonsymmetric
(Figures 6 and 7) and symmetric (Figure 8) junctions,it
comes about that the “dip” is simply a depression between
the hump,which is mainly of the CDW origin,and the
superconducting coherent peak.Therefore,as has been noted
in [617],the dip has no separate physical meaning.It
disappears as T increases,because the coherent peak forming
Advances in Condensed Matter Physics 17
RdJ/dV
0
0.5
1
5
10
15
eV (meV)
−
100
−
50 0 50 100
T
=
4.2K
T
=
70K
T
=
100K
T
=
115K
T
=
118K
T
=
120K
T
=
160K
(a)
Bi
2
Sr
2
CaCu
2
O
8+δ
dI/dV(a.u.)
dI/dV(ms)
1
1.5
2
2.5
3
3.5
4
4.5
Voltage (mV)
−
400
−
300
−
200
−
100 0 100 200 300 400
129.2
121.2
110.3
107
105.2
103.2
101
99.1
97.1
95.1
93
91
89
87.1
86.1
85
83.1
81.2
79.2
77.3
T (K)
(b)
Figure 8:(a) The same as in Figure 7(a),but for a symmetric junction between similar CDWsuperconductors.(b) Temperature variations
of experimental diﬀerential currentvoltage characteristics (CVCs) for a Bi
2
Sr
2
CaCu
2
O
8+δ
break junction.(Reprinted from[399],taken from
[83].)
the other shoulder of the dip fades down,so that the former
dip,by expanding to the V
=
0 point,becomes an integral
constituent of the shallow pseudogap minimum.
Therefore,it became clear that the CDWmanifestations
against the nonhomogeneous background can explain both
subtle DHS structures in the tunnel spectra for highT
c
oxides and large pseudogap features observed both below
and above T
c
.The DHS is gradually transformed into the
pseudogaplike DOS,lowering as T grows.Hence,both
phenomena are closely interrelated,being in essence the
manifestations of the same CDWgoverned feature smeared
by inhomogeneity of CDW superconductors.Therefore,
the DHS and pseudogap features should not be treated
separately.The dependences of the calculated CVCs on the
CDWphase ϕ fairly well describe the variety of asymmetry
manifestations in the measured tunnel spectra for BSCCO
and related compounds.
4.4.Coexistence of CDWs and dWave Superconductivity.We
recognize that some of our results,which were obtained
assuming that the superconducting order parameter coexist
ing with CDWs is isotropic,might be applicable to cuprates
with certain reservations,since a large body of evidence in
favor of d
x
2
−
y
2
symmetry in highT
c
oxides [131,132,305,
306,618,619] is available,although there are experimentally
based objections [109,116–129].In any case,it seems
instructive to extend the partial dielectrization approach to
dwave Cooper pairing.For simplicity,we argue in terms
of twodimensional ﬁrst Brillouin zone and Fermi surface,
neglecting caxis quasiparticle dispersion,which should be
taken into account,in principle [620].Since the dielectric,
Σ,and superconducting,dwave Δ,order parameters have
diﬀerent momentumdependences,their joint presence inthe
electron spectrum is no longer reduced to a combined gap
(4),as it was for isotropic superconductivity.
In the dwave case,superconductivity is described by
a weakcoupling model with a Hamiltonian given,for
example,in [553,621].In accordance with photoemission
[371,622–624] and STM [359,368,370,506,507,512,
625] data (see Figure 1),the meanﬁeld CDWHamiltonian
is restricted to momenta near ﬂatband regions,antinodal
from the viewpoint of the fourlobe dwave gapfunction
Δ(T) cos 2θ [306].In those regions,the nesting conditions
(1) between pairs of mutually coupled quasiparticle branches
are fulﬁlled.For instance,static CDW wave vectors Q
=
(
±
2π/4.2a
0
,0) and (0,
±
2π/4.2a
0
)—with an accuracy of
15%—in Bi
2
Sr
2
CaCu
2
O
8+δ
are revealed in STM studies
[359].Thus,we characterize a CDW checkerboard state
(symmetric with respect to π/2 rotations) by four sectors
in the momentum space centered with the lobes and with
an opening 2α each (α < π/4).It should be noted that
vectors Q depend on doping,which was explicitly shown
18 Advances in Condensed Matter Physics
1
0.8
0.6
0.4
0.2
0
0.2
0.4
0.6
0.8
1
2α
0
30
60
90
120
150
180
210
240
270
300
330
Figure 9:(Color online) Orderparameter maps for a conventional
dwave superconductor (Δ,solid curve) and a partially gapped
CDWmetal (Σ,dashed curve).
for Bi
2
Sr
2
CuO
6+δ
[343].The dielectric (CDWinduced)
order parameter is Σ(T) inside the 2αcones,being angle
independent here,and zero outside (see Figure 9).
The plausibility of this scenario is supported—at least
partially—by recent STM studies of intrinsically inhomo
geneous BSCCO samples [626].Speciﬁcally,the authors
analyzed the composition,temperature,and angular depen
dences of the gaps on various FS sections and showed
that nodal superconducting gaps for overdoped specimens
exhibit more or less conventional dwave behavior,whereas
in underdoped samples nodal (superconducting) and anti
nodal gaps (CDWgaps,as is assumed here) superimpose on
one another in tunnel spectra.It is important that for under
doped compositions antinodal gaps do not change drastically
with T,when crossing T
c
.The conclusion made in [626]
that the entire FS contributes to bulk superconductivity in
overdoped samples corresponds—if proved to be correct—to
the actual shrinkage of nested FS sections,that is,to μ
→
0.
We obtained a new set of DysonGor’kov equations
for normal and superconducting Green’s functions for the
system with electronhole of whatever nature and dwave
Cooper pairings,which were solved in the same straightfor
ward manner as in the swave case [160,386] (see above).We
arrived at the systemof two coupled equations for Δ(T) and
Σ(T):
μπ/4
0
I
M
Σ
2
+Δ
2
cos
2
2θ,T,Σ
0
dθ
=
0,(17)
μπ/4
0
I
M
Σ
2
+Δ
2
cos
2
2θ,T,Δ
0
cos
2
2θ dθ
+
π/4
μπ/4
I
M
(
Δcos 2θ,T,Δ
0
)
cos
2
2θ dθ
=
0,
(18)
where μ
=
4α/π is the dielectrically gapped portion of the FS
for the speciﬁc model of partial gapping,shown in Figure 9,
and I
M
(Δcos 2θ,T,Δ
0
) is the M
¨
uhlschlegel integral (6).The
analysis of the generic T
−
δ phase diagramfor cuprates shows
that both Σ
0
and μ reduce with doping,whereas the holelike
FS pockets centered at the (π/a
0
,π/a
0
) point of the Brillouin
zone shrink for every speciﬁc highT
c
oxide (see,e.g.,[343]).
On the other hand,in the absence of CDWgapping,(18)
becomes a dwave gap equation:
π/4
0
I
M
(
Δcos 2θ,T,Δ
0
)
cos
2
2θ dθ
=
0,
(19)
the solution of which Δ
=
dM
¨
u(Δ
0
,T) is known [553,
621].In particular,the critical temperature is T
c0
=
(2Ωγ/π) exp[
−
1/V
BCS
N(0)],as in the swave case.From
(19),it follows that in agreement with [553],(Δ
0
/T
c0
)
d
=
(2/
√
e)(π/γ),revealing a modiﬁed “dwave” BCSratio dif
ferent fromthe spairing value
Δ
0
T
c0
s
=
π
γ
≈
0.824
Δ
0
T
c0
d
.
(20)
Here,e is the base of natural logarithm.It is evident that
our model takes into account manybody correlations both
explicitly (the emergence of two pairings) and implicitly (via
the renormalization of the parameters Σ
0
and μ).Weak
coupling values of the ratio Δ
0
/T
c0
for other anisotropic
order parameter symmetries do not diﬀer much from the
value of (Δ
0
/T
c0
)
d
[627,628].
Due to the diﬀerent order parameter symmetry,readily
seen from (17) and (18),the situation is mathematically
more involved than for isotropic CDW superconductors,
where a simple relationship (4) takes place.This was not
recognized in a recent work [629],where the opposite
wrong statement was made.Prima facie subtle mathematical
diﬀerences between descriptions of swave and dwave CDW
superconductors lead to conspicuous physical consequences.
Indeed,the numerical dependences Δ(T) and Σ(T) found
from (17) and (18) and shown in Figure 10 diﬀer qualita
tively from their counterparts Δ
s
(T) and Σ
s
(T) in a certain
range of model parameters.(In this subsection,we do not
introduce a natural subscript “d” for brevity.) Figure 10 (a)
demonstrates that a reduction of the bare parameter Σ
0
,
keeping Δ
0
and μ constant,resulting in the transformation
of Σ(T) with a cusp at T
=
T
c
and a concave region at T < T
c
(the behavior appropriate for CDW ssuperconductors in
the whole allowable parameter range,as is demonstrated in
Figure 3) into curves describing a novel peculiar reentrant
CDWstate.It is remarkable that the reentrance found by us
is appropriate to an extremely simple basic model with two
competing order parameters.At the same time,the CDW
structures in real systems may be much more complicated
with nonmonotonic Tdependencies even in the absence of
superconductivity [352].
Let us formulate conditions necessary to observe this
crossover.First,(20) means that Δ(T)/Δ
0
for conventional
dsuperconductors is steeper than (Δ(T)/Δ
0
)
s
.In our case,it
means that Δ(T)/Δ
0
,when the CDW disappears,is steeper
than Σ(T)/Σ
0
in the absence of superconductivity,which
is described by (6).Hence,for the CDW phase to exist
(the upper critical temperature T
u
CDW
> 0),it should be
T
u
CDW
=
(γ/π)Σ
0
> T
c0
=
(
√
eγ/2π)Δ
0
.As a consequence,the
ﬁrst constraint on the model parameters should be fulﬁlled:
Σ
0
> (
√
e/2)Δ
0
≈
0.824Δ
0
.The constraint stems from the
competition between emerging Δ and Σ on the d FS section
only.The actual coexistence between superconductivity and
Advances in Condensed Matter Physics 19
Σ/Δ0
0
0.5
1
1.5
T/Δ
0
0 0.2 0.4 0.6 0.8
1
2
3
4
5
6
(a)
Δ/Δ0
0
0.5
1
T/Δ
0
0 0.2 0.4
2
1
3
4
5
6
7
(b)
Figure 10:(Color online) Temperature,T,dependences of the normalized (a) CDWΣ and (b) superconducting Δ gap functions.Δ
0
equal
to Δ(T
=
0) when CDWs are absent is 1.The values of Σ
0
/Δ
0
equal to Σ(T
=
0)/Δ
0
in the absence of superconductivity are 1.5 (1),1.2 (2),1
(3),0.95 (4),0.9 (5),0.85 (6),and 0.8 (7);μ
=
0.3.
CDWs was not involved in these reasonings,so the inequality
does not include the control parameter μ.Therefore,T
u
CDW
thus deﬁned coincides with T
CDW0
.
Second,below the lower critical temperature of the
CDWreentrance region,T
l
CDW
,if any,(18) deﬁnes Δ(T)
=
dM
¨
u(Δ
0
,T),and we should use (17) with T
=
T
l
CDW
and
Δ(T
l
CDW
)
=
dM
¨
u(Δ
0
,T
l
CDW
) to determine T
l
CDW
(Δ
0
,Σ
0
,μ)
numerically.The crossover value of Σ
cr
0
,when T
l
CDW
=
0,corresponds to the separatrix on the order parameter
T plane,dividing possible Σ(T)curves (see Figure 10(a))
into two types:reentrant and nonreentrant.However,(17)
brings about Σ
cr
0
=
Δ
0
exp[(4/μπ)
μπ/4
0
ln(cos 2θ)dθ].To
observe the reentrant behavior,the second constraint should
be Σ < Σ
cr
0
.For the curves in Figure 10,μ
=
0.3 was
chosen,so that we obtain the reentrance range 0.824Δ
0
<
Σ
0
< 0.963Δ
0
,which agrees with numerical solutions of the
full selfconsistent equation set.We emphasize that CDWs
survives the competition with dwave superconductivity
even at Σ
0
/Δ
0
< 1,which is not the case for stronger isotropic
Cooper pairing (see the discussions above).
In Figure 10(b),the concomitant Δ(T) dependences are
depicted.One sees how dwave superconductivity,sup
pressed at large Σ
0
,recovers in the reentrance parameter
region.Therefore,two regimes of CDW manifestation can
be observed in superconductors.In both cases,the CDWis
seen as a pseudogap above T
c
[81,83] in photoemission and
tunnel experiments.However,the corresponding DHS at low
T may either be observed or not,depending on whether the
reentrance occurs.This might be an additional test for an
anisotropic (not necessarily d
x
2
−
y
2
wave) Cooper pairing to
dominate in cuprates.
To control the changeover between diﬀerent regimes in
cuprates,one can use either hydrostatic pressure or doping.
In both cases,μ is the main varying parameter.In Figure 11,
the curves Σ(T) and Δ(T) are shownfor Σ
0
/Δ
0
=
0.9 and var
ious μ.It is readily seen how drastic is the lowT depression
of Σ by superconductivity,when the dielectrically gapped FS
sectors are small enough.Doping Bi
2
Sr
2
CaCu
2
O
8+δ
[403]
and (Bi,Pb)
2
(Sr,La)
2
CuO
6+δ
[356] with oxygen was shown
to sharply shrink the parameter μ.Note that the Δ(T)
dependences are distorted by CDWs,and they do not
coincide with the scaled “parent” curve—dM
¨
u(T),in this
case—in contrast to what should be observed for CDW
ssuperconductors (Figure 3).Therefore,various observed
forms of Δ(T) per se cannot unambiguously testify to
the superconducting pairing symmetry.Moreover,cuprate
superconductivity might be,for example,a mixture of s and
dwave contributions [130,630].
It is evident that diﬀerent strengths of CDWimposed
suppression of the superconducting energy gap in the
electron spectrum Δ and the critical temperature T
c
must
change the ratio Δ(0)/T
c
—the benchmark of weakcoupling
superconductivity (see (20)).If one recalls that,as was shown
above,this ratio in CDW ssuperconductors remains the
same as in conventional sones,the situation becomes very
intriguing.In Figure 12(a),the dependences of 2Δ(0)/T
c
and T
c
/Δ
0
ratios on Σ
0
/Δ
0
are displayed.One sees that
2Δ(0)/T
c
sharply increases with Σ
0
/Δ
0
for Σ
0
/Δ
0
≤
1 and
swiftly saturates for larger Σ
0
/Δ
0
,whereas T
c
/Δ
0
decreases
almost evenly.The saturation value proves to be 5.2 for
μ
=
0.3.We stress that such large enhancement of 2Δ(0)/T
c
agrees well with experimental data [441,478,631,632] for
cuprates and cannot be achieved taking into account strong
coupling electronboson interaction eﬀects for reasonable
relationships between T
c
and eﬀective boson frequencies ω
E
[633,634] (one can hardly accept,e.g.,the value T
c
/ω
E
≈
0.3 [634] as practically meaningful).Furthermore,the
destruction of the alternatingsign superconducting order
20 Advances in Condensed Matter Physics
Σ/Δ0
0
0.5
1
T/Δ
0
0 0.2 0.4
4
3
2 1
(a)
Δ/Δ0
0
0.5
1
T/Δ
0
0 0.2 0.4
1234
(b)
Figure 11:(Color online) The same as in Figure 10 but for Σ
0
/Δ
0
=
0.9 and μ
=
0.1 (1),0.3 (2),0.5 (3),0.6 (4).
parameter by impurity scattering approximated by collective
boson modes also could not explain [635] high values of
2Δ(0)/T
c
,for example,inherent to underdoped BSCCO
[347,597].Therefore,our weakcoupling model is suﬃcient
to explain—on its own—the large magnitude of 2Δ(0)/T
c
in
cuprates,possible strongcoupling eﬀects resulting in at most
minor corrections.
Another possible alternative reason of high 2Δ(0)/T
c
ratios might be a singular energy dependence of the normal
state electron DOS near the FS,for instance,near the Van
Hove anomalies in lowdimensional electron subsystems
[518].It turned out,however,that,at least in the weak
coupling (BCS) approximation for swave Cooper pairing,
the ratio 2Δ(0)/T
c
is not noticeably altered [636,637].
Moreover,calculations in the framework of the strong
coupling Eliashberg theory [10] showed that the van Hove
singularity inﬂuence on T
c
is even smaller than in the BCS
limit [638].Furthermore,weakcoupling calculations for
orthorhombically distorted holedoped cuprate supercon
ductors (without CDWs) demonstrated that 2Δ(0)/T
c
can
be estimated as an intermediate between swave and d
wave limits [639],being smaller than needed to explain the
experiment.It means that our approach remains so far the
only one capable of explaining high 2Δ(0)/T
c
≈
5
÷
8 (and
even larger values [632]) for cuprates.We emphasize that it
is very important to reconcile theoretical values for 2Δ(0)/T
c
as well as ΔC/γ
S
T
c
with experimental ones.Otherwise,
the microscopic theory becomes “too” phenomenological
with Δ/T
c
as an additional free parameter of the system
[640].
It is instructive from the methodological point of view
to mention a previous unsuccessful attempt to explain
the increase of 2Δ(0)/T
c
by a pseudogap inﬂuence [641].
The authors of this reference assumed the identical d
wave symmetry for both the superconducting,Δ(T),and
temperatureindependent pseudogap,E
PG
,order parame
ters.Additionally,dielectric gapping was supposed to be
eﬀectively complete rather than partial,the latter being
intrinsic to our model and follows from the experiments
for cuprates.These circumstances excluded selfconsistency
from the approach and led to superﬂuous restrictions
imposed on E
PG
,namely,E
PG
0.53Δ
0
(T
=
0),where
Δ
0
(T
=
0) is the parent superconducting order parameter
amplitude.At the same time,it is well known that for existing
CDWsuperconductors the strength of CDWinstability is at
least not weaker than that of its Cooperpairing counterpart
[160].We should emphasize once more that the main
peculiarity of our model,dictated by the observations,which
led to the adequate description of thermodynamic properties
for dwave superconductors with CDWs,is the distinction
between relevant order parameter symmetries.
The μdependences of 2Δ(0)/T
c
and T
c
/Δ
0
are shown in
Figure 12(b).They illustrate that 2Δ(0)/T
c
can reach rather
large values,if the dielectric gapping sector is wide enough.
This growth is however limited by a drastic drop of T
c
leading to a quick disappearance of superconductivity.We
think that it is exactly the case of underdoped cuprates,
when a decrease of T
c
is accompanied by a conspicuous
widening of the superconducting gap.For instance,such a
scenario was clearly observed in breakjunction experiments
for Bi
2
Sr
2
CaCu
2
O
8+δ
samples with a large doping range
[642].
As was pointed out in [478],various photoemission and
tunneling measurements for diﬀerent cuprate families show
a typical average value 2Δ(0)/T
c
≈
5.5.From Figure 12(b),
we see that this ratio corresponds to μ
≈
0.35 at Σ
0
/Δ
0
=
1.
The other curve readily gives T
c
/Δ
0
≈
0.35.Since Δ
0
/T
c0
≈
2.14 for a dwave superconductor (see above),we obtain
T
c
/T
c0
≈
0.75,being quite a reasonable estimation of T
c

reduction by CDWs.
Advances in Condensed Matter Physics 21
2Δ(0)/Tc
4
dBCS
4.5
5
Σ
0
/Δ
0
0.8 1 1.2 1.4 1.6
Tc/Δ0
0.2
0.3
0.4
0.5
(a)
2Δ(0)/Tc
4
dBCS
5
6
7
8
μ
0 0.2 0.4 0.6
Tc/Δ0
0.1
0.2
0.3
0.4
(b)
Figure 12:(Color online) Dependences of 2Δ(0)/T
c
(squares) and T
c
/Δ
0
(circles) on Σ
0
/Δ
0
(panel (a),μ
=
0.3) and μ (panel (b),Δ
0
/Σ
0
=
1).
T
c
is the superconducting critical temperature,d
−
BCS
≈
4.28 is a value for a conventional superconductor with dwave symmetry of the
order parameter.
4.5.SDWs and Superconductivity.There are plenty of materi
als,where SDWs compete with superconductivity,although
a simultaneous existence of the order parameters cannot be
always proved [160,643,644].For completeness,we give here
certain short comments on the latest developments in this
direction.
During the last years,an interest arose to the phase
with the hidden order parameter in URu
2
Si
2
,emerging at
about 17.5K and being some kind of SDWs,coexisting
with superconductivity at T < 1.5K [153,645–647].It
should be noted that the partial gapping idea applied to
SDW materials [397,422–424,566,648–650] was invoked
to explain ordering in this compound at the times of the
discovery [651].
More attentionwas paid to Cr andits alloys,where CDWs
and SDWs are linked and coexist [652,653].It might be
interesting to observe mutual inﬂuence of CDWs and SDWs
on superconductivity [654–657].
The problem of an interplay between SDWs and super
conductivity received strong impetus recently,especially
because of the fundamental discovery of magnetic element
based highT
c
pnictide superconductors [49,654–657].
Theoretical eﬀorts were also continued (see,e.g.,[658–
662]).It is worthwhile noting that,for certain doping
ranges,superconducting cuprates also demonstrate [663] the
coexistence of Cooper pairing with SDWs rather than CDWs,
the latter being appropriate for the majority of highT
c
oxide
compositions (see above and [160]).
Although the coexistence of superconductivity with
SDWs or more exotic orbital antiferromagnetic and spin
current ordering [522,548,664] is left beyond the scope of
this review,the relevant physics is not less fascinating than
that of their CDWinvolving analogues.
5.Conclusions
The presented material testiﬁes that CDWs play the impor
tant role in highT
c
oxides and govern some of the properties
that usually have been considered as solely determined
by superconductivity per se.Sometimes CDWs manifest
themselves explicitly (observed checkerboard or unidirec
tional structures,DHSs,psedudogaps) but,in the majority
of phenomena,they “only”—but often drastically—change
the magnitude of certain eﬀects in the superconducting
state (the heat capacity anomaly,the paramagnetic limit,
the Tdependence of H
c2
,the Δ(0)/T
c
ratio).Cuprates
are not unique as materials with coexisting CDWs and
superconductivity,but the scale of the interplay is very large
here due to the strength of the Cooper pairing in those
compounds.
Acknowledgments
The authors are grateful to Antonio Bianconi,Sergei
Borisenko,Ilya Eremin,Peter Fulde,Stefan Kirchner,Alexan
der Kordyuk,Dirk Manske,and Kurt Scharnberg for useful
discussions.A.M.Gabovich and A.I.Voitenko are also
grateful to Kasa im.J
´
ozefa Mianowskiego,Polski Koncern
Naftowy ORLEN,and Fundacja Zygmunta Zaleskiego as well
as to project no.23 of the 2009–2011 Scientiﬁc Cooperation
Agreement between Poland and Ukraine for the ﬁnancial
support of their visits to Warsaw.A.M.Gabovich highly
appreciates the 2008 and 2009 Visitors Programs of the Max
Planck Institute for the Physics of Complex Systems (Dres
den,Germany).T.Ekino was partly supported by a Grant
inAid for Scientiﬁc Research (nos.19540370,19105006,
19014016) of Japan Society of Promotion of Science.M.S.Li
22 Advances in Condensed Matter Physics
was supported by the Ministry of Science and Informatics in
Poland (grant no.202204234).
References
[1] J.G.Bednorz and K.A.M
¨
uller,“Possible high T
c
supercon
ductivity in the BaLaCuOsystem,” Zeitschrift f
¨
ur Physik B,
vol.64,no.2,pp.189–193,1986.
[2] P.W.Anderson,The Theory of Superconductivity in the High
T
c
Cuprates,Princeton Univeristy Press,Princeton,NJ,USA,
1997.
[3] V.P.Mineev and K.V.Samokhin,Intoduction to Uncon
ventional Superconductivity,Gordon and Breach Science,
Amsterdam,The Netherlands,1999.
[4] M.L.Kuli
´
c,“Interplay of electronphonon interaction and
strong correlations:the possible way to hightemperature
superconductivity,” Physics Reports,vol.338,no.12,pp.1–
264,2000.
[5] S.L.Drechsler,H.Rosner,J.M
´
alek,and H.Eschrig,“Elec
tronic and magnetic properties of cuprate chains and related
materials.From bandstructure to aspects of manybody
physics in real materials,” in HighT
c
Superconductors and
Related Materials.Material Science,Fundamental Properties,
and Some Future Electronic Applications,S.L.Drechsler
and T.Mishonov,Eds.,p.81,Kluwer Academic Publishers,
Dordrecht,The Netherlands,2001.
[6] N.M.Plakida,Spectroscopy of HighT
c
Superconductors:A
Theoretical View,Taylor and Francis,New York,NY,USA,
2003.
[7] Y.Yanase,T.Jujo,T.Nomura,H.Ikeda,T.Hotta,and K.
Yamada,“Theory of superconductivity in strongly correlated
electron systems,” Physics Reports,vol.387,no.1–4,pp.1–
149,2003.
[8] A.S.Alexandrov,Theory of Superconductivity:From Weak to
Strong Coupling,IOP,Philadelphia,Pa,USA,2003.
[9] L.Pitaevskii,“Theoretical foundation:phenomenology and
microscopic theory,” in The Physics of Superconductors.
Vol.1:Conventional and HighT
c
Superconductors,K.H.
Bennemann and J.B.Ketterson,Eds.,p.23,Springer,Berlin,
Germany,2003.
[10] J.P.Carbotte and F.Marsiglio,“Electronphonon supercon
ductivity,” in The Physics of Superconductors.Vol.1:Conven
tional and HighT
c
Superconductors,K.H.Bennemann and J.
B.Ketterson,Eds.,p.233,Springer,Berlin,Germany,2003.
[11] A.V.Chubukov,D.Pines,and J.Schmalian,“A spin
ﬂuctuation model for dwave superconductivity,” in The
Physics of Superconductors.Vol.1:Conventional and HighT
c
Superconductors,K.H.Bennemann and J.B.Ketterson,Eds.,
p.495,Springer,Berlin,Germany,2003.
[12] S.A.Kivelson,I.P.Bindloss,E.Fradkin,et al.,“How to
detect ﬂuctuating stripes in the hightemperature supercon
ductors,” Reviews of Modern Physics,vol.75,no.4,pp.1201–
1241,2003.
[13] D.Manske,Theory of Unconventional Superconductors.
CooperPairing Mediated by Spin Excitations,Springer,New
York,NY,USA,2004.
[14] E.W.Carlson,V.J.Emery,S.A.Kivelson,and D.Orgad,
“Concepts in high temperature superconductivity,” in The
Physics of Superconductors.Vol.2:Conventional and HighT
c
Superconductors,K.H.Bennemann and J.B.Ketterson,Eds.,
p.275,Springer,Berlin,Germany,2004.
[15] D.Manske,I.Eremin,and K.H.Bennemann,“Elec
tronic theory for superconductivity in highT
c
cuprates and
Sr
2
RuO
4
,” in The Physics of Superconductors.Vol.2:Conven
tional and HighT
c
Superconductors,K.H.Bennemann and J.
B.Ketterson,Eds.,p.731,Springer,Berlin,Germany,2004.
[16] A.J.Leggett,“Superﬂuid
3
He and the cuprate superconduc
tors,” in The Physics of Superconductors.Vol.2:Conventional
and HighT
c
Superconductors,K.H.Bennemann and J.B.
Ketterson,Eds.,p.1087,Springer,Berlin,Germany,2004.
[17] M.L.Kuli
´
c,“Electronphonon interaction and strong cor
relations in hightemperature superconductors:One can not
avoid the unavoidable,” in Lectures on the Physics of Highly
Correlated Electron Systems VIII:Eighth Training Course,A.
Avella and F.Mancini,Eds.,p.75,American Institute of
Physics,Melville,NY,USA,2004.
[18] M.Eschrig,“The eﬀect of collective spin1 excitations on
electronic spectra in highT
c
superconductors,” Advances in
Physics,vol.55,no.12,pp.47–183,2006.
[19] A.V.Balatsky,I.Vekhter,and J.X.Zhu,“Impurityinduced
states in conventional and unconventional superconductors,”
Reviews of Modern Physics,vol.78,no.2,pp.373–433,2006.
[20] A.M.S.Tremblay,B.Kyung,and D.S
´
en
´
echal,“Pseudo
gap and hightemperature superconductivity from weak to
strong coupling.Towards quantitative theory,” Fizika Nizkikh
Temperatur,vol.32,no.45,pp.561–595,2006.
[21] B.Edegger,V.N.Muthukumar,and C.Gros,“Gutzwiller
RVB theory of hightemperature superconductivity:results
fromrenormalized meanﬁeld theory and variational Monte
Carlo calculations,” Advances in Physics,vol.56,no.6,pp.
927–1033,2007.
[22] V.Barzykin and D.Pines,“Universal behaviour and the two
component character of magnetically underdoped cuprate
superconductors,” Advances in Physics,vol.58,no.1,pp.1–
65,2009.
[23] J.Hauck and K.Mika,“Classiﬁcation of superconducting
oxide structures,” Superconductor Science and Technology,vol.
8,no.5,pp.374–381,1995.
[24] Z.Fisk and J.L.Sarrao,“The new generation high
temperature superconductors,” Annual Review of Materials
Science,vol.27,no.1,pp.35–67,1997.
[25] J.Hauck and K.Mika,“Structure families of superconducting
oxides and interstitial alloys,” Superconductor Science and
Technology,vol.11,no.7,pp.614–630,1998.
[26] R.J.Cava,“Oxide superconductors,” Journal of the American
Ceramic Society,vol.83,no.1,pp.5–28,2000.
[27] H.R.Ott,“HighT
c
superconductivity,” in The Physics of
Superconductors.Vol.1:Conventional and HighT
c
Supercon
ductors,K.H.Bennemann and J.B.Ketterson,Eds.,p.385,
Springer,Berlin,Germany,2003.
[28] J.R.Gavaler,M.A.Janocko,and C.K.Jones,“Preparation
and properties of highT
c
NbGe ﬁlms,” Journal of Applied
Physics,vol.45,no.7,pp.3009–3013,1974.
[29] L.R.Testardi,“Structural instability and superconductivity
in A15 compounds,” Reviews of Modern Physics,vol.47,no.
3,pp.637–648,1975.
[30] K.Holczer and R.L.Whetten,“Superconducting and normal
state properties of the A
3
C
60
compounds,” Carbon,vol.30,
no.8,pp.1261–1276,1992.
[31] O.Gunnarsson,“Superconductivity in fullerides,” Reviews of
Modern Physics,vol.69,no.2,pp.575–606,1997.
[32] R.J.Cava,B.Batlogg,J.J.Krajewski,et al.,“Superconductiv
ity near 30 K without copper:the Ba
0.6
K
0.4
BiO
3
perovskite,”
Nature,vol.332,no.6167,pp.814–816,1988.
[33] L.F.Mattheiss,E.M.Gyorgy,and D.W.Johnson Jr.,
“Superconductivity above 20 K in the BaKBiO system,”
Physical Review B,vol.37,no.7,pp.3745–3746,1988.
Advances in Condensed Matter Physics 23
[34] G.M.Zhao,“Muon spin relaxation and magnetic measure
ments on Ba
0.63
K
0.37
BiO
3
:evidence for polaronic strong
coupling phononmediated pairing,” Physical Review B,vol.
76,no.2,Article ID020501,4 pages,2007.
[35] S.Yamanaka,K.Hotehama,and H.Kawaji,“Superconduc
tivity at 25.5 K in electrondoped layered hafnium nitride,”
Nature,vol.392,no.6676,pp.580–582,1998.
[36] S.Yamanaka,“HighT
c
superconductivity in electrondoped
layer structured nitrides,” Annual Reviewof Materials Science,
vol.30,pp.53–82,2000.
[37] J.Nagamatsu,N.Nakagawa,T.Muranaka,Y.Zenitani,
and J.Akimitsu,“Superconductivity at 39 K in magnesium
diboride,” Nature,vol.410,no.6824,pp.63–64,2001.
[38] J.Akimitsu and T.Muranaka,“Superconductivity in MgB
2
,”
Physica C,vol.388389,pp.98–102,2003.
[39] V.A.Drozd,A.M.Gabovich,P.Gierłowski,M.Pe¸kała,and
H.Szymczak,“Transport properties of bulk and thinﬁlm
MgB
2
superconductors:eﬀects of preparation conditions,”
Physica C,vol.402,no.4,pp.325–334,2004.
[40] X.X.Xi,“Twoband superconductor magnesium diboride,”
Reports on Progress in Physics,vol.71,no.11,Article ID
116501,26 pages,2008.
[41] S.Reich,G.Leitus,R.PopovitzBiro,A.Goldbourt,and S.
Vega,“A possible 2D H
x
WO
3
superconductor with a T
c
of
120 K,” Journal of Superconductivity and Novel Magnetism,
vol.22,no.4,pp.343–346,2009.
[42] A.M.Gabovich,V.A.Drozd,M.Pe¸kała,T.Ekino,and
R.Ribeiro,“Competition between superconductivity and
charge carrier localization in plumbates,” in Superconductiv
ity Research Advances,J.E.Nolan,Ed.,p.149,Nova Science,
New York,NY,USA,2007.
[43] H.Takahashi,K.Igawa,K.Arii,Y.Kamihara,M.Hirano,
and H.Hosono,“Superconductivity at 43 K in an iron
based layered compound LaO
1
−
x
F
x
FeAs,” Nature,vol.453,
no.7193,pp.376–378,2008.
[44] H.Hosono,“Layered iron pnictide superconductors:dis
covery and current status,” Journal of the Physical Society of
Japan,vol.77,pp.1–8,2008.
[45] M.Rotter,M.Tegel,and D.Johrendt,“Superconductivity at
38 K in the iron arsenide (Ba
1
−
x
K
x
)Fe
2
As
2
,” Physical Review
Letters,vol.101,no.10,Article ID107006,4 pages,2008.
[46] A.L.Ivanovskii,“New hightemperature superconductors
based on rare earth and transition metal oxyarsenides and
related phases:synthesis,properties and simulation,” Uspekhi
Fizicheskikh Nauk,vol.178,p.1273,2008.
[47] T.C.Ozawa and S.M.Kauzlarich,“Chemistry of layered d
metal pnictide oxides and their potential as candidates for
new superconductors,” Science and Technology of Advanced
Materials,vol.9,no.3,Article ID033003,11 pages,2008.
[48] H.Hosono,“Two classes of superconductors discovered in
our material research:ironbased high temperature super
conductor and electride superconductor,” Physica C,vol.469,
no.9–12,pp.314–325,2009.
[49] C.Day,“Ironbased superconductors,” Physics Today,vol.62,
no.8,pp.36–40,2009.
[50] V.L.Ginzburg,“About ferromagnetic superconductors,”
Zhurnal Eksperimental’noi i Teoreticheskoi Fiziki,vol.31,p.
202,1956.
[51] M.B.Maple and ∅.Fischer,Eds.,Superconductivity in
Ternary Compounds II,Superconductivity and Magnetism,
vol.34 of Topics in Current Physics,Springer,Berlin,Ger
many,1982.
[52] L.N.Bulaevskii,A.I.Buzdin,M.L.Kuli
´
c,and S.V.
Panjukov,“Coexistence of superconductivity and magnetism
theoretical predictions and experimental results,” Advances in
Physics,vol.34,no.2,pp.175–261,1985.
[53] L.N.Bulaevskii,“Magnetic superconductors,” in Supercon
ductivity,Superdiamagnetism,Superﬂuidity,V.L.Ginzburg,
Ed.,p.69,Mir,Moscow,Russia,1987.
[54] Yu.A.Izyumov,M.I.Katsnelson,and Yu.N.Skryabin,
Itinerant Electron Magnetism,Fiziko Matematicheskaya Lit
eratura,Moscow,Russia,1994.
[55] A.I.Buzdin,“Proximity eﬀects in superconductor
ferromagnet heterostructures,” Reviews of Modern Physics,
vol.77,no.3,pp.935–976,2005.
[56] A.M.Gabovich and D.P.Moiseev,“Metalloxide supercon
ductor BaPb
1
−
x
Bi
x
O
3
:unusual properties and new applica
tions,” Uspekhi Fizicheskikh Nauk,vol.150,p.599,1986.
[57] R.Collongues,La NonStoechiometrie,Masson,Paris,France,
1971.
[58] A.M.Stoneham and L.W.Smith,“Defect phenomena
in superconducting oxides and analogous ceramic oxides,”
Journal of Physics:Condensed Matter,vol.3,no.3,pp.225–
278,1991.
[59] O.Matsumoto,A.Utsuki,A.Tsukada,H.Yamamoto,T.
Manabe,and M.Naito,“Synthesis and properties of super
conducting TR
2
CuO
4
(R
=
Pr,Nd,Sm,Eu,Gd),” Physical
Review B,vol.79,no.10,Article ID100508,4 pages,2009.
[60] Z.Ren,Q.Tao,S.Jiang,et al.,“Superconductivity induced by
phosphorus doping and its coexistence with ferromagnetism
in EuFe
2
(As
0.7
P
0.3
)
2
,” Physical ReviewLetters,vol.102,no.13,
Article ID137002,4 pages,2009.
[61] R.J.Cava,“Contemporary superconducting materials,”
Chemical Communications,no.43,pp.5373–5377,2005.
[62] W.E.Pickett,“The next breakthrough in phononmediated
superconductivity,” Physica C,vol.468,no.2,pp.126–135,
2008.
[63] J.C.Phillips,“Hardwired dopant networks and the predic
tionof hightransitiontemperatures inceramic superconduc
tors,” Advances in Condensed Matter Physics,vol.2010,Article
ID250891,13 pages,2010.
[64] J.C.Phillips,“Zigzag ﬁlamentary theory of longitudi
nal optical phonons in hightemperature superconductors,”
Philosophical Magazine B,vol.81,no.1,pp.35–53,2001.
[65] J.C.Phillips and J.Jung,“Nanodomain structure and func
tion of hightemperature superconductors,” Philosophical
Magazine B,vol.81,no.8,pp.745–756,2001.
[66] J.C.Phillips,“Percolative model of nanoscale phase sepa
ration in hightemperature superconductors,” Philosophical
Magazine B,vol.82,no.7,pp.783–790,2002.
[67] J.C.Phillips,“Selforganized networks and lattice eﬀects in
hightemperature superconductors,” Physical Review B,vol.
75,no.21,Article ID214503,23 pages,2007.
[68] G.Litak,A.M.Martin,B.Gy
¨
orﬀy,J.F.Annett,and K.I.
Wysoki
˜
nski,“Van Hove singularity and dwave pairing in
disordered superconductors,” Physica C,vol.309,no.34,pp.
257–262,1998.
[69] G.Litak and B.Gy
¨
orﬀy,“Random negativeU hubbard
model,” Physical Review B,vol.62,no.10,pp.6629–6637,
2000.
[70] G.Litak,B.Gy
¨
orﬀy,and K.I.Wysoki
˜
nski,“Charge and
order parameter ﬂuctuations in disordered superconduc
tors,” Physica C,vol.308,no.12,pp.132–146,1998.
[71] G.Litak,“Charge and phase ﬂuctuations in attractive
Hubbard model,” Physica C,vol.387,no.12,pp.86–88,
2003.
24 Advances in Condensed Matter Physics
[72] G.Litak,“Charge order versus superconductivity in inho
mogeneous systems,” Journal of Superconductivity and Novel
Magnetism,vol.22,no.3,pp.265–267,2009.
[73] A.M.Gabovich and A.I.Voitenko,“Temperaturedependent
inelastic electron scattering and superconducting state prop
erties,” Physics Letters A,vol.190,no.2,pp.191–195,1994.
[74] A.M.Gabovich and A.I.Voitenko,“Inﬂuence of inelastic
quasiparticle scattering on thermodynamic and transport
properties of highT
c
oxides,” Physica C,vol.258,no.34,pp.
236–252,1996.
[75] A.M.Gabovich,“Powerlaw lowtemperature asymptotics
for spatially nonhomogeneous swave superconductors,”
Fizika Nizkikh Temperatur,vol.25,no.7,pp.677–684,1999.
[76] A.M.Gabovich and A.I.Voitenko,“Inﬂuence of order
parameter nonhomogeneities on lowtemperature properties
of superconductors,” Physical Review B,vol.60,no.10,pp.
7465–7472,1999.
[77] A.M.Gabovich,A.I.Voitenko,M.S.Li,and H.Szymczak,
“Heat capacity of mesoscopically disordered superconduc
tors:implications for MgB
2
,” Fizika Nizkikh Temperatur,vol.
28,no.11,pp.1126–1137,2002.
[78] A.M.Gabovich,M.S.Li,M.Pe¸kała,H.Szymczak,and
A.I.Voitenko,“Heat capacity of mesoscopically disordered
superconductors with emphasis on MgB
2
,” Journal of Physics:
Condensed Matter,vol.14,no.41,pp.9621–9629,2002.
[79] A.M.Gabovich,M.S.Li,M.Pe¸kała,H.Szymczak,and A.I.
Voitenko,“Heat capacity of mesoscopically inhomogeneous
superconductors:theory and applications to MgB
2
,” Physica
C,vol.405,no.34,pp.187–211,2004.
[80] T.Ekino,A.M.Gabovich,M.S.Li,et al.,“Spatially
heterogeneous character of superconductivity in MgB
2
as
revealed by local probe and bulk measurements,” Physica C,
vol.426–431,no.1,pp.230–233,2005.
[81] A.M.Gabovich and A.I.Voitenko,“Chargedensitywave
origin of the diphump structure in tunnel spectra of the
BSCCO superconductor,” Physical Review B,vol.75,no.6,
Article ID064516,13 pages,2007.
[82] T.Ekino,A.M.Gabovich,M.S.Li,M.Pe¸kała,H.
Szymczak,and A.I.Voitenko,“Analysis of the pseudogap
related structure in tunneling spectra of superconducting
Bi
2
Sr
2
CaCu
2
O
8+δ
revealed by the breakjunction technique,”
Physical Review B,vol.76,no.18,Article ID180503,4 pages,
2007.
[83] T.Ekino,A.M.Gabovich,M.S.Li,M.Pe¸kała,H.Szymczak,
and A.I.Voitenko,“Temperaturedependent pseudogap
like features in tunnel spectra of highT
c
cuprates as a
manifestation of chargedensity waves,” Journal of Physics:
Condensed Matter,vol.20,no.42,Article ID 425218,15
pages,2008.
[84] J.C.Phillips,“Is there a lowest upper bound for super
conductive transition temperatures?” Journal of Physics:
Conference Series,vol.108,no.1,Article ID 012033,6 pages,
2008.
[85] B.T.Matthias,“Anticorrelations in superconductivity,” Phys
ica,vol.55,pp.69–72,1971.
[86] F.E.Wang and M.A.Mitchell,“A new correlation:
superconducting critical temperature vs number of naturally
occuring isotopes among superconducting elements,” Solid
State Communications,vol.15,no.5,pp.867–869,1974.
[87] D.M.Gualtieri,“The correlation between the superconduct
ing critical temperature and the number of stable isotopes
among superconducting elements,” Solid State Communica
tions,vol.16,no.7,pp.917–918,1975.
[88] I.O.Kulik,“Superconductivity and macroscopic stability
criteria for electronphonon systems,” Zhurnal Eksperimen
tal’noj i Teoreticheskoj Fiziki,vol.66,p.2224,1974.
[89] I.O.Kulik,“Spin ﬂuctuations and superconductivity,” Fizika
Nizkikh Temperatur,vol.2,p.486,1976.
[90] A.M.Gabovich,“On the criterion of superconductivity of
metals,” Ukrainskii Fizychnyi Zhurnal,vol.22,p.2072,1977.
[91] A.M.Gabovich and D.P.Moiseev,“Superconductivity of
metals with the allowance for ion core repulsion,” Fizika
Nizkikh Temperatur,vol.4,p.1115,1978.
[92] A.M.Gabovich and D.P.Moiseev,“Isotope eﬀect in jellium
and Brout models,” Fizika Tverdogo Tela,vol.23,p.1511,
1981.
[93] I.M.Chapnik,“On the possible relation between the absence
of superconductivity in Au and PdAg alloys and the negative
sign of the Hall coeﬃcient,” Journal of Physics F,vol.13,no.
5,pp.975–978,1983.
[94] I.M.Chapnik,“Regularities in the occurrence of supercon
ductivity,” Journal of Physics F,vol.14,no.8,pp.1919–1921,
1984.
[95] J.E.Hirsch,“Correlations between normalstate properties
and superconductivity,” Physical ReviewB,vol.55,no.14,pp.
9007–9024,1997.
[96] C.Buzea and K.Robbie,“Assembling the puzzle of super
conducting elements:a review,” Superconductor Science and
Technology,vol.18,no.1,pp.R1–R8,2005.
[97] F.Huber,H.P.Roeser,and M.von Schoenermark,“A
correlation between T
c
of Febased HT superconductors and
the crystal super lattice constants of the doping element
positions,” Journal of the Physical Society of Japan,vol.77,pp.
142–144,2008.
[98] B.J.Taylor and M.B.Maple,“Formula for the critical
temperature of superconductors based on the electronic
density of states and the eﬀective mass,” Physical Review
Letters,vol.102,no.13,Article ID137003,4 pages,2009.
[99] A.M.Gabovich,“About superconductivity of polar semicon
ductors,” Fizika Tverdogo Tela,vol.22,no.11,pp.3231–3235,
1980.
[100] R.Baquero,“What determines the magnitude of T
c
in
HTSC?” in Frontiers in Contemporary Physics—EAV08,L.M.
M.Zetina,G.T.Vega,M.G.Roclia,L.F.R.Oclioa,and
R.L.Fern
´
andez,Eds.,p.218,American Institute of Physics,
Melville,NY,USA,2008.
[101] X.Blase,E.Bustarret,C.Chapelier,T.Klein,and C.Marce
nat,“Superconducting groupIV semiconductors,” Nature
Materials,vol.8,no.5,pp.375–382,2009.
[102] B.E.C.Koltenbah and R.Joynt,“Materialspeciﬁc gap func
tion in the tJ model of hightemperature superconductors,”
Reports on Progress in Physics,vol.60,no.1,pp.23–56,1997.
[103] M.Ogata and H.Fukuyama,“The tJ model for the oxide
highT
c
superconductors,” Reports on Progress in Physics,vol.
71,no.3,Article ID036501,45 pages,2008.
[104] W.Fan,“Predictions of highest transitiontemperature for
electronphonon superconductors,” Physica C,vol.469,no.
4,pp.177–181,2009.
[105] G.M.Eliashberg,“Interaction of electrons with lattice
vibrations in a superconductor,” Zhurnal Eksperimental’noi
i Teoreticheskoi Fiziki,vol.38,p.966,1960.
[106] G.M.Eliashberg,“Temperature Green’s functions of elec
trons in a superconductor,” Zhurnal Eksperimental’noi i
Teoreticheskoi Fiziki,vol.39,p.1437,1960.
[107] B.Brandow,“Characteristic features of the exotic supercon
ductors,” Physics Reports,vol.296,no.1,pp.1–63,1998.
Advances in Condensed Matter Physics 25
[108] B.Brandow,“Explanation of the exotic superconductors
by a valenceﬂuctuation pairing mechanism,” Philosophical
Magazine B,vol.80,no.6,pp.1229–1297,2000.
[109] G.M.Zhao,“Experimental constraints on the physics of
cuprates,” Philosophical Magazine B,vol.81,no.10,pp.1335–
1388,2001.
[110] G.M.Zhao,“Pairing interactions and pairing mechanism
in hightemperature copper oxide superconductors,” Physical
Review B,vol.71,no.10,Article ID104517,9 pages,2005.
[111] A.S.Alexandrov,“High temperature superconductivity due
to a longrange electronphonon interaction,application
to isotope eﬀects,thermomagnetic transport and nanoscale
heterogeneity in cuprates,” Journal of Superconductivity,vol.
18,no.56,pp.603–612,2005.
[112] W.E.Pickett,“Design for a roomtemperature superconduc
tor,” Journal of Superconductivity and Novel Magnetism,vol.
19,no.3–5,pp.291–297,2006.
[113] A.M.Kadin,“Coherent lattice vibrations in superconduc
tors,” Physica C,vol.468,no.4,pp.255–259,2008.
[114] J.TahirKheli and W.A.Goddard III,“The Chiral Plaquette
Polaron Paradigm (CPPP) for high temperature cuprate
superconductors,” Chemical Physics Letters,vol.472,no.4–
6,pp.153–165,2009.
[115] V.Z.Kresin and S.A.Wolf,“Colloquium:electronlattice
interaction and its impact on high T
c
superconductivity,”
Reviews of Modern Physics,vol.81,no.2,pp.481–501,2009.
[116] C.Panagopoulos and T.Xiang,“Relationship between the
superconducting energy gap and the critical temperature in
highT
c
superconductors,” Physical Review Letters,vol.81,
no.11,pp.2336–2339,1998.
[117] R.A.Klemmand K.Scharnberg,“Theory of bicrystal caxis
twist Josephson junctions,” International Journal of Modern
Physics B,vol.15,no.2425,pp.3164–3189,2001.
[118] G.M.Zhao,“Identiﬁcation of the bulk pairing symmetry in
hightemperature superconductors:evidence for anextended
s wave with eight line nodes,” Physical Review B,vol.64,no.
2,Article ID024503,10 pages,2001.
[119] B.H.Brandow,“Arguments and evidence for a node
containing anisotropic swave gap form in the cuprate
superconductors,” Physical Review B,vol.65,no.5,Article
ID054503,5 pages,2002.
[120] B.H.Brandow,“Strongly anisotropic swave gaps in exotic
superconductors,” Philosophical Magazine,vol.83,no.21,pp.
2487–2519,2003.
[121] G.M.Zhao,“The magnetic resonance in hightemperature
superconductors:evidence for an extended swave pairing
symmetry,” Philosophical Magazine B,vol.84,no.36,pp.
3869–3882,2004.
[122] R.A.Klemm,“The phasesensitive caxis twist experiments
on Bi
2
Sr
2
CaCu
2
O
8+δ
and their implications,” Philosophical
Magazine,vol.85,no.8,pp.801–853,2005.
[123] T.H.Geballe,“The neverending search for high
temperature superconductivity,” Journal of Superconductivity
and Novel Magnetism,vol.19,no.3–5,pp.261–276,2006.
[124] R.Baquero,“Superconductivity today:a brief panorama,” in
Advanced Summer School in Physics 2005,O.RosasOrtiz,M.
Carbajal,and O.Miranda,Eds.,p.301,American Institute of
Physics,Melville,NY,USA,2006.
[125] R.Khasanov,S.Str
¨
assle,D.Di Castro,et al.,“Multiple gap
symmetries for the order parameter of cuprate superconduc
tors frompenetration depth measurements,” Physical Review
Letters,vol.99,no.23,Article ID237601,4 pages,2007.
[126] T.Das,R.S.Markiewicz,and A.Bansil,“Nodeless dwave
superconducting pairing due to residual antiferromagnetism
in underdoped Pr
2
−
x
Ce
x
CuO
4
−
δ
,” Physical Review Letters,
vol.98,no.19,Article ID197004,4 pages,2007.
[127] G.M.Zhao,“Precise determination of the superconducting
gap along the diagonal direction of Bi
2
Sr
2
CaCu
2
O
8+y
:evi
dence for an extended swave gap symmetry,” Physical Review
B,vol.75,no.14,Article ID140510,4 pages,2007.
[128] R.Khasanov,A.Shengelaya,A.Maisuradze,et al.,“Node
less superconductivity in the inﬁnitelayer electrondoped
cuprate superconductor Sr
0.9
La
0.1
CuO
2
,” Physical Review B,
vol.77,no.18,Article ID184512,6 pages,2008.
[129] R.Prozorov,“Superﬂuid density in a superconductor with an
extended dwave gap,” Superconductor Science and Technol
ogy,vol.21,no.8,Article ID082003,3 pages,2008.
[130] M.Bakr,A.P.Schnyder,L.Klam,et al.,“Electronic and
phononic Raman scattering in detwinned YBa
2
Cu
3
O
6.95
and
Y
0.85
Ca
0.15
Ba
2
Cu
3
O
6.95
:swave admixture to the d
x
2
−
y
2
wave
order parameter,” Physical Review B,vol.80,no.6,Article ID
064505,11 pages,2009.
[131] C.C.Tsuei and J.R.Kirtley,“Pairing symmetry in cuprate
superconductors,” Reviews of Modern Physics,vol.72,no.4,
pp.969–1016,2000.
[132] H.Hilgenkamp and J.Mannhart,“Grain boundaries in high
T
c
superconductors,” Reviews of Modern Physics,vol.74,no.
2,pp.485–549,2002.
[133] C.C.Tsuei and J.R.Kirtley,“Pairing symmetry in cuprate
superconductors:phasesensitive tests,” in The Physics of
Superconductors.Vol.1:Conventional and HighT
c
Supercon
ductors,K.H.Bennemann and J.B.Ketterson,Eds.,p.647,
Springer,Berlin,Germany,2003.
[134] R.Micnas,J.Ranninger,and S.Robaszkiewicz,“Supercon
ductivity in narrowband systems with local nonretarded
attractive interactions,” Reviews of Modern Physics,vol.62,
no.1,pp.113–171,1990.
[135] A.S.Alexandrov,“Polaronic and bipolaronic highT
c
super
conductivity,” in Models and Phenomenology for Conventional
and HighTemperature Superconductivity,G.Iadonisi,J.R.
Schrieﬀer,and M.L.Chiofalo,Eds.,p.309,IOS Press,
Amsterdam,The Netherlands,1998.
[136] T.Sko
´
skiewicz,A.W.Szafra
˜
nski,W.Bujnowski,and B.Bara
nowski,“Isotope eﬀect in the superconducting palladium
hydrogendeuteriumsystem,” Journal of Physics C,vol.7,no.
15,pp.2670–2676,1974.
[137] B.Stritzker,“Ion implantation and superconductivity,” Jour
nal of Nuclear Materials,vol.72,no.12,pp.256–262,1978.
[138] T.Matsubara and A.Kotani,Eds.,Superconductivity in
Magnetic and Exotic Materials,Springer,Berlin,Germany,
1984.
[139] A.Taraphder,R.Pandit,H.R.Krishnamurthy,and T.V.
Ramakrishnan,“The exotic barium bismuthates,” Interna
tional Journal of Modern Physics B,vol.10,no.8,pp.863–955,
1996.
[140] A.M.Gabovich,“Possibility of cold fusion in palladiumdeu
tendes:screening eﬀects and connection to superconducting
properties,” Philosophical Magazine B,vol.76,no.1,pp.107–
118,1997.
[141] N.D.Mathur,F.M.Grosche,S.R.Julian,et al.,“Magnetically
mediated superconductivity in heavy fermion compounds,”
Nature,vol.394,no.6688,pp.39–43,1998.
[142] E.Bauer,G.Hilscher,H.Michor,et al.,“Heavy fermion
superconductivity and magnetic order in noncentrosymmet
ric CePt
3
Si,” Physical Review Letters,vol.92,no.2,Article ID
027003,4 pages,2004.
26 Advances in Condensed Matter Physics
[143] S.G.Ovchinnikov,“Exotic superconductivity and mag
netism in ruthenates,” Uspekhi Fizicheskikh Nauk,vol.173,
no.1,pp.27–51,2003.
[144] A.P.Mackenzie and Y.Maeno,“The superconductivity of
Sr
2
RuO
4
and the physics of spintriplet pairing,” Reviews of
Modern Physics,vol.75,no.2,pp.657–712,2003.
[145] P.S.Riseborough,G.M.Schmiedeschoﬀ,and J.L.Smith,
“Heavy fermion superconductivity,” in The Physics of Super
conductors.Vol.2:Conventional and HighT
c
Superconductors,
K.H.Bennemann and J.B.Ketterson,Eds.,p.889,Springer,
Berlin,Germany,2004.
[146] P.Thalmeier,G.Zwicknagl,O.Stockert,G.Sparn,and F.
Steglich,“Superconductivity in heavy Fermion compounds,”
in Frontiers in Superconducting Materials,A.V.Narlikar,Ed.,
p.109,Springer,Berlin,Germany,2005.
[147] D.A.Bonn,“Are hightemperature superconductors exotic?”
Nature Physics,vol.2,no.3,pp.159–166,2006.
[148] S.Fujimoto,“Electron correlation and pairing states in
superconductors without inversion symmetry,” Journal of the
Physical Society of Japan,vol.76,no.5,Article ID051008,14
pages,2007.
[149] Y.Kitaoka,H.Mukuda,M.Yashima,and A.Harada,“Uncon
ventional pairing states in heavyfermion superconductors
studied by the NQR/NMR experiments,” Journal of the
Physical Society of Japan,vol.76,no.5,Article ID 051001,
15 pages,2007.
[150] T.Sakakibara,A.Yamada,J.Custers,et al.,“Nodal structures
of heavy fermion superconductors probed by the speciﬁc
heat measurements in magnetic ﬁelds,” Journal of the Physical
Society of Japan,vol.76,no.5,Article ID 051004,11 pages,
2007.
[151] J.L.Sarrao and J.D.Thompson,“Superconductivity in
cerium and plutoniumbased ‘115’ materials,” Journal of the
Physical Society of Japan,vol.76,no.5,Article ID 051013,9
pages,2007.
[152] Y.Haga,H.Sakai,and S.Kambe,“Recent advances in the 5f
relevant electronic states and unconventional superconduc
tivity of actinide compounds,” Journal of the Physical Society
of Japan,vol.76,no.5,Article ID051012,21 pages,2007.
[153] Y.Kasahara,T.Iwasawa,H.Shishido,et al.,“Gap structure
and exotic superconducting state of URu
2
Si
2
,” Journal of
Physics:Conference Series,vol.150,Article ID 052098,4
pages,2009.
[154] R.D.Parks,Ed.,Superconductivity,vol.1,Marcel Dekker,
New York,NY,USA,1969.
[155] R.D.Parks,Ed.,Superconductivity,vol.2,Marcel Dekker,
New York,NY,USA,1969.
[156] K.H.Bennemann and J.B.Ketterson,Eds.,The Physics of
Superconductors.Vol.1:Conventional and HighT
c
Supercon
ductors,Springer,Berlin,Germany,2003.
[157] K.H.Bennemann and J.B.Ketterson,Eds.,The Physics of
Superconductors.Vol.2:Conventional and HighT
c
Supercon
ductors,Springer,Berlin,Germany,2004.
[158] A.M.Gabovich and A.I.Voitenko,“Superconductors with
charge and spindensity waves:theory and experiment,”
Fizika Nizkikh Temperatur,vol.26,no.5,pp.419–452,2000.
[159] A.M.Gabovich,A.I.Voitenko,J.F.Annett,and M.
Ausloos,“Charge and spindensitywave superconductors,”
Superconductor Science and Technology,vol.14,no.4,pp.R1–
R27,2001.
[160] A.M.Gabovich,A.I.Voitenko,and M.Ausloos,“Charge
and spindensity waves in existing superconductors:com
petition between Cooper pairing and Peierls or excitonic
instabilities,” Physics Reports,vol.367,no.6,pp.583–709,
2002.
[161] I.I.Mazin and J.Schmalian,“Pairing symmetry and pairing
state in ferropnictides:theoretical overview,” Physica C,vol.
469,no.9–12,pp.614–627,2009.
[162] A.W.Sleight,J.L.Gillson,and P.E.Bierstedt,“High
temperature superconductivity in the BaPb
1
−
x
Bi
x
O
3
sys
tems,” Solid State Communications,vol.17,no.1,pp.27–28,
1975.
[163] S.Tajima,S.Uchida,A.Masaki,et al.,“Electronic states of
BaPb
1
−
x
Bi
x
O
3
in the semiconducting phase investigated by
optical measurements,” Physical Review B,vol.35,no.2,pp.
696–703,1987.
[164] S.Tajima,H.Ishii,I.Rittaporn,et al.,“Vacuumultraviolet
spectra and band structure of BaPb
1
−
x
Bi
x
O
3
,” Physical
Review B,vol.38,no.2,pp.1143–1147,1988.
[165] D.T.Marx,P.G.Radaelli,J.D.Jorgensen,et al.,“Metastable
behavior of the superconducting phase in the BaBi
1
−
x
Pb
x
O
3
system,” Physical Review B,vol.46,no.2,pp.1144–1156,
1992.
[166] M.Yasukawa and N.Murayama,“A phase transition with
an abrupt electrical resistivity change around 800 K in
BaBi
0.5
Pb
0.5
O
3
,” Physica C,vol.297,no.34,pp.326–332,
1998.
[167] A.Yamamoto,T.Furumochi,and S.Tajima,“Metalinsulator
transition and superconductivity in Sr and Lasubstituted
BaPb
1
−
x
Bi
x
O
3
,” Physica C,vol.328,no.1,pp.118–124,1999.
[168] V.J.Emery and S.A.Kivelson,“Superconductivity in bad
metals,” Physical Review Letters,vol.74,no.16,pp.3253–
3256,1995.
[169] N.F.Mott and E.A.Davis,Electron Processes in Non
Crystalline Materials,Clarendon Press,Oxford,UK,1979.
[170] J.F.Schooley,W.R.Hosler,E.Ambler,J.H.Becker,M.L.
Cohen,and C.S.Koonce,“Dependence of the supercon
ducting transition temperature on carrier concentration in
semiconducting SrTiO
3
,” Physical Review Letters,vol.14,no.
9,pp.305–307,1965.
[171] K.Shibuya,T.Ohnishi,T.Sato,and M.Lippmaa,“Metal
insulator transition in SrTiO
3
induced by ﬁeld eﬀect,” Journal
of Applied Physics,vol.102,no.8,Article ID083713,2007.
[172] C.H.Ahn,A.Bhattacharya,M.Di Ventra,et al.,“Electro
static modiﬁcation of novel materials,” Reviews of Modern
Physics,vol.78,no.4,pp.1185–1212,2006.
[173] A.Ohtomo and H.Y.Hwang,“A highmobility electron gas
at the LaAIO
3
/SrTiO
3
heterointerface,” Nature,vol.427,no.
6973,pp.423–426,2004.
[174] N.Reyren,S.Thiel,A.D.Caviglia,et al.,“Superconducting
interfaces between insulating oxides,” Science,vol.317,no.
5842,pp.1196–1199,2007.
[175] S.Gariglio,N.Reyren,A.D.Caviglia,and J.M.Triscone,
“Superconductivity at the LaAIO
3
/SrTiO
3
interface,” Journal
of Physics:Condensed Matter,vol.21,no.16,Article ID
164213,2009.
[176] L.J.de Jongh,“A comparative study of (BI)polaronic
(super)conductivity in high and lowT
c
superconducting
oxides,” Physica C,vol.152,no.2,pp.171–216,1988.
[177] T.Egami and S.J.L.Billinge,“Lattice eﬀects in high
temperature superconductors,” Progress in Materials Science,
vol.38,no.1,pp.359–424,1994.
[178] K.S.Aleksandrov and B.V.Beznosikov,“Hierarchy of
perovskitelike crystals:a review,” Fizika Tverdogo Tela,vol.
39,p.785,1997.
[179] K.S.Aleksandrov and J.Bartolom
´
e,“Structural distortions
in families of perovskitelike crystals,” Phase Transitions,vol.
74,no.3,pp.255–335,2001.
Advances in Condensed Matter Physics 27
[180] M.Karppinen and H.Yamauchi,“Control of the charge
inhomogeneity and highT
c
superconducting properties in
homologous series of multilayered copper oxides,” Materials
Science and Engineering R,vol.26,no.3,pp.51–96,1999.
[181] T.Yamauchi,M.Isobe,and Y.Ueda,“Charge order and
superconductivity in vanadium oxides,” Solid State Sciences,
vol.7,no.7,pp.874–881,2005.
[182] A.S.Barker Jr.and M.Tinkham,“Farinfrared ferroelectric
vibration mode in SrTiO
3
,” Physical Review,vol.125,no.5,
pp.1527–1530,1962.
[183] M.E.Lines and A.M.Glass,Principles and Application of
Ferroelectrics and Related Materials,Clarendon Press,Oxford,
UK,1977.
[184] C.Z.Bi,J.Y.Ma,J.Yan,et al.,“Electronphonon coupling
in Nbdoped SrTiO
3
single crystal,” Journal of Physics:
Condensed Matter,vol.18,no.8,pp.2553–2561,2006.
[185] D.M.Eagles,“Superconductivity at very low carrier con
centrations and indications of a charged bose gas in
SrTi
0.97
Zr
0.03
O
3
,” Solid State Communications,vol.60,no.6,
pp.521–524,1986.
[186] M.Jourdan,N.Bl
¨
umer,and H.Adrian,“Superconductivity
of SrTiO
3
−
δ
,” European Physical Journal B,vol.33,no.1,pp.
25–30,2003.
[187] M.Jourdan and H.Adrian,“Possibility of unconventional
superconductivity of SrTiO
3
−
δ
,” Physica C,vol.388389,pp.
509–510,2003.
[188] V.L.Vinetskii,“Bipolar states of current carriers in ionic
crystals,” Zhurnal Eksperimental’noi i Teoreticheskoi Fiziki,
vol.40,p.1459,1961.
[189] J.Bardeen,L.N.Cooper,and J.R.Schrieﬀer,“Theory of
superconductivity,” Physical Review,vol.108,no.5,pp.1175–
1204,1957.
[190] M.R.Schafroth,S.T.Butler,and J.M.Blatt,“Quasichemical
equilibriumapproach to superconductivity,” Helvetica Phys
ica Acta,vol.30,p.93,1957.
[191] D.M.Eagles,“Possible pairing without superconductivity at
low carrier concentrations in bulk and thinﬁlm supercon
ducting semiconductors,” Physical Review,vol.186,no.2,pp.
456–463,1969.
[192] A.S.Alexandrov and J.Ranninger,“Theory of bipolarons
and bipolaronic bands,” Physical Review B,vol.23,no.4,pp.
1796–1801,1981.
[193] A.S.Alexandrov and J.Ranninger,“Bipolaronic supercon
ductivity,” Physical Review B,vol.24,no.3,pp.1164–1169,
1981.
[194] A.S.Alexandrov,J.Ranninger,and S.Robaszkiewicz,
“Bipolaronic superconductivity:thermodynamics,magnetic
properties,and possibility of existence in real substances,”
Physical Review B,vol.33,no.7,pp.4526–4542,1986.
[195] D.Emin and M.S.Hillery,“Formation of a large sin
glet bipolaron:application to hightemperature bipolaronic
superconductivity,” Physical Review B,vol.39,no.10,pp.
6575–6593,1989.
[196] R.Friedberg,T.D.Lee,and H.C.Ren,“A correction to
Schafroth’s superconductivity solution of an ideal charged
boson system,” Annals of Physics,vol.208,no.1,pp.149–215,
1991.
[197] A.S.Alexandrov and N.F.Mott,“Bipolarons,” Reports on
Progress in Physics,vol.57,no.12,pp.1197–1288,1994.
[198] R.Friedberg and T.D.Lee,“Comments on the superconduc
tivity solution of an ideal charged boson system,” Journal of
Superconductivity and Novel Magnetism,vol.19,no.3–5,pp.
277–282,2006.
[199] J.T.Devreese and A.S.Alexandrov,“Fr
¨
ohlich polaron
and bipolaron:recent developments,” Reports on Progress in
Physics,vol.72,no.6,Article ID066501,2009.
[200] T.M.Rice and L.Sneddon,“Realspace and k
→
space
electron pairing in BaPb
1
−
x
Bi
x
O
3
,” Physical Review Letters,
vol.47,no.9,pp.689–692,1981.
[201] I.B.Bischofs,V.N.Kostur,and P.B.Allen,“Polaron and
bipolaron defects in a charge density wave:a model for lightly
doped BaBiO
3
,” Physical Review B,vol.65,no.11,Article ID
115112,7 pages,2002.
[202] I.B.Bischofs,P.B.Allen,V.N.Kostur,and R.Bhargava,
“Topological doping of a threedimensional Peierls system:
predicted structure of doped BaBiO
3
,” Physical ReviewB,vol.
66,no.17,Article ID174108,5 pages,2002.
[203] M.Merz,N.N
¨
ucker,S.Schuppler,et al.,“Xray absorption
of Ba
1
−
x
K
x
BiO
3
and BaPb
1
−
y
Bi
y
O
3
:competition between
bipolaronic and chargedensity wave states,” Europhysics
Letters,vol.72,no.2,pp.275–281,2005.
[204] D.G.Hinks,B.Dabrowski,J.D.Jorgensen,et al.,“Synthesis,
structure and superconductivity in the Ba
1
−
x
K
x
BiO
3
−
y
sys
tem,” Nature,vol.333,no.6176,pp.836–838,1988.
[205] A.I.Golovashkin,L.N.Zherikhina,G.V.Kuleshova,A.
M.Tskhovrebov,and M.L.Norton,“Selfconsistent spatially
inhomogeneous state in HTSC Ba
1
−
x
K
x
BiO
3
single crystals,”
Pis’ma v Zhurnal Eksperimental’noi i Teoreticheskoi Fiziki,vol.
129,p.684,2006.
[206] G.Iadonisi,M.Chiofalo,V.Cataudella,and D.Ninno,
“Phononplasmon cooperative eﬀects in the dilute large
bipolaron gas:a possible mechanism for highT
c
supercon
ductivity,” Physical Review B,vol.48,no.17,pp.12966–
12978,1993.
[207] T.Nishio,J.Ahmad,and H.Uwe,“Spectroscopic observation
of bipolaronic point defects in Ba
1
−
x
K
x
BiO
3
,” Physical Review
Letters,vol.95,no.17,Article ID176403,4 pages,2005.
[208] A.S.Alexandrov,“dwave BoseEinstein condensate and
tunnelling in superconducting cuprates,” Physica C,vol.305,
no.12,pp.46–56,1998.
[209] A.S.Alexandrov and V.V.Kabanov,“Parameterfree expres
sion for superconducting T
c
in cuprates,” Physical Review B,
vol.59,no.21,pp.13628–13631,1999.
[210] A.S.Alexandrov,“Polaron dynamics and bipolaron conden
sation in cuprates,” Physical Review B,vol.61,no.18,pp.
12315–12327,2000.
[211] Q.Chen,J.Stajic,S.Tan,and K.Levin,“BCSBEC crossover:
from high temperature superconductors to ultracold super
ﬂuids,” Physics Reports,vol.412,no.1,pp.1–88,2005.
[212] L.S.Marchenko,D.P.Moiseev,E.A.Muzalevskii,and
S.K.Uvarova,“Superconductivity in the solidsolutions
BaPb
1
−
x
Bi
x
O
3
,” Inorganic Materials,vol.15,p.1492,1979.
[213] T.D.Thanh,A.Koma,and S.Tanaka,“Superconductivity in
the BaPb
1
−
x
Bi
x
O
3
system,” Applied Physics,vol.22,no.2,pp.
205–212,1980.
[214] D.P.Moiseev,S.K.Uvarova,and M.B.Fenik,“Hall
voltage and conductivity in the superconducting oxide
system BaPbO
3
–BaBiO
3
,” Fizika Tverdogo Tela,vol.23,p.
2347,1981.
[215] M.L.Cohen,“Superconductivity in lowcarrierdensity
systems:degenerate semiconductors,” in Superconductivity,
R.D.Parks,Ed.,vol.1,p.615,Marcel Dekker,NewYork,NY,
USA,1969.
[216] Y.Takada,“Theory of superconductivity in polar semi
conductors and its application to ntype semiconducting
SrTiO
3
,” Journal of the Physical Society of Japan,vol.49,no.
4,pp.1267–1275,1980.
28 Advances in Condensed Matter Physics
[217] T.Egami,“Nanoscale complexities in the superconducting
cuprates,” Journal of Physics and Chemistry of Solids,vol.69,
no.9,pp.2191–2194,2008.
[218] L.Pietronero and E.Cappelluti,“Superconductivity,nona
diabaticity and strong correlation in the light of recent
experiments,” Journal of Physics:Conference Series,vol.108,
no.1,Article ID012025,2008.
[219] R.Friedberg and T.D.Lee,“Gap energy and longrange order
in the bosonfermion model of superconductivity,” Physical
Review B,vol.40,no.10,pp.6745–6762,1989.
[220] J.Ranninger and J.M.Robin,“The bosonfermion model of
highT
c
superconductivity.Doping dependence,” Physica C,
vol.253,no.34,pp.279–291,1995.
[221] J.Ranninger and J.M.Robin,“Manifestations of the
pseudogap in the bosonfermion model for BoseEinstein
condensationdriven superconductivity,” Physical Review B,
vol.53,no.18,pp.R11961–R11963,1996.
[222] E.Altman and A.Auerbach,“Plaquette bosonfermion
model of cuprates,” Physical Review B,vol.65,no.10,Article
ID104508,15 pages,2002.
[223] T.Doma
´
nski and K.I.Wysoki
´
nski,“Eﬀect of disorder on
superconductivity in the bosonfermion model,” Physical
Review B,vol.66,no.6,Article ID064517,6 pages,2002.
[224] R.Micnas,S.Robaszkiewicz,and A.BussmannHolder,
“Anisotropic superconductivity in systems with coexisting
electrons and local pairs,” Physical Review B,vol.66,no.10,
Article ID104516,9 pages,2002.
[225] R.Micnas,“Superﬂuid transition temperature of the boson
fermion model on a lattice,” Physical Review B,vol.76,no.
18,Article ID184507,5 pages,2007.
[226] A.S.Alexandrov,“Bosonfermion model beyond the mean
ﬁeld approximation,” Journal of Physics:Condensed Matter,
vol.8,no.37,pp.6923–6932,1996.
[227] A.S.Alexandrov,“Selfenergy catastrophe of the boson
fermion model of hightemperature superconductors,” Phys
ica C,vol.316,no.3,pp.239–242,1999.
[228] T.Egami,“Electronphonon coupling in highT
c
supercon
ductors,” in Superconductivity in Complex Systems,K.A.
M
¨
uller and A.BussmannHolder,Eds.,vol.114 of Structure
and Bonding,p.267,Springer,Berlin,Germany,2005.
[229] M.Fratini,N.Poccia,and A.Bianconi,“The Feshbach
resonance and nanoscale phase separation in a polaron liquid
near the quantumcritical point for a polaronWigner crystal,”
Journal of Physics:Conference Series,vol.108,no.1,Article ID
012036,2008.
[230] A.R.Bishop,“HTC oxides:a collusion of spin,charge and
lattice,” Journal of Physics:Conference Series,vol.108,no.1,
Article ID012027,2008.
[231] A.BussmannHolder and H.Keller,“Unconventional isotope
eﬀects,multicomponent superconductivity and polaron
formation in high temperature cuprate superconductors,”
Journal of Physics:Conference Series,vol.108,no.1,Article
ID012019,2008.
[232] O.Gunnarsson and O.R
¨
osch,“Interplay between electron
phonon and Coulomb interactions in cuprates,” Journal of
Physics:Condensed Matter,vol.20,no.4,Article ID 043201,
2008.
[233] C.S.Ting,D.N.Talwar,and K.L.Ngai,“Possible mecha
nism of superconductivity in metalsemiconductor eutectic
alloys,” Physical ReviewLetters,vol.45,no.14,pp.1213–1216,
1980.
[234] Y.BarYam,“Twocomponent superconductivity.I.Intro
duction and phenomenology,” Physical Review B,vol.43,no.
1,pp.359–377,1991.
[235] Y.BarYam,“Twocomponent superconductivity.II.Copper
oxide highT
c
superconductors,” Physical Review B,vol.43,
no.4,pp.2601–2614,1991.
[236] P.W.Anderson,“Model for the electronic structure of
amorphous semiconductors,” Physical ReviewLetters,vol.34,
no.15,pp.953–955,1975.
[237] G.A.Levin and K.F.Quader,“Tunneling asymmetry in high
T
c
cuprates:possible evidence for a submerged band with
nondegenerate fermions,” Physical Review B,vol.48,no.21,
pp.16184–16187,1993.
[238] K.F.Quader and G.A.Levin,“Origin and consequences of
the ‘gap’ in the cuprate normal state,” Philosophical Magazine
B,vol.74,no.5,pp.611–632,1996.
[239] H.Fr
¨
ohlich,“Superconductivity in metals with incomplete
inner shells,” Journal of Physics C,vol.1,no.2,pp.544–548,
1968.
[240] E.A.Pashitskii,“Plasmon mechanism of superconductivity
in degenerate semiconductors and semimetals.I,” Pis’ma v
Zhurnal Eksperimental’noi i Teoreticheskoi Fiziki,vol.55,p.
2387,1968.
[241] J.Ruvalds,“Are there acoustic plasmons?” Advances in
Physics,vol.30,no.5,pp.677–695,1981.
[242] Y.Takada,“Plasmon mechanismof superconductivity in the
multivalley electron gas,” Journal of the Physical Society of
Japan,vol.61,pp.238–253,1992.
[243] R.Blank and H.Haug,“Theory of plasmonassisted electron
pairing in semiconductors,” Physica Status Solidi B,vol.188,
no.1,pp.105–123,1995.
[244] E.A.Pashitskii,“Low frequency charge density excitations
and highT
c
superconductivity in cuprate metaloxide com
pounds.1.The HTSC problem prior to a discovery of the
highT
c
superconductors:Predictions and premises,” Fizika
Nizkikh Temperatur,vol.21,p.995,1995.
[245] E.A.Pashitskii,“Low frequency charge density excitations
and highT
c
superconductivity in cuprate metaloxide com
pounds.2.The HTSC problem after discovery of high
temperature superconductors:Achievements and outlooks,”
Fizika Nizkikh Temperatur,vol.21,p.1091,1995.
[246] A.Bill,H.Morawitz,and V.Z.Kresin,“Electronic collective
modes and superconductivity in layered conductors,” Phys
ical Review B,vol.68,no.14,Article ID 144519,12 pages,
2003.
[247] E.A.Pashitskii and V.I.Pentegov,“On the plasmon
mechanism of highT
c
superconductivity in layered crystals
and twodimensional systems,” Fizika Nizkikh Temperatur,
vol.34,no.2,pp.148–160,2008.
[248] V.P.Antropov,O.Gunnarsson,and A.I.Liechtenstein,
“Phonons,electronphonon,and electronplasmon coupling
in C
60
compounds,” Physical Review B,vol.48,no.10,pp.
7651–7664,1993.
[249] J.K.Hulm,M.Ashkin,D.W.Deis,and C.K.Jones,inProgress
in Low Temperature Physics,vol.6,p.205,NorthHolland,
Amsterdam,The Netherlands,1970.
[250] V.L.Ginzburg and D.A.Kirzhnitz,Eds.,Problem of
HighTemperature Superconductivity,Nauka,Moscow,Rus
sia,1977.
[251] V.L.Ginzburg and D.A.Kirzhnitz,Eds.,High Temperature
Superconductivity,Consultants Bureau,New York,NY,USA,
1982.
[252] S.A.Nemov and Yu.I.Ravich,“Thallium dopant in
lead chalcogenides:investigation methods and peculiarities,”
Uspekhi Fizicheskikh Nauk,vol.168,p.817,1998.
Advances in Condensed Matter Physics 29
[253] G.Binnig,A.Baratoﬀ,H.E.Hoenig,and J.G.Bednorz,
“Twoband superconductivity in Nbdoped SrTiO
3
,” Physical
Review Letters,vol.45,no.16,pp.1352–1355,1980.
[254] V.A.Moskalenko,“Superconductivity of metals taking into
account the overlap of the energy bands,” Fizika Metallov i
Metallovedenie,vol.8,p.503,1959.
[255] H.Suhl,B.T.Matthias,and L.R.Walker,“Bardeen
CooperSchrieﬀer theory of superconductivity in the case of
overlapping bands,” Physical ReviewLetters,vol.3,no.12,pp.
552–554,1959.
[256] A.M.Gabovich and E.A.Pashitskii,“Superconductivity of
manyvalley semiconductors,” Ukrainskii Fizychnyi Zhurnal,
vol.20,p.1814,1975.
[257] A.L.Kasatkin and E.A.Pashitskii,“Josephson eﬀect in two
band superconductors,” Ukrainskii Fizychnyi Zhurnal,vol.
21,p.578,1976.
[258] L.N.Bulaevskii and M.V.Zyskin,“Energy gap in layered
superconductors,” Physical Review B,vol.42,no.16,pp.
10230–10240,1990.
[259] V.Z.Kresin and S.A.Wolf,“Induced superconducting state
and twogap structure:application to cuprate superconduc
tors and conventional multilayers,” Physical ReviewB,vol.46,
no.10,pp.6458–6471,1992.
[260] S.H.Liu and R.A.Klemm,“Energy gap structure and tun
neling characteristics of layered superconductors,” Physica C,
vol.216,no.34,pp.293–304,1993.
[261] N.Klein,N.Tellmann,H.Schulz,K.Urban,S.A.Wolf,and
V.Z.Kresin,“Evidence of twogap swave superconductivity
in YBa
2
Cu
3
O
7
−
x
from microwave surface impedance mea
surements,” Physical ReviewLetters,vol.71,no.20,pp.3355–
3358,1993.
[262] A.BussmannHolder,L.Genzel,A.Simon,and A.R.Bishop,
“Gap distribution and multigapcoupling in high T
c
’s,”
Zeitschrift f
¨
ur Physik B,vol.92,no.2,pp.149–154,1993.
[263] N.Kristoﬀel,P.Konsin,and T.
¨
Ord,“Twoband model for
hightemperature superconductivity,” La Rivista Del Nuovo
Cimento,vol.17,no.9,pp.1–41,1994.
[264] P.Konsinand B.Sorkin,“Timedependent GinzburgLandau
equations for a twoband superconductor and the relaxation
times of the order parameters in Y
1
−
x
Ca
x
Ba
2
Cu
3
O
7
−
δ
,”
Physica Status Solidi B,vol.244,no.9,pp.3254–3259,2007.
[265] A.BussmannHolder,R.Khasanov,A.Shengelaya,et al.,
“Mixed order parameter symmetries in cuprate supercon
ductors,” Europhysics Letters,vol.77,no.2,Article ID 27002,
4 pages,2007.
[266] O.V.Dolgov,I.I.Mazin,D.Parker,and A.A.Golubov,
“Interband superconductivity:contrasts between Bardeen
CooperSchrieﬀer and Eliashberg theories,” Physical Review
B,vol.79,no.6,Article ID060502,4 pages,2009.
[267] A.Y.Liu,I.I.Mazin,and J.Kortus,“Beyond Eliashberg
superconductivity in MgB
2
:anharmonicity,twophonon
scattering,and multiple gaps,” Physical ReviewLetters,vol.87,
no.8,Article ID087005,4 pages,2001.
[268] I.I.Mazin and V.P.Antropov,“Electronic structure,
electronphonon coupling,and multiband eﬀects in MgB
2
,”
Physica C,vol.385,no.12,pp.49–65,2003.
[269] X.X.Xi,“MgB
2
thin ﬁlms,” Superconductor Science and
Technology,vol.22,no.4,Article ID043001,15 pages,2009.
[270] V.A.Gasparov,N.S.Sidorov,and I.I.Zver’Kova,“Two
gap superconductivity in ZrB
12
:temperature dependence of
critical magnetic ﬁelds in single crystals,” Physical Review B,
vol.73,no.9,Article ID094510,11 pages,2006.
[271] Yu.A.Nefyodov,A.M.Shuvaev,and M.R.Trunin,
“Microwave response of V
3
Si single crystals:evidence for
twogap superconductivity,” Europhysics Letters,vol.72,no.
4,pp.638–644,2005.
[272] I.Bonalde,R.L.Ribeiro,W.Br
¨
amerEscamilla,G.Mu,and
H.H.Wen,“Possible twogap behavior in noncentrosym
metric superconductor Mg
10
Ir
19
B
16
:a penetration depth
study,” Physical Review B,vol.79,no.5,Article ID 052506,
4 pages,2009.
[273] C.L.Huang,J.Y.Lin,C.P.Sun,et al.,“Comparative analysis
of speciﬁc heat of YNi
2
B
2
Cusing nodal and twogap models,”
Physical Review B,vol.73,no.1,Article ID 012502,4 pages,
2006.
[274] C.L.Huang,J.Y.Lin,Y.T.Chang,et al.,“Experimental
evidence for a twogap structure of superconducting NbSe
2
:
a speciﬁcheat study in external magnetic ﬁelds,” Physical
Review B,vol.76,no.21,Article ID212504,4 pages,2007.
[275] M.D.Hossain,Z.Salman,D.Wang,et al.,“Lowﬁeld cross
spin relaxation of
8
Li in superconducting NbSe
2
,” Physical
Review B,vol.79,no.14,Article ID144518,6 pages,2009.
[276] T.Tamegai,Y.Nakajima,T.Nakagawa,G.J.Li,and H.
Harima,“Twogap superconductivity in R
2
Fe
3
Si
5
(R
=
Lu
and Sc),” Journal of Physics:Conference Series,vol.150,Article
ID052264,4 pages,2009.
[277] Y.Nakajima,G.J.Li,and T.Tamegai,“Lowtemperature
speciﬁcheat study of Sc
5
Ir
4
Si
10
,” Journal of Physics:Confer
ence Series,vol.150,Article ID052180,4 pages,2009.
[278] N.E.Phillips,N.Oeschler,R.A.Fisher,J.E.Gordon,M.
L.Foo,and R.J.Cava,“Speciﬁcheat of Na
0.35
CoO
2
.1.3H
2
O:
eﬀects of sample age and pair breaking on twogap supercon
ductivity,” Physica C,vol.460–462,part 1,pp.473–474,2007.
[279] R.S.Gonnelli,M.Tortello,D.Daghero,G.A.Ummarino,
V.A.Stepanov,and J.S.Kim,“Twogap superconductivity
in the Fe1111 superconductor LaFeAsO
1
−
x
F
x
:a point
contact Andreevreﬂection study,” Central European Journal
of Physics,vol.7,no.2,pp.251–256,2009.
[280] P.Samuely,P.Szab
´
o,Z.Pribulov,M.E.Tillman,S.L.Bud’Ko,
and P.C.Canﬁeld,“Possible twogap superconductivity in
NdFeAsO
0.9
F
0.1
probed by pointcontact Andreevreﬂection
spectroscopy,” Superconductor Science and Technology,vol.
22,no.1,Article ID014003,6 pages,2009.
[281] Y.L.Wang,L.Shan,L.Fang,P.Cheng,C.Ren,and H.H.
Wen,“Multiple gaps in SmFeAsO
0.9
F
0.1
revealed by point
contact spectroscopy,” Superconductor Science and Technol
ogy,vol.22,no.1,Article ID015018,6 pages,2009.
[282] P.Szab
´
o,Z.Pribulov
´
a,G.Prist
´
a
ˇ
s,S.L.Bud’ko,P.C.Canﬁeld,
and P.Samuely,“Evidence for twogap superconductivity
in Ba
0.55
K
0.45
Fe
2
As
2
fromdirectional pointcontact Andreev
reﬂection spectroscopy,” Physical Review B,vol.79,no.1,
Article ID012503,4 pages,2009.
[283] R.Khasanov,D.V.Evtushinsky,A.Amato,et al.,“Twogap
superconductivity in Ba
1
−
x
K
x
Fe
2
As
2
:a complementary study
of the magnetic penetration depth by muonspin rotation
and angleresolved photoemission,” Physical Review Letters,
vol.102,no.18,Article ID187005,4 pages,2009.
[284] A.I.Golovashkin and A.N.Lykov,“Gap peculiarities of the
currentvoltage characteristics of superconducting contacts
with direct conductivity,” Trudy Fiz.Inst.Akad.Nauk SSSR,
vol.190,p.144,1988.
[285] A.Sharoni,I.Felner,and O.Millo,“Tunneling spectroscopy
and magnetization measurements of the superconducting
properties of MgB
2
,” Physical ReviewB,vol.63,no.22,Article
ID220508,4 pages,2001.
30 Advances in Condensed Matter Physics
[286] T.Takasaki,T.Ekino,T.Muranaka,H.Fujii,and J.Akimitsu,
“Superconducting gap in polycrystalline MgB
2
studied by
electron tunneling,” Physica C,vol.378–381,part 1,pp.229–
233,2002.
[287] Yu.G.Naidyuk,I.K.Yanson,L.V.Tyutrina,et al.,“
Superconducting energy gap distribution in caxis oriented
MgB
2
thin ﬁlm from point contact study,” JETP Letters,vol.
75,no.5,pp.238–241,2002.
[288] H.Schmidt,J.F.Zasadzinski,K.E.Gray,and D.G.Hinks,
“Breakjunction tunneling on MgB
2
,” Physica C,vol.385,no.
12,pp.221–232,2003.
[289] T.Ekino,T.Takasaki,T.Muranaka,J.Akimitsu,and H.
Fujii,“Tunneling spectroscopy of the superconducting gap
in MgB
2
,” Physical ReviewB,vol.67,no.9,Article ID094504,
2003.
[290] B.Barbiellini,O.Fischer,M.Peter,Ch.Renner,andM.Weger,
“Gap distribution of the tunneling spectra in Bi
2
Sr
2
CaCu
2
O
x
and some other superconductors,” Physica C,vol.220,no.1
2,pp.55–60,1994.
[291] M.C.Boyer,W.D.Wise,K.Chatterjee,et al.,“Imag
ing the two gaps of the hightemperature superconductor
Bi
2
Sr
2
CuO
6+x
,” Nature Physics,vol.3,no.11,pp.802–806,
2007.
[292] C.E.Gough,M.S.Colclough,E.M.Forgan,et al.,“Flux
quantization in a highT
c
superconductor,” Nature,vol.326,
no.6116,p.855,1987.
[293] M.N.Keene,T.J.Jackson,and C.E.Gough,“Demonstration
of the phase coherence of the superconducting wavefunctions
betweenconventional andhighT
c
superconductors,” Nature,
vol.340,no.6230,pp.210–211,1989.
[294] E.Dagotto,“Correlated electrons in hightemperature super
conductors,” Reviews of Modern Physics,vol.66,no.3,pp.
763–840,1994.
[295] A.P.Kampf,“Magnetic correlations in high temperature
superconductivity,” Physics Reports,vol.249,no.45,pp.
219–351,1994.
[296] W.Brenig,“Aspects of electron correlations in the cuprate
superconductors,” Physics Reports,vol.251,no.34,pp.153–
266,1995.
[297] M.Imada,A.Fujimori,and Y.Tokura,“Metalinsulator
transitions,” Reviews of Modern Physics,vol.70,no.4,pp.
1039–1263,1998.
[298] S.Sachdev,“Colloquium:order and quantum phase tran
sitions in the cuprate superconductors,” Reviews of Modern
Physics,vol.75,no.3,pp.913–932,2003.
[299] E.Demler,W.Hanke,and S.C.Zhang,“SO(5) theory
of antiferromagnetism and superconductivity,” Reviews of
Modern Physics,vol.76,no.3,pp.909–974,2004.
[300] T.Schneider,in The Physics of Superconductors.Vol.I:Con
ventional and HighT
c
Superconductors,K.H.Bennemann
and J.B.Ketterson,Eds.,p.111,Springer,Berlin,Germany,
2004.
[301] T.Schneider and H.Keller,“Implications evinced by the
phase diagram,anisotropy,magnetic penetrationdepths,iso
tope eﬀects and conductivities of cuprate superconductors,”
New Journal of Physics,vol.6,Article ID144,18 pages,2004.
[302] P.A.Lee,N.Nagaosa,and X.G.Wen,“Doping a Mott
insulator:physics of hightemperature superconductivity,”
Reviews of Modern Physics,vol.78,no.1,Article ID 17,69
pages,2006.
[303] K.M.Shen and J.C.S.Davis,“Cuprate highT
c
supercon
ductors,” Materials Today,vol.11,no.9,pp.14–21,2008.
[304] H.Alloul,J.Bobroﬀ,M.Gabay,and P.J.Hirschfeld,
“Defects in correlated metals and superconductors,” Reviews
of Modern Physics,vol.81,no.1,Article ID45,64 pages,2009.
[305] D.J.Scalapino,“The case for d
x2
−
y2
pairing in the cuprate
superconductors,” Physics Reports,vol.250,no.6,pp.329–
365,1995.
[306] J.F.Annett,N.D.Goldenfeld,and A.J.Leggett,“Experi
mental constraints on the pairing state of the cuprate super
conductors:an emerging consensus,” in Physical Properties of
High Temperature Superconductors V,D.M.Ginsberg,Ed.,p.
375,World Scientiﬁc,River Ridge,NJ,USA,1996.
[307] D.Pines,“Understanding high temperature superconduc
tors:progress and prospects,” Physica C,vol.282–287,part
1,pp.273–278,1997.
[308] T.S.Nunner,J.Schmalian,and K.H.Bennemann,“Inﬂuence
of electronphonon interaction on spinﬂuctuationinduced
superconductivity,” Physical Review B,vol.59,no.13,pp.
8859–8868,1999.
[309] D.Manske,I.Eremin,and K.H.Bennemann,“Theory for
electrondoped cuprate superconductors:dwave symmetry
order parameter,” Physical Review B,vol.62,no.21,pp.
13922–13925,2000.
[310] T.Dahm,V.Hinkov,S.V.Borisenko,et al.,“Strength of
the spinﬂuctuationmediated pairing interaction in a high
temperature superconductor,” Nature Physics,vol.5,no.3,
pp.217–221,2009.
[311] M.L.Cohen,“Electronphononinduced superconductiv
ity,” Journal of Superconductivity and Novel Magnetism,vol.
19,no.3–5,pp.283–290,2006.
[312] G.Varelogiannis,“Phononmediated unconventional super
conductivity in strongly correlated systems,” Physical Review
B,vol.57,no.21,pp.13743–13764,1998.
[313] G.Varelogiannis,“Smallq electronphonon interaction and
the phase diagramof the cuprates,” Physica C,vol.460–462,
part 2,pp.1125–1126,2007.
[314] A.S.Alexandrov,“dwave checkerboard bose condensate of
mobile bipolarons,” International Journal of Modern Physics
B,vol.21,no.1314,pp.2301–2312,2007.
[315] H.Kamimura and H.Ushio,“On the interplay of JahnTeller
physics and Mott physics in cuprates,” Journal of Physics:
Conference Series,vol.108,no.1,Article ID012030,2008.
[316] A.S.Alexandrov,“Unconventional pairs glued by con
ventional phonons in cuprate superconductors,” Journal of
Superconductivity and Novel Magnetism,vol.22,no.2,pp.
103–107,2009.
[317] E.A.Pashitskii and V.I.Pentegov,“The role of the charge
density ﬂuctuations and manybody Coulomb correlations
in the mechanismof hightemperature superconductivity in
cuprate metaloxides,” Fizika Nizkikh Temperatur,vol.27,no.
2,pp.140–152,2001.
[318] H.B.Sch
¨
uttler and C.H.Pao,“Isotope eﬀect in dwave
superconductors,” Physical Review Letters,vol.75,no.24,pp.
4504–4507,1995.
[319] Yu.Bang,“Eﬀects of phonon interaction on pairing in high
T
c
superconductors,” Physical ReviewB,vol.78,no.7,Article
ID075116,2008.
[320] A.I.Lichtenstein and M.L.Kuli
´
c,“Electronboson inter
action can help d wave pairing selfconsistent approach,”
Physica C,vol.245,no.12,pp.186–192,1995.
[321] T.Egami,P.Piekarz,and J.H.Chung,“Role of phonons
in the mechanism of hightemperature superconductivity,”
Physica C,vol.408–410,no.1–4,pp.292–295,2004.
Advances in Condensed Matter Physics 31
[322] E.G.Maksimov,“Electronphonon interaction and super
conductivity,” Trudy Fiz.Inst.Akad.Nauk SSSR,vol.86,p.
101,1975.
[323] L.Tonks and I.Langmuir,“Oscillations in ionized gases,”
Physical Review,vol.33,no.2,pp.195–210,1929.
[324] D.Bohm and T.Staver,“Application of collective treatment
of electron and ion vibrations to theories of conductivity and
superconductivity,” Physical Review,vol.84,no.4,pp.836–
837,1951.
[325] V.P.Silin and A.A.Rukhadze,Electromagnetic Properties
of Plasma and PlasmaLike Media,Gosatomizdat,Moscow,
Russia,1961.
[326] E.G.Brovman and Yu.M.Kagan,“Phonons in non
transition metals,” Uspekhi Fizicheskikh Nauk,vol.112,p.
369,1974.
[327] B.T.Geilikman,“Adiabatic perturbation theory for metals
and the problemof the lattice stability,” Uspekhi Fizicheskikh
Nauk,vol.115,p.403,1975.
[328] M.A.Eggington and A.J.Leggett,“Is ODLRO a necessary
condition for superﬂuidity?” Collective Phenomena,vol.2,p.
81,1975.
[329] B.T.Geilikman,Studies in LowTemperature Physics,Atomiz
dat,Moscow,Russia,1979.
[330] V.M.Kontorovich,“Dynamical equations of the elasticity
theory in metals,” Uspekhi Fizicheskikh Nauk,vol.142,p.265,
1984.
[331] S.Yu.Savrasov and E.G.Maksimov,“Ab initio calculations of
the lattice dynamics of crystals,” Uspekhi Fizicheskikh Nauk,
vol.165,p.773,1995.
[332] E.G.Maksimov,D.Yu.Savrasov,and S.Yu.Savrasov,
“Electronphonon interaction and physical properies of
metals,” Uspekhi Fizicheskikh Nauk,vol.167,p.353,1997.
[333] E.G.Maksimov and A.E.Karakozov,“On nonadiabatic
eﬀects in phonon spectra of metals,” Uspekhi Fizicheskikh
Nauk,vol.178,p.561,2008.
[334] J.Lee,K.Fujita,K.McElroy,et al.,“Interplay of
electronglattice interactions and superconductivity in
Bi
2
Sr
2
CaCu
2
O
8+δ
,” Nature,vol.442,no.7102,pp.546–550,
2006.
[335] D.Reznik,L.Pintschovius,M.Ito,et al.,“Electronphonon
coupling reﬂecting dynamic charge inhomogeneity in copper
oxide superconductors,” Nature,vol.440,no.7088,pp.1170–
1173,2006.
[336] K.McElroy,J.Lee,J.A.Slezak,et al.,“Atomicscale
sources and mechanism of nanoscale electronic disorder in
Bi
2
Sr
2
CaCu
2
O
8+δ
,” Science,vol.309,no.5737,pp.1048–
1052,2005.
[337] D.Mihailovic and V.V.Kabanov,“Dynamic inhomogeneity,
pairing and superconductivity in cuprates,” in Superconduc
tivity in Complex Systems,K.A.Muller and A.Bussmann
Holder,Eds.,vol.114 of Structure and Bonding,p.331,
Springer,Berlin,Germany,2005.
[338] A.Sugimoto,S.Kashiwaya,H.Eisaki,et al.,“Enhancement
of electronic inhomogeneities due to outofplane disorder
in Bi
2
Sr
2
CuO
6+δ
superconductors observed by scanning
tunneling spectroscopy,” Physical Review B,vol.74,no.9,
Article ID094503,2006.
[339] A.Yazdani,“Visualizing pair formation on the atomic scale
and the search for the mechanism of superconductivity in
highT
c
cuprates,” Journal of Physics:Condensed Matter,vol.
21,no.16,Article ID164214,2009.
[340] T.Kato,T.Machida,Y.Kamijo,R.Miyashita,and H.Sakata,
“Spatial correlation between the LDOS modulation and
electronic inhomogeneity in Bi
2
Sr
2
−
x
La
x
CuO
6+δ
,” Journal of
Physics:Conference Series,vol.150,Article ID 052101,4
pages,2009.
[341] K.Kudo,T.Nishizaki,N.Okumura,and N.Kobayashi,
“Electronic inhomogeneity in Pbsubstituted Bi
2
Sr
2
CuO
6+δ
studied by STM/STS measurements,” Journal of Physics:
Conference Series,vol.150,Article ID052133,4 pages,2009.
[342] M.Suzuki,T.Hamatani,Y.Yamada,K.Anagawa,and T.
Watanabe,“Signiﬁcantly dopingdependent Josephson criti
cal current—inhomogeneity in real space or heterogeneity in
kspace,” Journal of Physics:Conference Series,vol.150,Article
ID052252,4 pages,2009.
[343] W.D.Wise,K.Chatterjee,M.C.Boyer,et al.,“Imaging
nanoscale Fermisurface variations in an inhomogeneous
superconductor,” Nature Physics,vol.5,no.3,pp.213–216,
2009.
[344] W.D.Wise,M.C.Boyer,K.Chatterjee,et al.,“Charge
densitywave origin of cuprate checkerboard visualized by
scanning tunnelling microscopy,” Nature Physics,vol.4,no.
9,pp.696–699,2008.
[345] X.M.Li,F.H.Li,H.Q.Luo,L.Fang,and H.H.Wen,“Trans
mission electron microscopy study of onedimensional
incommensurate structural modulation in superconducting
oxides Bi
2+x
Sr
2
−
x
CuO
6+δ
(0.10
≤
x
≤
0.40),” Superconductor
Science and Technology,vol.22,no.6,Article ID 065003,
2009.
[346] A.Mourachkine,HighTemperature Superconductivity in
Cuprates,Kluwer Academic Publishers,Dordrecht,The
Netherlands,2002.
[347] J.F.Zasadzinski,“Tunneling spectroscopy of conventional
and unconventional superconductors,” in The Physics of
Superconductors.Vol.1:Conventional and HighT
c
Supercon
ductors,K.H.Bennemann and J.B.Ketterson,Eds.,p.591,
Springer,Berlin,Germany,2003.
[348] ∅.Fischer,M.Kugler,I.MaggioAprile,C.Berthod,and
C.Renner,“Scanning tunneling spectroscopy of high
temperature superconductors,” Reviews of Modern Physics,
vol.79,no.1,pp.353–419,2007.
[349] V.M.Krasnov,A.Yurgens,D.Winkler,P.Delsing,and T.
Claeson,“Evidence for coexistence of the superconducting
gap and the pseudogap in Bi2212 from intrinsic tunneling
spectroscopy,” Physical Review Letters,vol.84,no.25,pp.
5860–5863,2000.
[350] M.Oda,Y.H.Liu,T.Kurosawa,K.Takeyama,N.Momono,
and M.Ido,“On the relations among the pseudogap,
electronic charge order and Fermiarc superconductivity in
Bi
2
Sr
2
CaCu
2
O
8+δ
,” Journal of Physics:Conference Series,vol.
108,Article ID012008,6 pages,2008.
[351] K.Tanaka,W.S.Lee,Z.Hussain,and Z.X.Shen,“Direct
evidence of two gaps in underdoped Bi2212,” Journal of
Physics:Conference Series,vol.108,no.1,Article ID 012014,
2008.
[352] A.A.Kordyuk,S.V.Borisenko,V.B.Zabolotnyy,et al.,
“Nonmonotonic pseudogap in highT
c
cuprates,” Physical
Review B,vol.79,no.2,Article ID020504,2009.
[353] W.S.Lee,I.M.Vishik,D.H.Lu,and Z.X.Shen,“A brief
update of angleresolved photoemission spectroscopy on a
correlated electron system,” Journal of Physics:Condensed
Matter,vol.21,no.16,Article ID164217,2009.
[354] R.H.He,K.Tanaka,S.K.Mo,et al.,“Energy gaps in the
failed highT
c
superconductor La
1.875
Ba
0.125
CuO
4
,” Nature
Physics,vol.5,no.2,pp.119–123,2009.
[355] J.Meng,W.Zhang,G.Liu,et al.,“Monotonic dwave super
conducting gap of the optimally doped Bi
2
Sr
1.6
La
0.4
CuO
6
superconductor by laserbased angleresolved photoemission
32 Advances in Condensed Matter Physics
spectroscopy,” Physical Review B,vol.79,no.2,Article ID
024514,2009.
[356] T.Kondo,R.Khasanov,T.Takeuchi,J.Schmalian,and
A.Kaminski,“Competition between the pseudogap and
superconductivity in the highT
c
copper oxides,” Nature,vol.
457,no.7227,pp.296–300,2009.
[357] M.L.Teague,A.D.Beyer,M.S.Grinolds,S.I.Lee,and N.
C.Yeh,“Observation of vortices and hidden pseudogap from
scanning tunneling spectroscopic studies of the electron
doped cuprate superconductor Sr
0.9
La
0.1
CuO
2
,” Europhysics
Letters,vol.85,no.1,Article ID17004,2009.
[358] A.Sugimoto,K.Shohara,T.Ekino,et al.,“Scanning tun
neling microscopy/spectroscopy on multilayered cuprate
superconductor Ba
2
Ca
5
Cu
6
O
12
(O
1
−
x
F
x
)
2
,” Physica C,vol.
469,no.15–20,pp.1020–1023,2009.
[359] K.Mcelroy,D.H.Lee,J.E.Hoﬀman,et al.,“Coincidence of
checkerboard charge order and antinodal state decoherence
in strongly underdoped superconducting Bi
2
Sr
2
CaCu
2
O
8+δ
,”
Physical Review Letters,vol.94,no.19,Article ID 197005,
2005.
[360] J.P.Castellan,B.D.Gaulin,H.A.Dabkowska,et al.,
“Two and threedimensional incommensurate modulation
in optimallydoped Bi
2
Sr
2
CaCu
2
O
8+δ
,” Physical Review B,
vol.73,no.17,Article ID174505,2006.
[361] J.Etrillard,P.Bourges,and C.T.Lin,“Incommensurate com
posite structure of the superconductor Bi
2
Sr
2
CaCu
2
O
8+δ
,”
Physical Review B,vol.62,no.1,pp.150–153,2000.
[362] G.Kinoda,T.Hasegawa,S.Nakao,et al.,“Electronic struc
tures of twophase microstructures α and β in heavily Pb
doped Bi
2
Sr
2
CaCu
2
O
y
single crystals investigated by scan
ning tunneling microscopy/spectroscopy,” Applied Physics
Letters,vol.83,no.6,pp.1178–1180,2003.
[363] A.Sugimoto,S.Kashiwaya,H.Eisaki,et al.,“Correlation
between modulation structure and electronic inhomogeneity
on Pbdoped Bi2212 single crystals,” Physica C,vol.426–
431,part 1,pp.390–395,2005.
[364] M.Vershinin,S.Misra,S.Ono,Y.Abe,Y.Ando,and A.
Yazdani,“Local ordering in the pseudogap state of the high
T
c
superconductor Bi
2
Sr
2
CaCu
2
O
8+δ
,” Science,vol.303,no.
5666,pp.1995–1998,2004.
[365] A.Bianconi,M.Lusignoli,N.L.Saini,P.Bordet,A.Kvick,
and P.G.Radaelli,“Stripe structure of the CuO
2
plane in
Bi
2
Sr
2
CaCu
2
O
8+y
by anomalous Xray diﬀraction,” Physical
Review B,vol.54,no.6,pp.4310–4314,1996.
[366] E.V.L.de Mello and E.S.Caixeiro,“The theory of local
superconductivity and phase separation applied to cuprates,”
Journal of Superconductivity,vol.18,no.56,pp.53–57,2005.
[367] V.Z.Kresin,Yu.N.Ovchinnikov,and S.A.Wolf,“Inhomoge
neous superconductivity and the “pseudogap” state of novel
superconductors,” Physics Reports,vol.431,no.5,pp.231–
259,2006.
[368] J.E.Hoﬀman,E.W.Hudson,K.M.Lang,et al.,“A four
unit cell periodic pattern of quasiparticle states surrounding
vortex cores in Bi
2
Sr
2
CaCu
2
O
8+δ
,” Science,vol.295,no.5554,
pp.466–469,2002.
[369] N.Momono,A.Hashimoto,Y.Kobatake,S.Nakamura,M.
Oda,and M.Ido,“STM/STS study on local electronic states
of underdoped Bi
2
Sr
2
CaCu
2
O
8+δ
,” International Journal of
Modern Physics B,vol.19,no.1–3,pp.231–234,2005.
[370] A.Hashimoto,N.Momono,M.Oda,and M.Ido,“Scanning
tunneling microscopy and spectroscopy study of 4a
×
4a
electronic charge order and the inhomogeneous pairing gap
in superconducting Bi
2
Sr
2
CaCu
2
O
8+δ
,” Physical Review B,
vol.74,no.6,Article ID064508,2006.
[371] K.M.Shen,F.Ronning,D.H.Lu,et al.,“Nodal quasipar
ticles and antinodal charge ordering in Ca
2
−
x
Na
x
CuO
2
Cl
2
,”
Science,vol.307,no.5711,pp.901–904,2005.
[372] J.A.Robertson,S.A.Kivelson,E.Fradkin,A.C.Fang,and A.
Kapitulnik,“Distinguishing patterns of charge order:stripes
or checkerboards,” Physical Review B,vol.74,no.13,Article
ID134507,2006.
[373] W.Meevasana,N.J.C.Ingle,D.H.Lu,et al.,“Doping
dependence of the coupling of electrons to bosonic modes in
the singlelayer hightemperature Bi
2
Sr
2
CaCuO
6
supercon
ductor,” Physical Review Letters,vol.96,no.15,Article ID
157003,2006.
[374] D.S.Inosov,V.B.Zabolotnyy,D.V.Evtushinsky,et al.,
“Fermi surface nesting in several transition metal dichalco
genides,” New Journal of Physics,vol.10,Article ID 125027,
2008.
[375] S.V.Borisenko,A.A.Kordyuk,V.B.Zabolotnyy,et al.,“Two
energy gaps and fermisurface “arcs” in NbSe
2
,” Physical
Review Letters,vol.102,no.16,Article ID166402,2009.
[376] D.S.Inosov,D.V.Evtushinsky,V.B.Zabolotnyy,et al.,
“Temperaturedependent Fermi surface of 2HTaSe
2
driven
by competing density wave order ﬂuctuations,” Physical
Review B,vol.79,no.12,Article ID125112,2009.
[377] A.M.Gabovich,V.A.Medvedev,D.P.Moiseev,et al.,
“Superconductivity and thermal anomalies in the properties
of the crystal lattice of the metal oxide La
1.8
Ba
0.2
CuO
4
,” Fizika
Nizkikh Temperatur,vol.13,no.8,pp.844–847,1987.
[378] R.A.Klemm,“Striking similarities between the pseudogap
phenomena in cuprates and in layered organic and dichalco
genide superconductors,” Physica C,vol.341–348,pp.839–
842,2000.
[379] R.A.Klemm,“Origin of the pseudogap in high temperature
superconductors,” in Nonequilibrium Physics at Short Time
Scales:Formation of Correlations,K.Morawetz,Ed.,p.381,
Springer,Berlin,Germany,2004.
[380] E.Morosan,H.W.Zandbergen,B.S.Dennis,et al.,
“Superconductivity in Cu
x
TiSe
2
,” Nature Physics,vol.2,no.
8,pp.544–550,2006.
[381] S.L.Bud’ko,P.C.Canﬁeld,E.Morosan,R.J.Cava,and G.M.
Schmiedeshoﬀ,“Thermal expansionand eﬀect of pressure on
superconductivity inCu
x
TiSe
2
,” Journal of Physics:Condensed
Matter,vol.19,Article ID176230,8 pages,2005.
[382] M.V.Kartsovnik,D.Andres,W.Biberacher,P.D.Grigoriev,
E.A.Schuberth,and H.M
¨
uller,“New electronic phase tran
sitions in α(BEDTTTF)
2
KHg(SCN)
4
,” Journal de Physique
IV,vol.114,pp.191–197,2004.
[383] D.Graf,J.S.Brooks,M.Almeida,et al.,“Evolution of
superconductivity from a chargedensitywave ground state
in pressurized (Per)
2
[Au(mnt)
2
],” Europhysics Letters,vol.85,
no.2,Article ID27009,2009.
[384] J.J.Hamlin,D.A.Zocco,T.A.Sayles,M.B.Maple,J.H.Chu,
and I.R.Fisher,“Pressureinduced superconducting phase
in the chargedensitywave compound terbium tritelluride,”
Physical Review Letters,vol.102,no.17,Article ID 177002,
2009.
[385] G.Bilbro and W.L.McMillan,“Theoretical model of
superconductivity and the martensitic transformation in A15
compounds,” Physical ReviewB,vol.14,no.5,pp.1887–1892,
1976.
[386] A.M.Gabovich,M.S.Li,H.Szymczak,and A.I.Voitenko,
“Thermodynamics of superconductors with chargedensity
waves,” Journal of Physics:Condensed Matter,vol.15,no.17,
pp.2745–2753,2003.
Advances in Condensed Matter Physics 33
[387] N.Oeschler,R.A.Fisher,N.E.Phillips,J.E.Gordon,M.L.
Foo,and R.J.Cava,“Speciﬁc heat of Na
0.3
CoO
2
·
1.3H
2
O:two
energy gaps,nonmagnetic pair breaking,strong ﬂuctuations
in the superconducting state,and eﬀects of sample age,”
Physical Review B,vol.78,no.5,Article ID054528,2008.
[388] H.Fu,N.Oeschler,R.A.Fisher,et al.,“Competition
between superconductivity and chargedensity wave order in
Na
0.3
CoO
2
·
1.3H
2
O,” Journal of Superconductivity and Novel
Magnetism,vol.22,no.3,pp.295–298,2009.
[389] N.E.Phillips,R.A.Fisher,H.Fu,et al.,“Superconductivity
and chargedensitywave order in Na
0.3
CoO
2
·
1.3H
2
O,”
Journal of Physics:Conference Series,vol.150,Article ID
052210,2009.
[390] M.S.Li,“Paramagnetic Meissner eﬀect and related dynami
cal phenomena,” Physics Reports,vol.376,no.3,pp.133–223,
2003.
[391] G.K.Perkins,Y.Bugoslavsky,A.D.Caplin,et al.,“Eﬀects
of proton irradiation and ageing on the superconducting
properties of single crystalline and polycrystalline MgB
2
,”
Superconductor Science and Technology,vol.17,no.1,pp.
232–235,2004.
[392] A.M.Gabovich,D.P.Moiseev,L.V.Prokopovich,S.K.
Uvarova,and V.E.Yachmenev,“Experimental proof of
bulk superconductivity in perovskite systemBaPb
1
−
x
Bi
x
O
3
,”
Zhurnal
´
Eksperimental’noi i Teoreticheskoi Fiziki,vol.86,p.
1727,1984.
[393] I.R.Gomersall and B.L.Gyorﬀy,“On the connection
between high superconducting transition temperature,T
c
,
and lattice instability in transition metal compounds:NbN,”
Journal of Physics F,vol.3,pp.L138–L144,1973.
[394] J.C.Phillips,“Lattice instabilities and hightemperature
superconductivity,” Physical Review Letters,vol.26,no.10,
pp.543–546,1971.
[395] I.Nakayama,“Structural transformation and superconduc
tivity in A15 compounds,” Journal of the Physical Society of
Japan,vol.43,p.1533,1977.
[396] A.M.Gabovich,D.P.Moiseev,and A.S.Shpigel,“The
nature of superconductivity for solid solutions BaPb
1
−
x
Bi
x
O
3
with a perovskite structure.Role of the electron spectrum
dielectrization,” Zhurnal
´
Eksperimental’noi i Teoreticheskoi
Fiziki,vol.83,p.1383,1982.
[397] A.M.Gabovich and A.S.Shpigel,“Thermodynamics
of superconductors with charge and spindensity waves,”
Journal of Physics F,vol.14,no.12,pp.3031–3039,1984.
[398] A.M.Gabovich,“Partial dielectrization model for oxide
superconductivity,” inHighT
c
Superconductivity,Experiment
and Theory,A.S.Davydov and V.M.Loktev,Eds.,pp.161–
169,Springer,Berlin,Germany,1992.
[399] T.Ekino,Y.Sezaki,and H.Fujii,“Features of the energy
gap above T
c
in Bi
2
Sr
2
CaCu
2
O
8+δ
as seen by breakjunction
tunneling,” Physical Review B,vol.60,no.9,pp.6916–6922,
1999.
[400] J.Demsar,R.Hudej,J.Karpinski,V.V.Kabanov,and
D.Mihailovic,“Quasiparticle dynamics and gap structure
in HgBa
2
Ca
2
Cu
3
O
8+δ
investigated with femtosecond spec
troscopy,” Physical ReviewB,vol.63,no.5,Article ID054519,
7 pages,2001.
[401] M.Le Tacon,A.Sacuto,A.Georges,et al.,“Two energy scales
and two distinct quasiparticle dynamics in the superconduct
ing state of underdoped cuprates,” Nature Physics,vol.2,no.
8,pp.537–543,2006.
[402] K.Tanaka,W.S.Lee,D.H.Lu,et al.,“Distinct fermi
momentumdependent energy gaps in deeply underdroped
Bi2212,” Science,vol.314,no.5807,pp.1910–1913,2006.
[403] W.S.Lee,I.M.Vishik,K.Tanaka,et al.,“Abrupt onset of
a second energy gap at the superconducting transition of
underdoped Bi2212,” Nature,vol.450,no.7166,pp.81–84,
2007.
[404] T.Das,R.S.Markiewicz,and A.Bansil,“Competing
order scenario of twogap behavior in holedoped cuprates,”
Physical Review B,vol.77,no.13,Article ID134516,2008.
[405] V.J.Emery and S.A.Klvelson,“Importance of phase ﬂuc
tuations in superconductors with small superﬂuid density,”
Nature,vol.374,no.6521,pp.434–437,1995.
[406] M.R.Norman,D.Pines,and C.Kallin,“The pseudogap:
friend or foe of high T
c
?” Advances in Physics,vol.54,no.
8,pp.715–733,2005.
[407] T.Valla,A.V.Fedorov,J.Lee,J.C.Davis,and G.D.Gu,“The
ground state of the pseudogap in cuprate supercondustors,”
Science,vol.314,no.5807,pp.1914–1916,2006.
[408] A.Kanigel,U.Chatterjee,M.Randeria,et al.,“Protected
nodes and the collapse of fermi arcs in highT
c
cuprate
superconductors,” Physical Review Letters,vol.99,no.15,
Article ID157001,2007.
[409] A.Kanigel,U.Chatterjee,M.Randeria,et al.,“Evidence for
pairing above the transition temperature of cuprate super
conductors from the electronic dispersion in the pseudogap
phase,” Physical Review Letters,vol.101,no.13,Article ID
137002,2008.
[410] H.B.Yang,J.D.Rameau,P.D.Johnson,T.Valla,A.Tsvelik,
and G.D.Gu,“Emergence of preformed cooper pairs from
the doped Mott insulating state in Bi
2
Sr
2
CaCu
2
O
8+δ
,” Nature,
vol.456,no.7218,pp.77–80,2008.
[411] M.Shi,J.Chang,S.Pailh
´
es,et al.,“Coherent dWave
superconducting gap in underdoped La
2
−
x
Sr
x
CuO
4
by angle
resolved photoemission spectroscopy,” Physical Review Let
ters,vol.101,no.4,Article ID047002,2008.
[412] S.H
¨
ufner and F.M
¨
uller,“Temperature dependence of the
gaps of hightemperature superconductors in the Fermiarc
region,” Physical Review B,vol.78,no.1,Article ID 014521,
2008.
[413] S.H
¨
ufner,M.A.Hossain,A.Damascelli,and G.A.Sawatzky,
“Two gaps make a hightemperature superconductor?”
Reports on Progress in Physics,vol.71,no.6,Article ID
062501,2008.
[414] K.Nakayama,T.Sato,Y.Sekiba,et al.,“Evolution of a
pairinginduced pseudogap fromthe superconducting gap of
(Bi,Pb)
2
Sr
2
CuO
6
,” Physical Review Letters,vol.102,no.22,
Article ID227006,2009.
[415] C.C.Chien,Y.He,Q.Chen,and K.Levin,“Twoenergygap
preformedpair scenario for cuprate superconductors:impli
cations for angleresolved photoemission spectroscopy,”
Physical Review B,vol.79,no.21,Article ID214527,2009.
[416] J.Lee,K.Fujita,A.R.Schmidt,et al.,“Spectroscopic
ﬁngerprint of phaseincoherent superconductivity in the
underdoped Bi
2
Sr
2
CaCu
2
O
8+δ
,” Science,vol.325,no.5944,
pp.1099–1103,2009.
[417] V.M.Krasnov,“Interlayer tunneling spectroscopy of
Bi
2
Sr
2
CaCu
2
O
8+δ
:a look from inside on the doping phase
diagramof highT
c
superconductors,” Physical ReviewB,vol.
65,no.14,Article ID140504,4 pages,2002.
[418] E.E.M.Chia,J.X.Zhu,D.Talbayev,et al.,“Observation
of competing order in a highT
c
superconductor using
femtosecond optical pulses,” Physical Review Letters,vol.99,
no.14,Article ID147008,2007.
[419] M.Hashimoto,T.Yoshida,A.Fujimori,et al.,“Eﬀects
of outofplane disorder on the nodal quasiparticle and
superconducting gap in singlelayer Bi
2
Sr
1.6
L
0.4
CuO
6+δ
34 Advances in Condensed Matter Physics
(L
=
La,Nd,Gd),” Physical Review B,vol.79,no.14,Article
ID144517,2009.
[420] V.M.Krasnov,A.E.Kovalev,A.Yurgens,and D.Winkler,
“Magnetic ﬁeld dependence of the superconducting gap and
the pseudogap in Bi2212 and HgBr
2
Bi2212,studied by
intrinsic tunneling spectroscopy,” Physical ReviewLetters,vol.
86,no.12,pp.2657–2660,2001.
[421] D.E.Moncton,J.D.Axe,and F.J.DiSalvo,“Neutron
scattering study of the chargedensity wave transitions in
2HTaSe
2
and 2HNbSe
2
,” Physical Review B,vol.16,no.2,
pp.801–819,1977.
[422] K.Machida,“Spin density wave and superconductivity in
highly anisotropic materials,” Journal of the Physical Society
of Japan,vol.50,pp.2195–2202,1981.
[423] K.Machida and T.Matsubara,“Spin density wave and super
conductivity in highly anisotropic materials.II.Detailed
study of phase transitions,” Journal of the Physical Society of
Japan,vol.50,p.3231,1981.
[424] K.Machida,“Spin density wave and superconductivity in
highly anisotropic materials.III.Energy gap structure and
nonmagnetic impurity eﬀects,” Journal of the Physical Society
of Japan,vol.51,p.1420,1982.
[425] A.M.Gabovich,D.P.Moiseev,and A.S.Shpigel,
“Thermodynamic properties of superconducting ceramics
BaPb
1
−
x
Bi
x
O
3
,” Journal of Physics C,vol.15,no.18,pp.L569–
L572,1982.
[426] A.M.Gabovich and A.S.Shpigel,“Inﬂuence of impurity
scattering on the critical temperature of superconductors
with a partial gap in the electron spectrum,” Journal of Low
Temperature Physics,vol.51,no.56,pp.581–599,1983.
[427] A.M.Gabovich,A.S.Gerber,and A.S.Shpigel,“Thermo
dynamics of superconductors with charge and spindensity
waves,” Physica Status Solidi B,vol.141,no.2,pp.575–587,
1987.
[428] A.M.Gabovich and A.S.Shpigel,“Upper critical magnetic
ﬁeld of superconductors with a dielectric gap on the Fermi
surface sections,” Physical Review B,vol.38,no.1,pp.297–
306,1988.
[429] K.Levin,D.L.Mills,and S.L.Cunningham,“Incompatibility
of BCS pairing and the Peierls distortion in onedimensional
systems.I.Meanﬁeld theory,” Physical Review B,vol.10,no.
9,pp.3821–3831,1974.
[430] K.Levin,S.L.Cunningham,and D.L.Mills,“Incompatibility
of BCS pairing and the Peierls distortion in onedimensional
systems.II.Fluctuation eﬀects,” Physical Review B,vol.10,
no.9,pp.3832–3843,1974.
[431] Yu.V.Kopaev,“About the interplay theory between elec
tron and structural transformations and superconductivity,”
Trudy Fiz.Inst.Akad.Nauk SSSR,vol.86,p.3,1975.
[432] C.A.Balseiro and L.M.Falicov,“Superconductivity and
chargedensity waves,” Physical Review B,vol.20,no.11,pp.
4457–4464,1979.
[433] A.M.Gabovich and E.A.Pashitskii,“About the existence of
mixed phase superconductorexcitonicinsulator in intrinsic
semimetals,” Fizika Tverdogo Tela,vol.17,p.1584,1975.
[434] Y.Ishida,T.Shimojima,K.Ishizaka,et al.,“Temperature
dependent pseudogap in the oxypnictides LaFeAsO
1
−
x
F
x
and LaFePO
1
−
x
F
x
seen via angleintegrated photoemission,”
Physical Review B,vol.79,no.6,Article ID060503,2009.
[435] T.Mertelj,V.V.Kabanov,C.Gadermaier,et al.,“Dis
tinct pseudogap and quasiparticle relaxation dynamics
in the superconducting state of nearly optimally doped
SmFeAsO
0.8
F
0.2
single crystals,” Physical Review Letters,vol.
102,no.11,Article ID117002,2009.
[436] V.B.Zabolotnyy,D.S.Inosov,D.V.Evtushinsky,et al.,
“(π,π) electronic order in iron arsenide superconductors,”
Nature,vol.457,no.7229,pp.569–572,2009.
[437] R.H.Friend and D.J
´
erome,“Periodic lattice distortions and
charge density waves in one and twodimensional metals,”
Journal of Physics C,vol.12,no.8,pp.1441–1477,1979.
[438] P.B.Littlewood and V.Heine,“The eﬀect of electronelectron
interactions on the Peierls transition in metals with strong
nesting of Fermi surfaces,” Journal of Physics C,vol.14,no.
21,pp.2943–2949,1981.
[439] M.Rotter,M.Tegel,D.Johrendt,I.Schellenberg,W.Hermes,
and R.P
¨
ottgen,“Spindensitywave anomaly at 140 K in the
ternary iron arsenide BaFe
2
As
2
,” Physical Review B,vol.78,
no.2,Article ID020503,2008.
[440] N.Miyakawa,K.Tokiwa,S.Mikusu,et al.,“Tunneling studies
of multilayered superconducting cuprate Ba
2
Ca
3
Cu
4
O
12+δ
,”
International Journal of Modern Physics B,vol.17,no.18–20,
pp.3612–3616,2003.
[441] K.K.Gomes,A.N.Pasupathy,A.Pushp,S.Ono,Y.Ando,and
A.Yazdani,“Visualizing pair formation on the atomic scale in
the highT
c
superconductor Bi
2
Sr
2
CaCu
2
O
8+δ
,” Nature,vol.
447,no.7144,pp.569–572,2007.
[442] N.Miyakawa,K.Tokiwa,S.Mikusu,et al.,“Tunneling
spectroscopy of trilayer highT
c
cuprate,TlBa
2
Ca
2
Cu
2
O
10+δ
,”
International Journal of Modern Physics B,vol.19,no.1–3,pp.
225–229,2005.
[443] Y.DeWilde,N.Miyakawa,P.Guptasarma,et al.,“Unusual
strongcoupling eﬀects in the tunneling spectroscopy of
optimally doped and overdoped Bi
2
Sr
2
CaCu
2
O
8+δ
,” Physical
Review Letters,vol.80,no.1,pp.153–156,1998.
[444] M.Eschrig and M.R.Norman,“Neutron resonance:model
ing photoemission and tunneling data in the superconduct
ing state of Bi
2
Sr
2
CaCu
2
O
8+δ
,” Physical Review Letters,vol.
85,no.15,pp.3261–3264,2000.
[445] J.X.Zhu,J.Sun,Q.Si,and A.V.Balatsky,“Eﬀects of a
collective spin resonance mode on the scanning tunneling
microscopy spectra of dwave superconductors,” Physical
ReviewLetters,vol.92,no.1,Article ID017002,4 pages,2004.
[446] J.F.Zasadzinski,L.Ozyuzer,L.Coﬀey,K.E.Gray,D.
G.Hinks,and C.Kendziora,“Persistence of strong elec
tron coupling to a narrow boson spectrum in overdoped
Bi
2
Sr
2
CaCu
2
O
8+δ
tunneling data,” Physical Review Letters,
vol.96,no.1,Article ID017004,2006.
[447] J.X.Zhu,A.V.Balatsky,T.P.Devereaux,et al.,“Fourier
transformed local density of states and tunneling into a d
wave superconductor with bosonic modes,” Physical Review
B,vol.73,no.1,Article ID014511,9 pages,2006.
[448] P.W.Anderson and N.P.Ong,“Theory of asymmetric
tunneling in the cuprate superconductors,” Journal of Physics
and Chemistry of Solids,vol.67,no.1–3,pp.1–5,2006.
[449] G.L.de Castro,C.Berthod,A.Piriou,E.Giannini,and
∅.Fischer,“Preeminent role of the van Hove singular
ity in the strongcoupling analysis of scanning tunneling
spectroscopy for twodimensional cuprate superconductors,”
Physical Review Letters,vol.101,no.26,Article ID 267004,
2008.
[450] J.Nieminen,H.Lin,R.S.Markiewicz,and A.Bansil,“Origin
of the electronhole asymmetry in the scanning tunneling
spectrum of the hightemperature Bi
2
Sr
2
CaCu
2
O
8+δ
super
conductor,” Physical ReviewLetters,vol.102,no.3,Article ID
037001,2009.
[451] J.X.Liu,J.C.Wan,A.M.Goldman,Y.C.Chang,and
P.Z.Jiang,“Features of the density of states of high
T
c
superconductors probed by vacuum tunneling,” Physical
Review Letters,vol.67,no.16,pp.2195–2198,1991.
Advances in Condensed Matter Physics 35
[452] T.Cren,D.Roditchev,W.Sacks,and J.Klein,“Nanometer
scale mapping of the density of states in an inhomogeneous
superconductor,” Europhysics Letters,vol.54,no.1,pp.84–
90,2001.
[453] S.H.Pan,J.P.O’Neal,R.L.Badzey,et al.,“Microscopic
electronic inhomogeneity in the highT
c
superconductor
Bi
2
Sr
2
CaCu
2
O
8+x
,” Nature,vol.413,no.6853,pp.282–285,
2001.
[454] K.M.Lang,V.Madhavan,J.E.Hoﬀman,et al.,“Imaging
the granular structure of highT
c
superconductivity in
underdoped Bi
2
Sr
2
CaCu
2
O
8+δ
,” Nature,vol.415,no.6870,
pp.412–416,2002.
[455] G.Kinoda,S.Nakao,T.Motohashi,et al.,“Inhomogeneous
electronic structures in heavily Pbdoped Bi
2
Sr
2
CaCu
2
O
y
single crystals probed by lowtemperature STM/STS,” Physica
C,vol.388389,pp.273–274,2003.
[456] H.Mashima,N.Fukuo,Y.Matsumoto,et al.,“Electronic
inhomogeneity of heavily overdoped Bi
2x
Pb
x
Sr
2
CuO
y
studied by lowtemperature scanning tunneling
microscopy/spectroscopy,” Physical Review B,vol.73,
no.6,Article ID060502,4 pages,2006.
[457] A.C.Fang,L.Capriotti,D.J.Scalapino,et al.,“Gap
inhomogeneityinduced electronic states in superconducting
Bi
2
Sr
2
CaCu
2
O
8+δ
,” Physical Review Letters,vol.96,no.1,
Article ID017007,2006.
[458] J.A.Slezak,J.Lee,M.Wang,et al.,“Imaging the impact
on cuprate superconductivity of varying the interatomic
distances within individual crystal unit cells,” Proceedings
of the National Academy of Sciences of the United States of
America,vol.105,no.9,pp.3203–3208,2008.
[459] K.Fujita,J.Lee,M.Wang,et al.,“Imaging the eﬀect of
electron lattice interactions on highT
c
superconductivity in
Bi
2
Sr
2
CaCu
2
O
8+δ
,” Journal of Physics:Conference Series,vol.
108,no.1,Article ID012028,2008.
[460] K.Anagawa,T.Watanabe,and M.Suzuki,“Superconducting
gap and pseudogap for overdoped Bi
2
−
x
Pb
x
Sr
2
CaCu
2
O
8+δ
using 60 ns timescale shortpulse interlayer tunneling
spectroscopy,” Physical Review B,vol.73,no.18,Article ID
184512,2006.
[461] Y.Yamada and M.Suzuki,“Interlayer tunneling spectroscopy
for deeply underdoped Bi
2
Sr
2
CaCu
2
O
8+δ
:spectroscopic
evidence for inhomogeneous superconductivity,” Physical
Review B,vol.74,Article ID054508,2006.
[462] S.Johnston,F.Vernay,and T.P.Devereaux,“Impact of an
oxygen dopant in Bi
2
Sr
2
CaCu
2
O
8+δ
,” Europhysics Letters,vol.
86,p.37007,2009.
[463] J.H.Ma,Z.H.Pan,F.C.Niestemski,et al.,“Coexistence
of competing orders with two energy gaps in real and
momentum space in the high temperature superconductor
Bi
2
Sr
2
−
x
La
x
CuO
6+δ
,” Physical Review Letters,vol.101,no.20,
Article ID207002,2008.
[464] J.L.Tallon and J.W.Loram,“Comment on “thermodynamic
transitions in inhomogeneous dwave superconductors”,”
Physical Review B,vol.79,no.9,Article ID096501,2009.
[465] A.Guti
´
errezSosa,U.Bangert,and W.R.Flavell,“Inves
tigations of chemical and electronic inhomogeneities in
BaPb
1
−
x
Bi
x
O
3
via highly spatially resolved electron energy
loss spectroscopy,” Journal of Applied Physics,vol.94,no.10,
pp.6639–6643,2003.
[466] I.Roshchin,V.Stepankin,and A.Kuznetsov,“Reentrant
superconducting transport behavior of single grain bound
ary Josephson junction in BaPb
1
−
x
Bi
x
O
3
bicrystals,” Journal
of Low Temperature Physics,vol.100,no.34,pp.229–240,
1995.
[467] E.L.Nagaev,“Ground state and anomalous magnetic
moment of conduction electrons in an antiferromagnetic
semiconductor,” Pis’ma Zhurnal Eksperimental’noi i Teo
reticheskoi Fiziki,vol.6,p.484,1967.
[468] E.L.Nagaev,“Ferromagnetic domains in a semiconducting
antiferromagnet,” Zhurnal
´
Eksperimental’noi i Teoreticheskoi
Fiziki,vol.54,p.228,1968.
[469] E.L.Nagaev,Physics of Magnetic Semiconductors,Nauka,
Moscow,Russia,1979.
[470] E.L.Nagaev,“Phase separation in hightemperature super
conductors and related magnetic systems,” Uspekhi Fizich
eskikh Nauk,vol.165,p.529,1995.
[471] M.A.Krivoglaz,“Electron states near the phase transition
point and in disordered systems,” Fizika Tverdogo Tela,vol.
11,p.2230,1969.
[472] M.A.Krivoglaz,“Fluctuonic states of electrons,” Uspekhi
Fizicheskikh Nauk,vol.111,p.617,1973.
[473] M.A.Krivoglaz and A.I.Karasevskii,“Condensation in in
the systemof polarons or ﬂuctuons with the formation of the
nonhomogeneous state and peculiarities of conductance,”
Pis’ma Zhurnal Eksperimental’noi i Teoreticheskoi Fiziki,vol.
19,p.454,1974.
[474] M.A.Krivoglaz,Diﬀuse Scattering of XRays and Neutrons by
Fluctuations,Springer,Berlin,Germany,1996.
[475] J.M.Tranquada,B.J.Sternlieb,J.D.Axe,Y.Nakamura,and
S.Uchida,“Evidence for stripe correlations of spins and holes
in copper oxide superconductors,” Nature,vol.375,no.6532,
pp.561–563,1995.
[476] J.M.Tranquada,“Phase separation,charge segregation and
superconductivity in layered cuprates,” in Neutron Scattering
in Layered CopperOxide Superconductors,A.Furrer,Ed.,
pp.225–260,Kluwer Academic Publishers,Dordrecht,The
Netherlands,1998.
[477] M.B.Salamon and M.Jaime,“The physics of manganites:
structure and transport,” Reviews of Modern Physics,vol.73,
no.3,pp.583–628,2001.
[478] A.Damascelli,Z.Hussain,and Z.X.Shen,“Angleresolved
photoemission studies of the cuprate superconductors,”
Reviews of Modern Physics,vol.75,no.2,pp.473–541,2003.
[479] T.Yanagisawa,“Lattice distortions and stripes in the under
doped region of highT
c
cuprates,” Journal of Physics A,vol.
36,no.35,pp.9337–9349,2003.
[480] J.M.Tranquada,H.Woo,T.G.Perring,et al.,“Quantum
magnetic excitations fromstripes in copper oxide supercon
ductors,” Nature,vol.429,no.6991,pp.534–538,2004.
[481] O.N.Bakharev,I.M.AbuShiekah,H.B.Brom,A.A.
Nugroho,I.P.McCulloch,and J.Zaanen,“NMRevidence for
a twostep phase separation in Nd
1.85
Ce
0.15
CuO
4
−
δ
,” Physical
ReviewLetters,vol.93,no.3,Article ID037002,1 pages,2004.
[482] C.J.Zhang and H.Oyanagi,“Eﬀects of local lattice disorder
on the superconductivity studied by XAFS,” Journal of
Physics:Conference Series,vol.108,no.1,Article ID 012048,
2008.
[483] H.Oyanagi,C.Zhang,A.Tsukada,and M.Naito,“Lattice
instability in high temperature superconducting cuprates
probed by Xray absorption spectroscopy,” Journal of Physics:
Conference Series,vol.108,no.1,Article ID012038,2008.
[484] Y.Koike,T.Adachi,Y.Tanabe,K.Omori,T.Noji,and H.Sato,
“Inhomogeneous superconductivity inboth underdoped and
overdoped regimes of highT
c
cuprates,” Journal of Physics:
Conference Series,vol.108,no.1,Article ID012003,2008.
[485] H.Keller,A.BussmannHolder,and K.A.M
¨
uller,“Jahn
Teller physics and highT
c
superconductivity,” Materials
Today,vol.11,no.9,pp.38–46,2008.
36 Advances in Condensed Matter Physics
[486] J.C.Phillips,A.Saxena,and A.R.Bishop,“Pseudogaps,
dopants,and strong disorder in cuprate hightemperature
superconductors,” Reports on Progress in Physics,vol.66,no.
12,pp.2111–2182,2003.
[487] R.A.Klemm,“The pseudogap and the superconducting
order parameter in inhomogeneous Bi
2
Sr
2
CaCu
2
O
8+δ
,” Jour
nal of Superconductivity and Novel Magnetism,vol.17,no.1,
pp.69–74,2004.
[488] J.C.Phillips,“Quantum percolation in cuprate high
temperature superconductors,” Proceedings of the National
Academy of Sciences of the United States of America,vol.105,
no.29,pp.9917–9919,2008.
[489] F.V.Kusmartsev and M.Saarela,“What is the most
important for a nanoscale structure formations in HTSC?
Spin,phonon or third way in Coulomb interaction and
correlations?” Journal of Physics:Conference Series,vol.108,
no.1,Article ID012029,2008.
[490] F.V.Kusmartsev and M.Saarela,“Twocomponent physics of
cuprates and superconductorinsulator transitions,” Super
conductor Science and Technology,vol.22,no.1,Article ID
014008,2009.
[491] B.Fine and T.Egami,“Intermediate spincharge order in the
cuprates,” Journal of Physics:Conference Series,vol.108,no.1,
Article ID012005,2008.
[492] M.M
¨
uller and B.I.Shklovskii,“Compensationdriven
superconductorinsulator transition,” Physical Review B,vol.
79,no.13,Article ID134504,2009.
[493] A.S.Alexandrov,“Phase separation of electrons strongly
coupled with phonons in cuprates and manganites,” Journal
of Superconductivity and Novel Magnetism,vol.22,no.2,pp.
95–101,2009.
[494] J.T.Park,D.S.Inosov,Ch.Niedermayer,et al.,“Electronic
phase separation in the slightly underdoped iron pnictide
superconductor Ba
1
−
x
K
x
Fe
2
As
2
,” Physical Review Letters,vol.
102,no.11,Article ID117006,2009.
[495] B.Sac
´
ep
´
e,C.Chapelier,T.I.Baturina,V.M.Vinokur,
M.R.Baklanov,and M.Sanquer,“Disorderinduced inho
mogeneities of the superconducting state close to the
superconductorinsulator transition,” Physical Review Let
ters,vol.101,no.15,Article ID157006,2008.
[496] H.L.Edwards,A.L.Barr,J.T.Markert,and A.L.De Lozanne,
“Modulations in the CuO chain layer of YBa
2
Cu
3
O
7
−
δ
:
charge density waves?” Physical Review Letters,vol.73,no.8,
pp.1154–1157,1994.
[497] D.J.Derro,E.W.Hudson,K.M.Lang,et al.,“Nanoscale
onedimensional scattering resonances in the CuO chains of
YBa
2
Cu
3
O
6+x
,” Physical Review Letters,vol.88,no.9,Article
ID097002,4 pages,2002.
[498] A.A.Abrikosov,Fundamentals of the Theory of Metals,
NorthHolland,Amsterdam,The Netherlands,1987.
[499] K.McElroy,R.W.Simmonds,J.E.Hoﬀman,et al.,“Relating
atomicscale electronic phenomena to wavelike quasiparti
cle states in superconducting Bi
2
Sr
2
CaCu
2
O
8+δ
,” Nature,vol.
422,no.6932,pp.592–596,2003.
[500] T.PeregBarnea and M.Franz,“Theory of quasiparticle
interference patterns in the pseudogap phase of the cuprate
superconductors,” Physical Review B,vol.68,no.18,Article
ID180506,4 pages,2003.
[501] T.PeregBarnea and M.Franz,“Quasiparticle interference
patterns as a test for the nature of the pseudogap phase in the
cuprate superconductors,” International Journal of Modern
Physics B,vol.19,no.4,pp.731–761,2005.
[502] T.S.Nunner,W.Chen,B.M.Andersen,A.Melikyan,
and P.J.Hirschfeld,“Fourier transform spectroscopy of d
wave quasiparticles in the presence of atomic scale pairing
disorder,” Physical Review B,vol.73,no.10,Article ID
104511,7 pages,2006.
[503] T.Hanaguri,Y.Kohsaka,J.C.Davis,et al.,“Quasiparticle
interference and superconducting gap in Ca
2
−
x
Na
x
CuO
2
Cl
2
,”
Nature Physics,vol.3,no.12,pp.865–871,2007.
[504] Y.Kohsaka,C.Taylor,P.Wahl,et al.,“How Cooper pairs
vanish approaching the Mott insulator in Bi
2
Sr
2
CaCu
2
O
8+δ
,”
Nature,vol.454,no.7208,pp.1072–1078,2008.
[505] T.Hanaguri,Y.Kohsaka,M.Ono,et al.,“Coherence factors
in a highT
c
cuprate probed by quasiparticle scattering oﬀ
vortices,” Science,vol.323,no.5916,pp.923–926,2009.
[506] C.Howald,H.Eisaki,N.Kaneko,M.Greven,and A.Kapit
ulnik,“Periodic densityofstates modulations in supercon
ducting Bi
2
Sr
2
CaCu
2
O
8+δ
,” Physical Review B,vol.67,no.1,
Article ID014533,10 pages,2003.
[507] T.Hanaguri,C.Lupien,Y.Kohsaka,et al.,“A
‘checkerboard’ electronic crystal state in lightly hole
doped Ca
2
−
x
Na
x
CuO
2
Cl
2
,” Nature,vol.430,no.7003,pp.
1001–1005,2004.
[508] Y.Kohsaka,C.Taylor,K.Fujita,et al.,“An intrinsic bond
centered electronic glass with unidirectional domains in
underdoped cuprates,” Science,vol.315,no.5817,pp.1380–
1385,2007.
[509] M.F.Crommie,C.P.Lutz,and D.M.Eigler,“Imaging
standing waves in a twodimensional electron gas,” Nature,
vol.363,no.6429,pp.524–527,1993.
[510] G.A.Fiete and E.J.Heller,“Colloquium:theory of quantum
corrals and quantum mirages,” Reviews of Modern Physics,
vol.75,no.3,pp.933–948,2003.
[511] J.Friedel,“Metallic alloys,” Il Nuovo Cimento,vol.7,
supplement 2,pp.287–311,1958.
[512] J.E.Hoﬀman,K.McElroy,D.H.Lee,et al.,“Imaging
quasiparticle interference in Bi
2
Sr
2
CaCu
2
O
8+δ
,” Science,vol.
297,no.5584,pp.1148–1151,2002.
[513] A.M.Gabovich and E.A.Pashitskii,“Polarization operator
of the superconducting electron gas.Kohn anomalies and
charge screening in superconductors,” Ukrainskii Fizychnyi
Zhurnal,vol.18,p.549,1973.
[514] J.P.Hurault,“Note sur les polarisations de spin et de charge
autour d’une impurete dans un supraconducteur,” Journal de
Physique,vol.26,p.252,1965.
[515] A.M.Gabovich,L.G.Il’chenko,and E.A.Pashitskii,Fizika
Tverdogo Tela,vol.21,p.2191,1979.
[516] G.Gr
¨
uner,Density Waves in Solids,AddisonWesley,Reading,
Mass,USA,1994.
[517] T.M.Rice and G.K.Scott,“New mechanism for a charge
densitywave instability,” Physical Review Letters,vol.35,no.
2,pp.120–123,1975.
[518] R.S.Markiewicz,“A survey of the Van Hove scenario
for highT
c
superconductivity with special emphasis on
pseudogaps and striped phases,” Journal of Physics and
Chemistry of Solids,vol.58,no.8,pp.1179–1310,1997.
[519] R.Peierls,“Zur Theorie der elektrischen urnd therrnlschen
Leitf
¨
ahigkeit von Metallen,” Annals of Physics,vol.4,p.121,
1930.
[520] R.E.Peierls,Quantum Theory of Solids,Clarendon Press,
Oxford,UK,1955.
[521] L.V.Keldysh and Yu.V.Kopaev,Fizika Tverdogo Tela,vol.6,
p.2791,1964.
Advances in Condensed Matter Physics 37
[522] B.I.Halperin and T.M.Rice,“The excitonic state at the
semiconductorsemimetal transition,” in Solid State Physics,
vol.21,p.115,Academic Press,New York,NY,USA,1968.
[523] A.N.Kozlov and L.A.Maksimov,“On the metalinsulator
phase transition.Divalent crystal,” Zhurnal Eksperimental’noi
i Teoreticheskoi Fiziki,vol.48,p.1184,1965.
[524] T.Ishiguro and K.Yamaji,Organic Superconductors,Springer,
Berlin,Germany,1990.
[525] C.Schlenker,J.Dumas,M.Greenblatt,and S.van Smaalen,
Eds.,Physics and Chemistry of LowDimensional Inorganic
Conductors,PlenumPress,New York,NY,USA,1996.
[526] B.Kyung,“Meanﬁeld study of the interplay between
antiferromagnetismand dwave superconductivity,” Physical
Review B,vol.62,no.13,pp.9083–9088,2000.
[527] H.Wilhelm,D.Jaccard,R.Duprat,et al.,“The case for
universality of the phase diagramof the Fabre and Bechgaard
salts,” European Physical Journal B,vol.21,no.2,pp.175–183,
2001.
[528] C.Colin,C.R.Pasquier,and K.Bechgaard,“Multiphase
coexistence in the organic conductor (TMTSF)
2
ReO
4
,” Jour
nal de Physique,vol.131,pp.313–314,2005.
[529] A.Aperis,G.Varelogiannis,P.B.Littlewood,and B.D.
Simons,“Coexistence of spin density wave,dwave singlet
and staggered πtriplet superconductivity,” Journal of Physics:
Condensed Matter,vol.20,Article ID434235,5 pages,2008.
[530] J.T.Devreese,R.P.Evrard,and V.E.van Doren,Eds.,
Highly Conducting OneDimensional Solids,Plenum Press,
New York,NY,USA,1979.
[531] P.Monceau,Ed.,Electronic Properties of Inorganic QuasiOne
Dimensional Compounds—Part II:Experimental,D.Reidel,
Dordrecht,The Netherlands,1985.
[532] S.RothandD.Carroll,OneDimensional Metals,WileyVCH,
Weinheim,Germany,2004.
[533] M.J.Rice and Yu.N.Gartstein,“The excitonic ground
state of the halfﬁlled Peierls insulator,” Journal of Physics:
Condensed Matter,vol.17,no.29,pp.4615–4620,2005.
[534] W.Kohn and D.Sherrington,“Two kinds of bosons and bose
condensates,” Reviews of Modern Physics,vol.42,no.1,pp.
1–11,1970.
[535] H.Cercellier,C.Monney,F.Clerc,et al.,“Evidence for
an excitonic insulator phase in 1TTiSe
2
,” Physical Review
Letters,vol.99,no.14,Article ID146403,4 pages,2007.
[536] C.Monney,H.Cercellier,F.Clerc,et al.,“Spontaneous exci
ton condensation in 1TTiSe
2
:BCSlike approach,” Physical
Review B,vol.79,no.4,Article ID045116,11 pages,2009.
[537] B.Bucher,P.Steiner,and P.Wachter,“Excitonic insulator
phase in TmSe
0.45
Te
0.55
,” Physical Review Letters,vol.67,no.
19,pp.2717–2720,1991.
[538] P.Wachter,A.Jung,and P.Steiner,“Pressuredriven metal
insulator transition in Ladoped SmS:excitonic condensa
tion,” Physical Review B,vol.51,no.8,pp.5542–5545,1995.
[539] Y.Wakisaka,T.Sudayama,K.Takubo,et al.,“Excitonic
insulator state in Ta
2
NiSe
5
probed by photoemission spec
troscopy,” Physical Review Letters,vol.103,no.2,Article ID
026402,4 pages,2009.
[540] J.Zaanen,“Superconductivity:quantum stripe search,”
Nature,vol.440,no.7088,pp.1118–1119,2006.
[541] P.Wr
´
obel,“Checkerboard or stripes:hardcore bosons on the
checkerboard lattice as a model of charge ordering in planar
cuprates,” Physical ReviewB,vol.74,no.1,Article ID014507,
8 pages,2006.
[542] V.Cvetkovic,Z.Nussinov,S.Mukhin,and J.Zaanen,
“Observing the ﬂuctuating stripes in highT
c
superconduc
tors,” Europhysics Letters,vol.81,no.2,Article ID 27001,6
pages,2008.
[543] C.W.Misner,K.S.Thorne,and W.H.Zurek,“John Wheeler,
relativity,and quantuminformation,” Physics Today,vol.62,
no.4,pp.40–46,2009.
[544] P.Abbamonte,A.Rusydi,S.Smadici,G.D.Gu,G.A.
Sawatzky,and D.L.Feng,“Spatially modulated ‘Mottness’ in
La
2
−
x
Ba
x
CuO
4
,” Nature Physics,vol.1,pp.155–158,2005.
[545] M.Fujita,H.Goka,K.Yamada,and M.Matsuda,“Competi
tionbetweencharge andspindensitywave order andsuper
conductivity in La
1.875
Ba
0.125
−
x
Sr
x
CuO
4
,” Physical Review
Letters,vol.88,no.16,Article ID167008,4 pages,2002.
[546] J.Fink,E.Schierle,E.Weschke,et al.,“Charge ordering in
La
1.8
−
x
Eu
0.2
Sr
x
CuO
4
studied by resonant soft Xray diﬀrac
tion,” Physical Review B,vol.79,no.10,Article ID 100502,4
pages,2009.
[547] C.M.Varma,“NonFermiliquid states and pairing insta
bility of a general model of copper oxide metals,” Physical
Review B,vol.55,no.21,pp.14554–14580,1997.
[548] H.J.Schulz,“Fermisurface instabilities of a generalized two
dimensional Hubbard model,” Physical Review B,vol.39,no.
4,pp.2940–2943,1989.
[549] S.Chakravarty,R.B.Laughlin,D.K.Morr,and C.Nayak,
“Hidden order in the cuprates,” Physical Review B,vol.63,
no.9,Article ID094503,10 pages,2001.
[550] D.J
´
erome,C.Berthier,P.Molini
´
e,and J.Rouxel,“Layer
compounds.Charge density waves in transitions metal com
pounds.Electronic properties of transition metal dichalco
genides:connection between structural instabilities and
superconductivity,” Journal de Physique,vol.37,pp.C4–
C125,1976.
[551] O.Degtyareva,M.V.Magnitskaya,J.Kohanoﬀ,et al.,“Com
petition of chargedensity waves and superconductivity in
sulfur,” Physical Review Letters,vol.99,Article ID 155505,4
pages,2007.
[552] K.Kudo,N.Okumura,Y.Miyoshi,T.Nishizaki,T.Sasaki,
and N.Kobayashi,“Narrow carrier concentration range of
superconductivity and critical point of pseudogap formation
temperature in Pbsubstituted Bi
2
Sr
2
CuO
6+δ
,” Journal of the
Physical Society of Japan,vol.78,no.8,Article ID 084722,5
pages,2009.
[553] H.Won and K.Maki,“dwave superconductor as a model of
highT
c
superconductors,” Physical Review B,vol.49,no.2,
pp.1397–1402,1994.
[554] H.Won,K.Maki,and E.Puchkaryov,in HighT
c
Supercon
ductors and Related Materials:Material Science,Fundamental
Properties,and Some Future Electronic Applications,S.L.
Drechsler and T.Mishonov,Eds.,p.375,Kluwer Academic,
Dordrecht,The Netherlands,2001.
[555] H.Won,S.Haas,D.Parker,S.Telang,A.V
´
anyolos,and K.
Maki,in Lectures on the Physics of Highly Correlated Electron
Systems IX:Ninth Training Course,A.Avella and F.Mancini,
Eds.,p.3,American Institute of Physics,Melville,NY,USA,
2005.
[556] A.M.Gabovich and A.I.Voitenko,“Josephson tunnelling
involving superconductors with chargedensity waves,” Jour
nal of Physics:Condensed Matter,vol.9,no.19,pp.3901–
3920,1997.
[557] A.M.Gabovich and A.I.Voitenko,“Asymmetrical tunneling
between similar metallic junctions with chargedensity or
spindensity waves:the case of broken symmetry,” Physical
Review B,vol.56,no.13,pp.7785–7788,1997.
38 Advances in Condensed Matter Physics
[558] B.M
¨
uhlschlegel,“Die thermodynamischen Funktionen des
Supraleiters,” Zeitschrift f
¨
ur Physik A,vol.155,no.3,pp.313–
327,1959.
[559] V.M.Krasnov,“Temperature dependence of the bulk energy
gap in underdoped Bi
2
Sr
2
CaCu
2
O
8+δ
:evidence for the mean
ﬁeld superconducting transition,” Physical Review B,vol.79,
no.21,Article ID214510,17 pages,2009.
[560] M.Suzuki and T.Watanabe,“Discriminating the supercon
ducting gap from the pseudogap in Bi
2
Sr
2
CaCu
2
O
8+δ
by
interlayer tunneling spectroscopy,” Physical Review Letters,
vol.85,no.22,pp.4787–4790,2000.
[561] T.Ekino,S.Hashimoto,T.Takasaki,and H.Fujii,
“Tunneling spectroscopy of the normalstate gap in
(Bi,Pb)
2
Sr
2
Ca
2
Cu
3
O
10+δ
,” Physical Review B,vol.64,no.9,
Article ID092510,4 pages,2001.
[562] T.Ekino,Y.Sezaki,S.Hashimoto,and H.Fujii,“Obser
vation of the energy gap above (Bi,Pb)
2
Sr
2
Ca
2
Cu
3
O
10+δ
using breakjunction tunneling,” Journal of Low Temperature
Physics,vol.117,no.34,pp.359–363,1999.
[563] A.Sugimoto,T.Ekino,and H.Eisaki,“Nanoscale modulation
of local barrier height on Bibased cuprate superconductors
observed by scanning tunneling microscopy/spectroscopy,”
Journal of the Physical Society of Japan,vol.77,no.4,Article
ID043705,4 pages,2008.
[564] J.W.Alldredge,J.Lee,K.McElroy,et al.,“Evolution of
the electronic excitation spectrumwith strongly diminishing
hole density in superconducting Bi
2
Sr
2
CaCu
2
O
8+δ
,” Nature
Physics,vol.4,no.4,pp.319–326,2008.
[565] Y.Kohsaka,K.Iwaya,S.Satow,M.Azuma,M.Takano,and
H.Takagi,“Imaging nanoscale electronic inhomogeneity in
the lightly doped mott insulator Ca
2
−
x
Na
x
CuO
2
Cl
2
,” Physical
ReviewLetters,vol.93,no.9,Article ID097004,4 pages,2004.
[566] A.M.Gabovich and A.S.Shpigel,Fizika Tverdogo Tela,vol.
26,p.1569,1984.
[567] R.Escudero,F.Morales,and S.Bern
`
es,“Speciﬁc heat studies
of pure Nb
3
Sn single crystals at low temperature,” Journal of
Physics:Condensed Matter,vol.21,no.32,Article ID325701,
7 pages,2009.
[568] N.E.Phillips,R.A.Fisher,and J.E.Gordon,in Progress in
Low Temperature Physics,vol.13,p.267,Elsevier,Amster
dam,The Netherlands,1992.
[569] J.W.Loram,K.A.Mirza,W.Y.Liang,and J.Osborne,“Asys
tematic study of the speciﬁc heat anomaly in La
2
−
x
Sr
x
CuO
4
,”
Physica C,vol.162–164,part 1,pp.498–499,1989.
[570] J.L.Tallon and J.W.Loram,“Doping dependence of T
∗
—
what is the real highT
c
phase diagram?” Physica C,vol.349,
no.12,pp.53–68,2001.
[571] H.H.Wen,G.Mu,H.Luo,et al.,“Speciﬁcheat measure
ment of a residual superconducting state in the normal
state of underdoped Bi
2
Sr
2
−
x
La
x
CuO
6+δ
cuprate supercon
ductors,” Physical Review Letters,vol.103,no.6,Article ID
067002,4 pages,2009.
[572] B.Krunavakarn,S.Kaskamalas,and S.Yoksan,“Thermody
namic properties of a BCS superconductor,” Physica C,vol.
338,no.4,pp.305–315,2000.
[573] H.Balci and R.L.Greene,“Thermodynamic properties of
Pr
1.85
Ce
0.15
CuO
4
−
δ
,” Physical ReviewB,vol.70,no.14,Article
ID140508,4 pages,2004.
[574] C.E.Methfessel,A.R.Stewart,B.T.Matthias,and C.K.
N.Patel,“Why is there no bulk speciﬁc heat anomaly at the
superconducting transition temperature of BaPb
1
−
x
Bi
x
O
3
?”
Proceedings of the National Academy of Sciences of the United
States of America,vol.77,no.11,pp.6307–6308,1980.
[575] S.Tanaka,K.Kitazawa,and T.Tani,Annual Report of
the Engineering Research Institute,Faculty of Engineering,
University of Tokyo,vol.41,p.131,1982.
[576] M.Sato,H.Fujishita,and S.Hoshino,“Speciﬁc heat anomaly
of BaPb
1
−
x
Bi
x
O
3
at the superconducting transition,” Journal
of Physics C,vol.16,no.13,pp.L417–L421,1983.
[577] B.B.Schwartz and S.Foner,“Largescale applications of
superconductivity,” Physics Today,vol.30,p.34,1977.
[578] D.Larbalestier,G.Fisk,B.Montgomery,and D.Hawksworth,
“Highﬁeld superconductivity,” Physics Today,vol.39,no.3,
pp.24–35,1986.
[579] D.Larbalestier,A.Gurevich,D.M.Feldmann,and A.
Polyanskii,“HighT
c
superconducting materials for electric
power applications,” Nature,vol.414,no.6861,pp.368–377,
2001.
[580] S.Kang,A.Goyal,J.Li,et al.,“Highperformance highT
c
superconducting wires,” Science,vol.311,no.5769,pp.1911–
1914,2006.
[581] A.M.Clogston,“Upper limit for the critical ﬁeld in hard
superconductors,” Physical Review Letters,vol.9,no.6,pp.
266–267,1962.
[582] B.S.Chandrasekhar,“A note on the maximum critical ﬁeld
of highﬁeld superconductors,” Applied Physics Letters,vol.1,
no.1,pp.7–8,1962.
[583] P.Fulde,“High ﬁeld superconductivity in thin ﬁlms,”
Advances in Physics,vol.22,no.6,pp.667–719,1973.
[584] R.C.Bruno and B.B.Schwartz,“Magnetic ﬁeld splitting of
the density of states of thinsuperconductors,” Physical Review
B,vol.8,no.7,pp.3161–3178,1973.
[585] P.M.Tedrow and R.Meservey,“Experimental test of
the theory of highﬁeld superconductivity,” Physical Review
Letters,vol.43,no.5,pp.384–387,1979.
[586] R.G.Dias and J.A.Silva,“Huge metastability in highT
c
superconductors induced by parallel magnetic ﬁeld,” Physical
Review B,vol.67,no.9,Article ID092511,4 pages,2003.
[587] A.M.Gabovich,E.A.Pashitskii,and A.S.Shpigel,“Exceed
ing of paramagnetic limit in superconductors with dielectric
gap on the Fermi surface,” Zhurnal Eksperimental’noi i
Teoreticheskoi Fiziki,vol.28,p.302,1978.
[588] A.M.Gabovich,E.A.Pashitskii,and A.S.Shpigel,“Para
magnetic limit of superconductors with a dielectric gap on
the Fermi surface,” Zhurnal Eksperimental’noi i Teoreticheskoi
Fiziki,vol.77,p.1157,1979.
[589] A.Gabovich,A.I.Voitenko,and T.Ekino,“Enhanced
paramagnetic limit of the upper critical magnetic ﬁeld
for superconductors with chargedensity waves,” Journal of
Physics:Condensed Matter,vol.16,no.21,pp.3681–3690,
2004.
[590] R.H.McKenzie,“Is the ground state of alpha(BEDT
TTF)
2
MHg(SCN)
4
[M
=
K,Rb,Tl] a chargedensity wave or a
spindensity wave?” http://arxiv.org/abs/condmat/9706235.
[591] N.Harrison,“Destabilization of a chargedensity wave by an
oscillatory chemical potential,” Physical Review Letters,vol.
83,no.7,pp.1395–1398,1999.
[592] J.S.Qualls,L.Balicas,J.S.Brooks,N.Harrison,L.K.
Montgomery,and M.Tokumoto,“Competition between
Pauli and orbital eﬀects in a chargedensitywave system,”
Physical Review B,vol.62,no.15,pp.10008–10012,2000.
[593] L.D.Landau and E.M.Lifshits,Electrodynamics of Continu
ous Media,Pergamon,New York,NY,USA,1984.
[594] N.P.Ong and P.Monceau,“Anomalous transport properties
of a linearchain metal:NbSe
3
,” Physical ReviewB,vol.16,no.
8,pp.3443–3455,1977.
Advances in Condensed Matter Physics 39
[595] S.Sugai,Y.Takayanagi,and N.Hayamizu,“Phason and
amplitudon in the chargedensitywave phase of one
dimensional charge stripes in La
2
−
x
Sr
x
CuO
4
,” Physical
Review Letters,vol.96,no.13,Article ID 137003,4 pages,
2006.
[596] A.M.Gabovich and A.I.Voitenko,“Nonstationary Joseph
son eﬀect for superconductors with chargedensity waves,”
Physical Review B,vol.55,no.2,pp.1081–1099,1997.
[597] N.Miyakawa,J.F.Zasadzinski,L.Ozyuzer,et al.,“Pre
dominantly superconducting origin of large energy gaps in
underdoped Bi
2
Sr
2
CaCu
2
O
8+δ
fromtunneling spectroscopy,”
Physical Review Letters,vol.83,no.5,pp.1018–1021,1999.
[598] Ch.Renner,B.Revaz,J.Y.Genoud,K.Kadowakj,and ∅.
Fischer,“Pseudogap precursor of the superconducting gap
in under and overdoped Bi
2
Sr
2
CaCu
2
O
8+δ
,” Physical Review
Letters,vol.80,no.1,pp.149–152,1998.
[599] A.K.Gupta and K.W.Ng,“abplane tunneling spectroscopy
of underdoped Bi
2
Sr
2
CaCu
2
O
y
,” Physical Review B,vol.58,
no.14,pp.R8901–R8904,1998.
[600] J.F.Zasadzinski,L.Ozyuzer,N.Miyakawa,K.E.Gray,D.G.
Hinks,and C.Kendziora,“Correlation of tunneling spectra
in Bi
2
Sr
2
CaCu
2
O
8+δ
with the resonance spin excitation,”
Physical Review Letters,vol.87,no.6,Article ID 067005,4
pages,2001.
[601] D.N.Dias,E.S.Caixeiro,and E.V.L.de Mello,“Magnetic
properties of cuprate superconductors based on a phase
separation theory,” Physica C,vol.468,no.6,pp.480–486,
2008.
[602] A.Bille,R.A.Klemm,and K.Scharnberg,“Models of caxis
twist Josephson tunneling,” Physical ReviewB,vol.64,no.17,
Article ID174507,23 pages,2001.
[603] A.I.Larkin and Yu.N.Ovchinnikov,“Tunnel eﬀect between
superconductors in an alternating ﬁeld,” Zhurnal Eksperi
mental’noi i Teoreticheskoi Fiziki,vol.51,p.1535,1966.
[604] W.A.Roshen,“Thermodynamic properties of charge
density waves,” Physical Review B,vol.31,no.11,pp.7296–
7305,1985.
[605] I.B
ˆ
aldea,“Reentrant chargedensity wave in the one
dimensional system with impurities—a selfconsistent
approach,” Physica Scripta,vol.42,no.6,pp.749–760,1990.
[606] J.Zittartz,“Theory of the excitonic insulator in the presence
of normal impurities,” Physical Review,vol.164,no.2,pp.
575–582,1967.
[607] A.A.Abrikosov and L.P.Gor’kov,“On the theory of
superconducting alloys.1.Electrodynamics of alloys at the
absolute zero,” Zhurnal Eksperimental’noi i Teoreticheskoi
Fiziki,vol.35,p.1558,1958.
[608] A.A.Abrikosov and L.P.Gor’kov,“Superconducting alloys at
temperatures above the absolute zero,” Zhurnal Eksperimen
tal’noi i Teoreticheskoi Fiziki,vol.36,p.319,1959.
[609] P.W.Anderson,“Theory of dirty superconductors,” Journal
of Physics and Chemistry of Solids,vol.11,no.12,pp.26–30,
1959.
[610] H.Kim,G.Preosti,and P.Muzikar,“Penetration depth and
impurity scattering in unconventional superconductors:T
=
0 results,” Physical Review B,vol.49,no.5,pp.3544–3547,
1994.
[611] Y.Sun and K.Maki,“Impurity eﬀects in dwave supercon
ductors,” Physical Review B,vol.51,no.9,pp.6059–6063,
1995.
[612] D.Manske,I.Eremin,and K.H.Bennemann,“Analysis of
the elementary excitations in highT
c
cuprates:explanation
of the new energy scale observed by angleresolved photoe
mission spectroscopy,” Physical ReviewLetters,vol.87,no.17,
Article ID177005,4 pages,2001.
[613] D.S.Inosov,S.V.Borisenko,I.Eremin,et al.,“Relation
between the oneparticle spectral function and dynamic
spin susceptibility of superconducting Bi
2
Sr
2
CaCu
2
O
8
−
δ
,”
Physical Review B,vol.75,no.17,Article ID172505,4 pages,
2007.
[614] A.N.Pasupathy,A.Pushp,K.K.Gomes,et al.,“Electronic
origin of the inhomogeneous pairing interaction in the high
T
c
superconductor Bi
2
Sr
2
CaCu
2
O
8+δ
,” Science,vol.320,no.
5873,pp.196–201,2008.
[615] M.H.Bae,J.H.Park,J.H.Choi,H.J.Lee,and K.S.
Park,“Pseudogap behavior revealed in interlayer tunneling
in overdoped Bi
2
Sr
2
CaCu
2
O
8+x
,” Physical Review B,vol.77,
no.9,Article ID094519,8 pages,2008.
[616] A.Kussmaul,E.S.Hellman,E.H.Hartford Jr.,and P.
M.Tedrow,“Superconductorinsulatorsuperconductor tun
neling in Ba
1
−
x
K
x
BiO
3
grain boundaries,” Applied Physics
Letters,vol.63,no.20,pp.2824–2826,1993.
[617] A.Mourachkine,“Origin of dips in tunneling dI/dV charac
teristics of cuprates,” Physica C,vol.460–462,pp.956–957,
2007.
[618] D.J.van Harlingen,“Phasesensitive tests of the symmetry of
the pairing state in the hightemperature superconductors
evidence for d
x
2
y
2
symmetry,” Reviews of Modern Physics,vol.
67,no.2,pp.515–535,1995.
[619] J.Mannhart and P.Chaudhari,“HighT
c
bicrystal grain
boundaries,” Physics Today,vol.54,no.11,pp.48–53,2001.
[620] N.E.Hussey,M.AbdelJawad,A.Carrington,A.P.Macken
zie,and L.Balicas,“A coherent threedimensional Fermi
surface in a hightransitiontemperature superconductor,”
Nature,vol.425,no.6960,pp.814–817,2003.
[621] K.Yang and S.L.Sondhi,“Response of a d
x
2
y
2
superconduc
tor to a Zeeman magnetic ﬁeld,” Physical Review B,vol.57,
no.14,pp.8566–8570,1998.
[622] A.Kanigel,M.R.Norman,M.Randeria,et al.,“Evolution of
the pseudogap from Fermi arcs to the nodal liquid,” Nature
Physics,vol.2,no.7,pp.447–451,2006.
[623] M.Hashimoto,T.Yoshida,K.Tanaka,et al.,“Distinct doping
dependences of the pseudogap and superconducting gap of
La
2
−
x
Sr
x
CuO
4
cuprate superconductors,” Physical Review B,
vol.75,no.14,Article ID140503,4 pages,2007.
[624] K.McElroy,“Death of a Fermi surface,” Nature Physics,vol.
2,no.7,pp.441–442,2006.
[625] Y.H.Liu,K.Takeyama,T.Kurosawa,N.Momono,M.Oda,
and M.Ido,“4a
×
4a electronic charge order enhanced in
the inhomogeneous pseudogap state of Bi
2
Sr
2
CaCu
2
O
8+δ
,”
Physical Review B,vol.75,no.21,Article ID212507,4 pages,
2007.
[626] A.Pushp,C.V.Parker,A.N.Pasupathy,et al.,“Extending
universal nodal excitations optimizes superconductivity in
Bi
2
Sr
2
CaCu
2
O
8+δ
,” Science,vol.324,no.5935,pp.1689–
1693,2009.
[627] D.Einzel,“Universal parameters in the response of uncon
ventional superconductors,” Journal of Low Temperature
Physics,vol.126,no.34,pp.867–880,2002.
[628] D.Einzel,“Analytic twoﬂuid description of unconventional
superconductivity,” Journal of Low Temperature Physics,vol.
131,no.12,pp.1–24,2003.
[629] B.L.Yu,J.C.F.Wang,A.D.Beyer,et al.,“Possible competing
orderinduced Fermi arcs in cuprate superconductors,” Solid
State Communications,vol.149,no.78,pp.261–265,2009.
[630] A.Furrer,“Admixture of an swave component to the d
wave gap symmetry in hightemperature superconductors,”
Journal of Superconductivity and Novel Magnetism,vol.21,
no.1,pp.1–5,2008.
40 Advances in Condensed Matter Physics
[631] T.Hasegawa,H.Ikuta,and K.Kitazawa,“Tunneling spec
troscopy of oxide superconductors,” in Physical Properties of
High Temperature Superconductors III,D.M.Ginsberg,Ed.,
p.525,World Scientiﬁc,Singapore,1992.
[632] M.Oda,N.Momono,and M.Ido,“What is the energy
scale in determining the T
c
of cuprate superconductivity?”
Superconductor Science and Technology,vol.13,no.11,pp.
R139–R146,2000.
[633] B.T.Geilikman,V.Z.Kresin,and N.F.Masharov,“Transition
temperature and energy gap for superconductors with strong
coupling,” Journal of Low Temperature Physics,vol.18,no.3
4,pp.241–271,1975.
[634] J.P.Carbotte and C.Jiang,“Strongcoupling eﬀects in dwave
superconductors,” Physical ReviewB,vol.48,no.6,pp.4231–
4234,1993.
[635] R.Combescot and X.Leyronas,“A simple theory for high
Δ/T
c
ratio in dwave superconductors,” European Physical
Journal B,vol.23,no.2,pp.159–163,2001.
[636] D.C.Mattis and M.Molina,“Ratio 2Δ
0
/kT
c
in superconduc
tivity,” Physical Review B,vol.44,no.22,pp.12565–12566,
1991.
[637] P.Udomsamuthirun,S.Ratanaburi,N.Saentalard,and S.
Yoksan,“The ratio 2Δ
0
/T
c
in BCS superconductivity,” Journal
of Superconductivity,vol.9,no.6,pp.603–604,1996.
[638] R.J.Radtke,K.Levin,H.B.Sch
¨
uttler,and M.R.Norman,
“Role of Van Hove singularities and momentumspace
structure in hightemperature superconductivity,” Physical
Review B,vol.48,no.21,pp.15957–15965,1993.
[639] D.Einzel and I.Sch
¨
urrer,“Weak coupling theory of clean
(d + s)wave superconductors,” Journal of Low Temperature
Physics,vol.117,no.12,pp.15–52,1999.
[640] H.Padamsee,J.E.Neighbor,and C.A.Shiﬀman,“Quasi
particle phenomenology for thermodynamics of strong
coupling superconductors,” Journal of Low Temperature
Physics,vol.12,no.34,pp.387–411,1973.
[641] I.Tifrea,I.Grosu,and M.Crisan,“Pseudogap inﬂuence on
the 2Δ
0
/T
c
ratio in dwave superconductors,” Physica C,vol.
371,no.2,pp.104–110,2002.
[642] N.Miyakawa,P.Guptasarma,J.F.Zasadzinski,D.G.Hinks,
and K.E.Gray,“Strong dependence of the superconducting
gap on oxygen doping from tunneling measurements on
Bi
2
Sr
2
CaCu
2
O
8
−
δ
,” Physical Review Letters,vol.80,no.1,pp.
157–160,1998.
[643] C.Pasquier,P.AubanSenzier,T.Vuletic,S.Tomic,M.
Heritier,and D.J
´
erome,“Coexistence of superconductivity
and spin density wave orderings in Bechgaard and Fabre
salts,” Journal de Physique,vol.12,no.9,pp.197–200,2002.
[644] D.J
´
erome,“The development of organic conductors:organic
superconductors,” Solid State Sciences,vol.10,no.12,pp.
1692–1700,2008.
[645] J.R.Jeﬀries,N.P.Butch,B.T.Yukich,and M.B.Maple,
“Competing ordered phases in URu
2
Si
2
:hydrostatic pressure
and rhenium substitution,” Physical Review Letters,vol.99,
no.21,Article ID217207,4 pages,2007.
[646] J.A.Janik,H.D.Zhou,Y.J.Jo,et al.,“Itinerant spin
excitations near the hidden order transition in URu
2
Si
2
,”
Journal of Physics:Condensed Matter,vol.21,no.19,Article
ID192202,4 pages,2009.
[647] S.Elgazzar,J.Rusz,M.Amft,P.M.Oppeneer,and J.A.
Mydosh,“Hidden order in URu
2
Si
2
originates from Fermi
surface gapping induced by dynamic symmetrybreaking,”
Nature Materials,vol.8,no.4,pp.337–341,2009.
[648] G.C.Psaltakis and E.W.Fenton,“Superconductivity and
spindensity waves:organic superconductors,” Journal of
Physics C,vol.16,no.20,pp.3913–3932,1983.
[649] E.W.Fenton,“Cooper pairing in the presence of inhomoge
neous magnetism,” Progress of Theoretical Physics,no.80,pp.
94–102,1984.
[650] A.M.Gabovich and A.I.Voitenko,“Nonstationary Joseph
son tunneling involving superconductors with spindensity
waves,” Physica C,vol.329,no.3,pp.198–230,2000.
[651] T.T.M.Palstra,A.A.Menovsky,J.V.D.Berg,et al.,
“Superconducting and magnetic transitions in the heavy
fermion systemURu
2
Si
2
,” Physical ReviewLetters,vol.55,no.
24,pp.2727–2730,1985.
[652] A.J.A.de Oliveira and P.C.de Camargo,“Spindensity
waves and chargedensity waves in Cr alloys,” in Handbook of
Advanced Magnetic Materials Bolume IV:Advanced Magnetic
Materials:Properties and Applications,Y.Liu,D.J.Sellmyer,
and D.Shindo,Eds.,p.159,Springer,Heidelberg,Germany,
2006.
[653] R.Jaramillo,Y.Feng,J.C.Lang,et al.,“Breakdown of the
BardeenCooperSchrieﬀer ground state at a quantumphase
transition,” Nature,vol.459,no.7245,pp.405–409,2009.
[654] H.Chen,Y.Ren,Y.Qiu,et al.,“Coexistence of the
spindensity wave and superconductivity in Ba
1
−
x
K
x
Fe
2
As
2
,”
Europhysics Letters,vol.85,no.1,Article ID 17006,5 pages,
2009.
[655] K.Terashima,Y.Sekiba,J.H.Bowen,et al.,“Fermi surface
nesting induced strong pairing in ironbased superconduc
tors,” Proceedings of the National Academy of Sciences of the
United States of America,vol.106,no.18,pp.7330–7333,
2009.
[656] P.M.R.Brydon and C.Timm,“Theory of the excitonic spin
densitywave state in iron pnictides,” Physical Review B,vol.
79,no.18,Article ID180504,4 pages,2009.
[657] S.A.J.Kimber,A.Kreyssig,Y.Z.Zhang,et al.,“Similarities
between structural distortions underpressure and chemical
doping in superconducting BaFe
2
As
2
,” Nature Materials,vol.
8,no.6,pp.471–475,2009.
[658] M.M.Korshunov and I.Eremin,“Theory of magnetic
excitations in ironbased layered superconductors,” Physical
Review B,vol.78,no.14,Article ID140509,4 pages,2008.
[659] I.Dimov,P.Goswami,X.Jia,and S.Chakravarty,“Compet
ing order,Fermi surface reconstruction,and quantumoscil
lations in underdoped hightemperature superconductors,”
Physical ReviewB,vol.78,no.13,Article ID134529,14 pages,
2008.
[660] B.Pradhan and G.C.Rout,“Antiferromagnetic and super
conducting gaps of some superconductors,” Physica C,vol.
468,no.1,pp.72–80,2008.
[661] A.D.Beyer,C.T.Chen,M.S.Grinolds,M.L.Teague,
and N.C.Yeh,“Competing orders and the doping and
momentum dependent quasiparticle excitations in cuprate
superconductors,” Physica C,vol.468,no.6,pp.471–479,
2008.
[662] A.B.Vorontsov,M.G.Vavilov,and A.V.Chubukov,
“Interplay between magnetismand superconductivity in the
iron pnictides,” Physical Review B,vol.79,no.6,Article ID
060508,4 pages,2009.
[663] A.N.Lavrov,L.P.Kozeeva,M.R.Trunin,and V.N.
Zverev,“Competitionand coexistence of antiferromagnetism
and superconductivity in RBa
2
Cu
3
O
6+x
(R
=
Lu,Y) single
crystals,” Physical ReviewB,vol.79,no.21,Article ID214523,
6 pages,2009.
[664] A.A.Gorbatsevich and Yu.V.Kopaev,“Magnetic state
with orbital toroidal ordering and superdiamagnetism,” in
Superconductivity,Superdiamagnetism,Superﬂuidity,V.L.
Ginzburg,Ed.,pp.175–241,Mir,Moscow,Russia,1987.
Submit your manuscripts at
http://www.hindawi.com
Hindawi Publishing Corporation
http://www.hindawi.com Volume 2013
High Energy Physics
Advances in
Hindawi Publishing Corporation
http://www.hindawi.com Volume 2013
Hindawi Publishing Corporation
http://www.hindawi.com Volume 2013
The Scientific
World Journal
Hindawi Publishing Corporation
http://www.hindawi.com Volume 2013
Fluids
Journal of
Hindawi Publishing Corporation
http://www.hindawi.com
ISRN
Astronomy and
Astrophysics
Volume 2013
Hindawi Publishing Corporation
http://www.hindawi.com Volume 2013
Advances in
Condensed Matter Physics
Optics
International Journal of
Hindawi Publishing Corporation
http://www.hindawi.com Volume 2013
Hindawi Publishing Corporation
http://www.hindawi.com Volume 2013
Advances in
Astronomy
ISRN
High Energy Physics
Hindawi Publishing Corporation
http://www.hindawi.com Volume 2013
Hindawi Publishing Corporation
http://www.hindawi.com Volume 2013
Statistical Mechanics
International Journal of
Hindawi Publishing Corporation
http://www.hindawi.com Volume 2013
Gravity
Journal of
ISRN
Condensed
Matter Physics
Hindawi Publishing Corporation
http://www.hindawi.com Volume 2013
Hindawi Publishing Corporation
http://www.hindawi.com Volume 2013
Physics
Research International
ISRN
Thermodynamics
Volume 2013
Hindawi Publishing Corporation
http://www.hindawi.com
Computational
Methods in Physics
Journal of
Hindawi Publishing Corporation
http://www.hindawi.com Volume 2013
Hindawi Publishing Corporation
http://www.hindawi.com Volume 2013
Soft Matter
Journal of
Hindawi Publishing Corporation
http://www.hindawi.com
Aerodynamics
Journal of
Volume 2013
Hindawi Publishing Corporation
http://www.hindawi.com Volume 2013
Photonics
Journal of
ISRN
Optics
Hindawi Publishing Corporation
http://www.hindawi.com Volume 2013
Hindawi Publishing Corporation
http://www.hindawi.com
Volume 2013
Thermodynamics
Journal of
Enter the password to open this PDF file:
File name:

File size:

Title:

Author:

Subject:

Keywords:

Creation Date:

Modification Date:

Creator:

PDF Producer:

PDF Version:

Page Count:

Preparing document for printing…
0%
Σχόλια 0
Συνδεθείτε για να κοινοποιήσετε σχόλιο